# Electronic Supplementary Material (ESI) for Chemical Science.
# This journal is © The Royal Society of Chemistry 2023

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_naco2fe2ws
_database_code_depnum_ccdc_archive 'CCDC 2068065'
_audit_update_record             
;
2023-09-29 deposited with the CCDC.	2023-10-30 downloaded from the CCDC.
;
_audit_creation_date             2023-09-01
_audit_creation_method           
;
Olex2 1.5
(compiled 2023.08.24 svn.re1ec1418 for OlexSys, GUI svn.r6817)
;
_shelx_SHELXL_version_number     2019/1
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Co4 Fe2 H92 Na14 O114 W18'
_chemical_formula_sum            'Co4 Fe2 H92 Na14 O114 W18'
_chemical_formula_weight         5927.06
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           56
_space_group_name_H-M_alt        'P c c n'
_space_group_name_Hall           '-P 2ab 2ac'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y+1/2, z'
'-x, y+1/2, -z+1/2'
'x+1/2, -y, -z+1/2'
'-x, -y, -z'
'x-1/2, y-1/2, -z'
'x, -y-1/2, z-1/2'
'-x-1/2, y, z-1/2'

_cell_length_a                   21.063(2)
_cell_length_b                   26.187(2)
_cell_length_c                   17.8488(19)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     9845.2(16)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    9833
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      28.22
_cell_measurement_theta_min      2.38
_shelx_estimated_absorpt_T_max   0.162
_shelx_estimated_absorpt_T_min   0.109
_exptl_absorpt_coefficient_mu    22.068
_exptl_absorpt_correction_T_max  0.7459
_exptl_absorpt_correction_T_min  0.4821
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            brown
_exptl_crystal_colour_primary    green
_exptl_crystal_density_diffrn    3.915
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             10232
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.13
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.1106
_diffrn_reflns_av_unetI/netI     0.0353
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            246675
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.371
_diffrn_reflns_theta_min         1.241
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_source_current           0.6
_diffrn_source_power             0.02979
_diffrn_source_voltage           49.65
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                7811
_reflns_number_total             10071
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL  (Sheldrick, 2008)'
_computing_structure_solution    ?
_refine_diff_density_max         4.554
_refine_diff_density_min         -2.978
_refine_diff_density_rms         0.459
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.199
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     688
_refine_ls_number_reflns         10071
_refine_ls_number_restraints     354
_refine_ls_R_factor_all          0.0819
_refine_ls_R_factor_gt           0.0545
_refine_ls_restrained_S_all      1.187
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0058P)²+1003.3821P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1078
_refine_ls_wR_factor_ref         0.1216
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(O25) \\sim Ueq: with sigma of 0.02 and sigma for terminal atoms of 0.04
Uanis(Na1) \\sim Ueq, Uanis(O12) \\sim Ueq: with sigma of 0.0051 and sigma for
terminal atoms of 0.0102
Uanis(O1) \\sim Ueq, Uanis(O33) \\sim Ueq, Uanis(O50) \\sim Ueq, Uanis(O2)
\\sim Ueq, Uanis(O42) \\sim Ueq, Uanis(O3) \\sim Ueq, Uanis(O58) \\sim Ueq,
Uanis(O4) \\sim Ueq, Uanis(O37) \\sim Ueq, Uanis(O5) \\sim Ueq, Uanis(O46)
\\sim Ueq, Uanis(O6) \\sim Ueq, Uanis(O54) \\sim Ueq, Uanis(O7) \\sim Ueq,
Uanis(O31) \\sim Ueq, Uanis(O8) \\sim Ueq, Uanis(O35) \\sim Ueq, Uanis(O9)
\\sim Ueq, Uanis(O39) \\sim Ueq, Uanis(O10) \\sim Ueq, Uanis(O44) \\sim Ueq,
Uanis(O11) \\sim Ueq, Uanis(O48) \\sim Ueq, Uanis(O12) \\sim Ueq, Uanis(O52)
\\sim Ueq, Uanis(O13) \\sim Ueq, Uanis(O56) \\sim Ueq, Uanis(O14) \\sim Ueq,
Uanis(O30) \\sim Ueq, Uanis(O15) \\sim Ueq, Uanis(O32) \\sim Ueq, Uanis(O16)
\\sim Ueq, Uanis(O34) \\sim Ueq, Uanis(O17) \\sim Ueq, Uanis(O36) \\sim Ueq,
Uanis(O18) \\sim Ueq, Uanis(O38) \\sim Ueq, Uanis(O19) \\sim Ueq, Uanis(O40)
\\sim Ueq, Uanis(O20) \\sim Ueq, Uanis(O43) \\sim Ueq, Uanis(O21) \\sim Ueq,
Uanis(O45) \\sim Ueq, Uanis(O22) \\sim Ueq, Uanis(O47) \\sim Ueq, Uanis(O23)
\\sim Ueq, Uanis(O49) \\sim Ueq, Uanis(O24) \\sim Ueq, Uanis(O51) \\sim Ueq,
Uanis(O25) \\sim Ueq, Uanis(O53) \\sim Ueq, Uanis(O26) \\sim Ueq, Uanis(O55)
\\sim Ueq, Uanis(O27) \\sim Ueq, Uanis(O57) \\sim Ueq, Uanis(O28) \\sim Ueq,
Uanis(O59) \\sim Ueq, Uanis(O29) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.02
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.35239(3) 0.36081(3) 0.70495(5) 0.02081(18) Uani 1 1 d . . . . .
W2 W 0.50638(4) 0.36950(3) 0.80952(5) 0.02270(18) Uani 1 1 d . . . . .
W3 W 0.39329(4) 0.48021(3) 0.81125(4) 0.02078(17) Uani 1 1 d . . . . .
W4 W 0.33056(3) 0.43019(3) 0.55013(4) 0.01530(16) Uani 1 1 d . . . . .
W5 W 0.43249(4) 0.33560(3) 0.54887(5) 0.02110(18) Uani 1 1 d . . . . .
W6 W 0.58528(4) 0.34340(3) 0.65164(5) 0.02272(18) Uani 1 1 d . . . . .
W7 W 0.61895(3) 0.44680(3) 0.74462(5) 0.02024(17) Uani 1 1 d . . . . .
W8 W 0.50793(4) 0.55543(3) 0.74444(5) 0.02066(17) Uani 1 1 d . . . . .
W9 W 0.37077(3) 0.54893(3) 0.65598(4) 0.01631(16) Uani 1 1 d . . . . .
Co1 Co 0.47805(11) 0.44575(9) 0.64252(13) 0.0136(5) Uani 1 1 d . . . . .
Co2 Co 0.61115(11) 0.45816(9) 0.54190(15) 0.0165(5) Uani 1 1 d . . . . .
Fe2 Fe 0.48286(11) 0.45115(9) 0.45623(15) 0.0132(5) Uani 1 1 d . . . . .
O1 O 0.2996(6) 0.3253(6) 0.7569(10) 0.036(4) Uani 1 1 d . U . . .
O2 O 0.4964(7) 0.3359(6) 0.8928(9) 0.034(4) Uani 1 1 d . U . . .
O3 O 0.3519(7) 0.4790(6) 0.8956(9) 0.033(4) Uani 1 1 d . U . . .
O4 O 0.2579(6) 0.4390(5) 0.5052(8) 0.022(3) Uani 1 1 d . U . . .
O5 O 0.4300(7) 0.2775(5) 0.4984(9) 0.031(3) Uani 1 1 d . U . . .
O6 O 0.6266(7) 0.2875(5) 0.6344(10) 0.039(4) Uani 1 1 d . U . . .
O7 O 0.6872(6) 0.4637(5) 0.7932(8) 0.028(3) Uani 1 1 d . U . . .
O8 O 0.5426(7) 0.6075(5) 0.7905(8) 0.028(3) Uani 1 1 d . U . . .
O9 O 0.3115(6) 0.5945(5) 0.6420(8) 0.024(3) Uani 1 1 d . U . . .
O10 O 0.2926(6) 0.3911(5) 0.6370(8) 0.021(3) Uani 1 1 d . U . . .
O11 O 0.3762(7) 0.3096(5) 0.6347(9) 0.029(3) Uani 1 1 d . U . . .
O12 O 0.4294(6) 0.3480(5) 0.7582(7) 0.016(3) Uani 1 1 d . U . . .
O13 O 0.3516(6) 0.4251(5) 0.7577(7) 0.017(3) Uani 1 1 d . U . . .
O14 O 0.5506(6) 0.3192(5) 0.7546(8) 0.026(3) Uani 1 1 d . U . . .
O15 O 0.5805(6) 0.4067(5) 0.8326(8) 0.026(3) Uani 1 1 d . U . . .
O16 O 0.4578(6) 0.4312(5) 0.8318(7) 0.022(3) Uani 1 1 d . U . . .
O17 O 0.4518(6) 0.5333(5) 0.8326(8) 0.024(3) Uani 1 1 d . U . . .
O18 O 0.3380(6) 0.5259(5) 0.7576(8) 0.022(3) Uani 1 1 d . U . . .
O19 O 0.3518(6) 0.3638(5) 0.5097(7) 0.019(3) Uani 1 1 d . U . . .
O20 O 0.5028(6) 0.3235(5) 0.6123(8) 0.024(3) Uani 1 1 d . U . . .
O21 O 0.6487(6) 0.3786(5) 0.7124(8) 0.022(3) Uani 1 1 d . U . . .
O22 O 0.5629(6) 0.5022(5) 0.7748(7) 0.023(3) Uani 1 1 d . U . . .
O23 O 0.4288(6) 0.5921(5) 0.7135(7) 0.018(3) Uani 1 1 d . U . . .
O24 O 0.3288(6) 0.4883(5) 0.6176(7) 0.019(3) Uani 1 1 d . U . . .
O25 O 0.4117(5) 0.4014(5) 0.6181(7) 0.017(3) Uani 1 1 d . U . . .
O26 O 0.5348(6) 0.4078(5) 0.7020(8) 0.021(3) Uani 1 1 d . U . . .
O27 O 0.4430(6) 0.4968(5) 0.7023(7) 0.020(3) Uani 1 1 d . U . . .
O28 O 0.5173(5) 0.4722(4) 0.5572(7) 0.014(3) Uani 1 1 d . U . . .
O29 O 0.3877(6) 0.4628(5) 0.4890(8) 0.020(3) Uani 1 1 d . U . . .
O30 O 0.4754(6) 0.3767(5) 0.4868(8) 0.020(3) Uani 1 1 d . U . . .
O31 O 0.6019(6) 0.3818(5) 0.5710(7) 0.019(3) Uani 1 1 d . U . . .
O32 O 0.6310(6) 0.4736(5) 0.6535(7) 0.016(3) Uani 1 1 d . U . . .
O33 O 0.5391(6) 0.5607(5) 0.6514(7) 0.020(3) Uani 1 1 d . U . . .
O34 O 0.4187(6) 0.5547(5) 0.5709(7) 0.019(3) Uani 1 1 d . U . . .
O35 O 0.7070(7) 0.4478(6) 0.5292(8) 0.031(3) Uani 1 1 d . U . . .
O36 O 0.2186(7) 0.4478(6) 0.8369(8) 0.034(4) Uani 1 1 d . U . . .
O37 O 0.3357(7) 0.4237(6) 1.1480(8) 0.033(4) Uani 1 1 d . U . . .
O38 O 0.6109(8) 0.7587(6) 0.6379(10) 0.045(4) Uani 1 1 d . U . . .
O39 O 0.5286(9) 0.7348(8) 0.7955(11) 0.059(5) Uani 1 1 d . U . . .
O40 O 0.5143(8) 0.1773(6) 0.8595(9) 0.039(4) Uani 1 1 d . U . . .
Na41 Na 0.2698(7) 0.5923(6) 0.8520(11) 0.097(5) Uani 1 1 d . . . . .
O42 O 0.6655(12) 0.3254(8) 0.4655(13) 0.076(7) Uani 1 1 d . U . . .
O43 O 0.3935(11) 0.6651(8) 0.8139(12) 0.068(6) Uani 1 1 d . U . . .
O44 O 0.6674(12) 0.6472(8) 0.6412(13) 0.075(7) Uani 1 1 d . U . . .
O45 O 0.6729(12) 0.7100(10) 0.7998(15) 0.087(7) Uani 1 1 d . U . . .
O46 O 0.4550(10) 0.5106(9) 1.0627(14) 0.081(7) Uani 1 1 d . U . . .
O47 O 0.3072(11) 0.5434(9) 1.0564(11) 0.068(6) Uani 1 1 d . U . . .
O48 O 0.5966(19) 0.6835(15) 0.938(2) 0.155(14) Uani 1 1 d . U . . .
O49 O 0.4463(17) 0.7226(11) 0.982(2) 0.126(11) Uani 1 1 d . U . . .
O50 O 0.4470(18) 0.5963(13) 0.953(2) 0.138(12) Uani 1 1 d . U . . .
O51 O 0.386(2) 0.3851(19) 0.973(3) 0.207(19) Uani 1 1 d . U . . .
O52 O 0.750000 0.250000 0.808(3) 0.136(17) Uani 1 2 d S TU P . .
O53 O 0.750000 0.750000 0.667(2) 0.103(12) Uani 1 2 d S TU P . .
O54 O 0.8120(18) 0.2763(14) 0.714(2) 0.144(13) Uani 1 1 d . U . . .
O55 O 0.767(2) 0.3053(19) 0.560(3) 0.22(2) Uani 1 1 d . U . . .
O56 O 0.2423(19) 0.2994(14) 0.536(2) 0.159(14) Uani 1 1 d . U . . .
O57 O 0.345(2) 0.6476(16) 0.933(2) 0.158(14) Uani 1 1 d . U . . .
O58 O 0.650(2) 0.360(2) 0.942(3) 0.21(2) Uani 1 1 d . U . . .
O59 O 0.690(2) 0.2629(18) 0.929(3) 0.20(2) Uani 1 1 d . U . . .
Na1 Na 0.2529(3) 0.4656(3) 0.7147(4) 0.0154(14) Uani 1 1 d . U . . .
Na2 Na 0.3527(5) 0.4648(6) 1.0263(7) 0.071(4) Uani 1 1 d . . . . .
Na3 Na 0.5854(6) 0.6846(4) 0.7132(7) 0.056(3) Uani 1 1 d . . . . .
Na4 Na 0.4976(13) 0.6680(9) 0.8817(16) 0.172(11) Uani 1 1 d . . . . .
Na5 Na 0.7342(15) 0.3326(11) 0.803(2) 0.25(2) Uani 1 1 d . . . . .
Na6 Na 0.6182(12) 0.2423(9) 0.820(2) 0.205(15) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.721(15) . ?
W1 O10 1.921(12) . ?
W1 O11 1.902(15) . ?
W1 O12 1.910(11) . ?
W1 O13 1.930(13) . ?
W1 O25 2.256(13) . ?
W1 Na1 3.458(7) . ?
W2 O2 1.741(15) . ?
W2 O12 1.946(12) . ?
W2 O14 1.889(15) . ?
W2 O15 1.886(14) . ?
W2 O16 1.954(13) . ?
W2 O26 2.246(13) . ?
W3 O3 1.740(15) . ?
W3 O13 1.940(12) . ?
W3 O16 1.904(13) . ?
W3 O17 1.896(13) . ?
W3 O18 1.925(13) . ?
W3 O27 2.251(13) . ?
W3 Na1 3.444(7) . ?
W4 O4 1.742(13) . ?
W4 O10 2.022(13) . ?
W4 O19 1.934(13) . ?
W4 O24 1.940(13) . ?
W4 O25 2.227(12) . ?
W4 O29 1.835(13) . ?
W4 Na1 3.488(7) . ?
W5 O5 1.768(14) . ?
W5 O11 2.053(15) . ?
W5 O19 1.981(12) . ?
W5 O20 1.892(13) . ?
W5 O25 2.166(12) . ?
W5 O30 1.790(14) . ?
W6 O6 1.730(15) . ?
W6 O14 2.077(14) . ?
W6 O20 1.944(13) . ?
W6 O21 1.953(13) . ?
W6 O26 2.188(13) . ?
W6 O31 1.791(13) . ?
W7 O7 1.737(13) . ?
W7 O15 2.055(14) . ?
W7 O21 1.977(13) . ?
W7 O22 1.946(14) . ?
W7 O26 2.182(13) . ?
W7 O32 1.790(12) . ?
W7 Na1 3.707(7) 4_566 ?
W8 O8 1.752(14) . ?
W8 O17 2.052(14) . ?
W8 O22 1.892(13) . ?
W8 O23 2.002(13) . ?
W8 O27 2.189(12) . ?
W8 O33 1.790(14) . ?
W9 O9 1.744(13) . ?
W9 O18 2.032(14) . ?
W9 O23 1.956(13) . ?
W9 O24 1.943(13) . ?
W9 O27 2.204(13) . ?
W9 O34 1.830(13) . ?
W9 Na1 3.468(7) . ?
Co1 O25 1.869(12) . ?
Co1 O26 1.882(13) . ?
Co1 O27 1.864(13) . ?
Co1 O28 1.867(12) . ?
Co2 O28 2.028(12) . ?
Co2 O29 2.142(13) 5_666 ?
Co2 O31 2.075(12) . ?
Co2 O32 2.075(13) . ?
Co2 O34 2.135(13) 5_666 ?
Co2 O35 2.050(14) . ?
Fe2 O28 2.019(13) . ?
Fe2 O28 2.022(12) 5_666 ?
Fe2 O29 2.110(12) . ?
Fe2 O30 2.030(13) . ?
Fe2 O33 2.000(13) 5_666 ?
Fe2 O34 2.135(13) 5_666 ?
O3 Na2 2.362(19) . ?
O4 Na2 2.456(18) 8_655 ?
O7 Na1 2.314(15) 4_566 ?
O8 Na3 2.605(19) . ?
O8 Na4 2.46(3) . ?
O9 Na5 2.69(3) 4_466 ?
O10 Na1 2.536(15) . ?
O13 Na1 2.457(13) . ?
O14 Na6 2.73(2) . ?
O18 Na41 2.81(2) . ?
O18 Na1 2.507(14) . ?
O21 Na41 2.90(2) 4_566 ?
O21 Na5 2.71(3) . ?
O24 Na1 2.432(14) . ?
O35 Na41 2.71(2) 4_566 ?
O36 Na1 2.344(16) . ?
O37 Na1 2.470(17) 8_656 ?
O37 Na2 2.450(19) . ?
O38 Na3 2.42(2) . ?
O39 Na3 2.31(2) . ?
O39 Na4 2.42(3) . ?
O40 Na3 2.475(19) 3_646 ?
O40 Na6 2.86(3) . ?
Na41 O57 2.59(4) . ?
Na41 Na1 4.139(18) . ?
Na41 Na5 3.48(4) 4_466 ?
O43 Na4 2.51(4) . ?
O44 Na3 2.37(3) . ?
O45 Na3 2.50(3) . ?
O46 Na2 2.55(3) . ?
O47 Na2 2.33(3) . ?
O48 Na4 2.35(5) . ?
O49 Na4 2.53(4) . ?
O50 Na4 2.51(4) . ?
O51 Na2 2.40(5) . ?
O52 Na5 2.19(3) . ?
O52 Na5 2.19(3) 2_655 ?
O52 Na6 2.79(3) 2_655 ?
O52 Na6 2.79(3) . ?
O54 Na5 2.71(6) . ?
O54 Na6 2.44(5) 2_655 ?
O59 Na6 2.51(5) . ?
Na3 Na4 3.56(3) . ?
Na5 Na6 3.69(4) 2_655 ?
Na5 Na6 3.41(4) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O10 98.0(6) . . ?
O1 W1 O11 98.3(7) . . ?
O1 W1 O12 100.7(6) . . ?
O1 W1 O13 101.7(7) . . ?
O1 W1 O25 169.2(6) . . ?
O1 W1 Na1 90.6(5) . . ?
O10 W1 O13 86.7(5) . . ?
O10 W1 O25 74.6(5) . . ?
O10 W1 Na1 46.1(4) . . ?
O11 W1 O10 92.7(6) . . ?
O11 W1 O12 88.8(6) . . ?
O11 W1 O13 159.8(6) . . ?
O11 W1 O25 74.5(5) . . ?
O11 W1 Na1 138.8(5) . . ?
O12 W1 O10 160.8(5) . . ?
O12 W1 O13 85.3(5) . . ?
O12 W1 O25 87.4(5) . . ?
O12 W1 Na1 129.0(4) . . ?
O13 W1 O25 85.9(5) . . ?
O13 W1 Na1 43.7(4) . . ?
O25 W1 Na1 89.8(3) . . ?
O2 W2 O12 98.9(6) . . ?
O2 W2 O14 98.6(7) . . ?
O2 W2 O15 100.1(6) . . ?
O2 W2 O16 100.5(6) . . ?
O2 W2 O26 171.0(6) . . ?
O12 W2 O16 84.2(5) . . ?
O12 W2 O26 87.1(5) . . ?
O14 W2 O12 88.0(6) . . ?
O14 W2 O16 160.3(6) . . ?
O14 W2 O26 74.8(5) . . ?
O15 W2 O12 160.4(6) . . ?
O15 W2 O14 93.8(6) . . ?
O15 W2 O16 87.8(6) . . ?
O15 W2 O26 74.6(5) . . ?
O16 W2 O26 86.7(5) . . ?
O3 W3 O13 100.7(6) . . ?
O3 W3 O16 100.3(6) . . ?
O3 W3 O17 99.5(7) . . ?
O3 W3 O18 98.0(6) . . ?
O3 W3 O27 169.8(6) . . ?
O3 W3 Na1 90.0(5) . . ?
O13 W3 O27 85.9(5) . . ?
O13 W3 Na1 44.1(4) . . ?
O16 W3 O13 85.3(5) . . ?
O16 W3 O18 161.1(6) . . ?
O16 W3 O27 88.0(5) . . ?
O16 W3 Na1 129.4(4) . . ?
O17 W3 O13 159.7(6) . . ?
O17 W3 O16 89.5(6) . . ?
O17 W3 O18 92.2(5) . . ?
O17 W3 O27 74.3(5) . . ?
O17 W3 Na1 137.7(4) . . ?
O18 W3 O13 86.7(5) . . ?
O18 W3 O27 74.4(5) . . ?
O18 W3 Na1 45.6(4) . . ?
O27 W3 Na1 89.3(3) . . ?
O4 W4 O10 94.2(6) . . ?
O4 W4 O19 98.6(6) . . ?
O4 W4 O24 99.5(6) . . ?
O4 W4 O25 165.7(5) . . ?
O4 W4 O29 103.9(6) . . ?
O4 W4 Na1 86.6(5) . . ?
O10 W4 O25 73.4(5) . . ?
O10 W4 Na1 45.9(4) . . ?
O19 W4 O10 85.5(5) . . ?
O19 W4 O24 160.1(5) . . ?
O19 W4 O25 73.9(5) . . ?
O19 W4 Na1 131.4(4) . . ?
O24 W4 O10 85.1(6) . . ?
O24 W4 O25 86.7(5) . . ?
O24 W4 Na1 42.3(4) . . ?
O25 W4 Na1 89.5(4) . . ?
O29 W4 O10 161.9(5) . . ?
O29 W4 O19 92.6(5) . . ?
O29 W4 O24 90.9(6) . . ?
O29 W4 O25 88.8(5) . . ?
O29 W4 Na1 133.2(4) . . ?
O5 W5 O11 94.5(6) . . ?
O5 W5 O19 96.6(6) . . ?
O5 W5 O20 100.7(6) . . ?
O5 W5 O25 165.7(6) . . ?
O5 W5 O30 102.5(6) . . ?
O11 W5 O25 73.8(5) . . ?
O19 W5 O11 83.8(5) . . ?
O19 W5 O25 74.4(5) . . ?
O20 W5 O11 87.1(6) . . ?
O20 W5 O19 161.0(6) . . ?
O20 W5 O25 87.1(5) . . ?
O30 W5 O11 162.3(6) . . ?
O30 W5 O19 89.5(5) . . ?
O30 W5 O20 94.3(6) . . ?
O30 W5 O25 88.7(5) . . ?
O6 W6 O14 94.3(7) . . ?
O6 W6 O20 99.2(7) . . ?
O6 W6 O21 98.9(7) . . ?
O6 W6 O26 165.9(7) . . ?
O6 W6 O31 103.5(7) . . ?
O14 W6 O26 72.6(5) . . ?
O20 W6 O14 85.6(6) . . ?
O20 W6 O21 159.7(6) . . ?
O20 W6 O26 85.4(5) . . ?
O21 W6 O14 83.9(6) . . ?
O21 W6 O26 74.9(5) . . ?
O31 W6 O14 162.1(5) . . ?
O31 W6 O20 92.0(6) . . ?
O31 W6 O21 92.7(6) . . ?
O31 W6 O26 89.6(5) . . ?
O7 W7 O15 94.3(6) . . ?
O7 W7 O21 96.4(6) . . ?
O7 W7 O22 100.0(6) . . ?
O7 W7 O26 165.0(6) . . ?
O7 W7 O32 103.7(6) . . ?
O7 W7 Na1 27.7(5) . 4_566 ?
O15 W7 O26 73.0(5) . . ?
O15 W7 Na1 117.8(4) . 4_566 ?
O21 W7 O15 83.5(6) . . ?
O21 W7 O26 74.6(5) . . ?
O21 W7 Na1 112.0(4) . 4_566 ?
O22 W7 O15 86.0(6) . . ?
O22 W7 O21 161.1(5) . . ?
O22 W7 O26 87.3(5) . . ?
O22 W7 Na1 86.9(4) . 4_566 ?
O26 W7 Na1 167.3(4) . 4_566 ?
O32 W7 O15 161.9(5) . . ?
O32 W7 O21 92.6(6) . . ?
O32 W7 O22 92.6(6) . . ?
O32 W7 O26 89.0(5) . . ?
O32 W7 Na1 80.1(4) . 4_566 ?
O8 W8 O17 95.8(6) . . ?
O8 W8 O22 100.6(6) . . ?
O8 W8 O23 95.9(6) . . ?
O8 W8 O27 165.4(6) . . ?
O8 W8 O33 102.9(6) . . ?
O17 W8 O27 72.9(5) . . ?
O22 W8 O17 85.7(6) . . ?
O22 W8 O23 160.5(5) . . ?
O22 W8 O27 88.0(5) . . ?
O23 W8 O17 82.4(5) . . ?
O23 W8 O27 73.8(5) . . ?
O33 W8 O17 160.7(5) . . ?
O33 W8 O22 95.6(6) . . ?
O33 W8 O23 90.7(5) . . ?
O33 W8 O27 87.9(5) . . ?
O9 W9 O18 95.0(6) . . ?
O9 W9 O23 97.3(6) . . ?
O9 W9 O24 100.5(6) . . ?
O9 W9 O27 166.1(6) . . ?
O9 W9 O34 102.7(6) . . ?
O9 W9 Na1 87.8(5) . . ?
O18 W9 O27 73.5(5) . . ?
O18 W9 Na1 45.6(4) . . ?
O23 W9 O18 85.2(5) . . ?
O23 W9 O27 74.3(5) . . ?
O23 W9 Na1 130.7(4) . . ?
O24 W9 O18 85.2(5) . . ?
O24 W9 O23 160.4(5) . . ?
O24 W9 O27 86.6(5) . . ?
O24 W9 Na1 42.8(4) . . ?
O27 W9 Na1 89.5(3) . . ?
O34 W9 O18 162.3(5) . . ?
O34 W9 O23 92.5(5) . . ?
O34 W9 O24 91.5(6) . . ?
O34 W9 O27 89.0(5) . . ?
O34 W9 Na1 134.3(4) . . ?
O25 Co1 O26 106.2(5) . . ?
O27 Co1 O25 106.4(5) . . ?
O27 Co1 O26 107.9(6) . . ?
O27 Co1 O28 112.1(6) . . ?
O28 Co1 O25 111.9(6) . . ?
O28 Co1 O26 112.0(6) . . ?
O28 Co2 O29 82.6(5) . 5_666 ?
O28 Co2 O31 92.8(5) . . ?
O28 Co2 O32 91.8(5) . . ?
O28 Co2 O34 82.4(5) . 5_666 ?
O28 Co2 O35 176.8(6) . . ?
O31 Co2 O29 175.2(5) . 5_666 ?
O31 Co2 O34 93.2(5) . 5_666 ?
O32 Co2 O29 93.3(5) . 5_666 ?
O32 Co2 O31 88.1(5) . . ?
O32 Co2 O34 174.2(5) . 5_666 ?
O34 Co2 O29 85.0(5) 5_666 5_666 ?
O35 Co2 O29 95.1(5) . 5_666 ?
O35 Co2 O31 89.5(6) . . ?
O35 Co2 O32 86.2(5) . . ?
O35 Co2 O34 99.5(5) . 5_666 ?
O28 Fe2 O28 80.5(5) . 5_666 ?
O28 Fe2 O29 83.5(5) 5_666 . ?
O28 Fe2 O29 93.1(5) . . ?
O28 Fe2 O30 92.9(5) . . ?
O28 Fe2 O30 170.1(5) 5_666 . ?
O28 Fe2 O34 92.7(5) 5_666 5_666 ?
O28 Fe2 O34 82.7(5) . 5_666 ?
O29 Fe2 O34 174.8(5) . 5_666 ?
O30 Fe2 O29 89.5(5) . . ?
O30 Fe2 O34 93.8(5) . 5_666 ?
O33 Fe2 O28 92.3(5) 5_666 5_666 ?
O33 Fe2 O28 169.2(5) 5_666 . ?
O33 Fe2 O29 94.0(5) 5_666 . ?
O33 Fe2 O30 95.3(5) 5_666 . ?
O33 Fe2 O34 89.7(5) 5_666 5_666 ?
W3 O3 Na2 148.6(9) . . ?
W4 O4 Na2 143.0(8) . 8_655 ?
W7 O7 Na1 131.9(8) . 4_566 ?
W8 O8 Na3 119.9(7) . . ?
W8 O8 Na4 130.6(10) . . ?
Na4 O8 Na3 89.1(8) . . ?
W9 O9 Na5 150.0(12) . 4_466 ?
W1 O10 W4 115.7(6) . . ?
W1 O10 Na1 100.9(6) . . ?
W4 O10 Na1 99.2(5) . . ?
W1 O11 W5 114.2(7) . . ?
W1 O12 W2 153.0(7) . . ?
W1 O13 W3 152.3(7) . . ?
W1 O13 Na1 103.4(5) . . ?
W3 O13 Na1 102.5(5) . . ?
W2 O14 W6 114.8(6) . . ?
W2 O14 Na6 123.4(10) . . ?
W6 O14 Na6 114.9(10) . . ?
W2 O15 W7 115.0(7) . . ?
W3 O16 W2 153.1(7) . . ?
W3 O17 W8 115.3(7) . . ?
W3 O18 W9 115.0(6) . . ?
W3 O18 Na41 113.2(7) . . ?
W3 O18 Na1 101.2(6) . . ?
W9 O18 Na41 121.6(7) . . ?
W9 O18 Na1 99.1(5) . . ?
Na1 O18 Na41 101.9(6) . . ?
W4 O19 W5 113.7(6) . . ?
W5 O20 W6 150.6(8) . . ?
W6 O21 W7 111.8(6) . . ?
W6 O21 Na41 120.4(7) . 4_566 ?
W6 O21 Na5 125.3(8) . . ?
W7 O21 Na41 99.0(6) . 4_566 ?
W7 O21 Na5 116.0(10) . . ?
Na5 O21 Na41 76.7(9) . 4_566 ?
W8 O22 W7 147.3(8) . . ?
W9 O23 W8 112.8(6) . . ?
W4 O24 W9 148.3(7) . . ?
W4 O24 Na1 105.3(6) . . ?
W9 O24 Na1 104.3(6) . . ?
W4 O25 W1 96.3(4) . . ?
W5 O25 W1 97.4(5) . . ?
W5 O25 W4 96.5(5) . . ?
Co1 O25 W1 123.2(6) . . ?
Co1 O25 W4 119.4(6) . . ?
Co1 O25 W5 118.4(6) . . ?
W6 O26 W2 97.8(5) . . ?
W7 O26 W2 97.3(5) . . ?
W7 O26 W6 96.2(5) . . ?
Co1 O26 W2 123.3(6) . . ?
Co1 O26 W6 118.9(7) . . ?
Co1 O26 W7 117.8(6) . . ?
W8 O27 W3 97.4(5) . . ?
W8 O27 W9 97.3(5) . . ?
W9 O27 W3 97.1(5) . . ?
Co1 O27 W3 122.7(6) . . ?
Co1 O27 W8 116.9(6) . . ?
Co1 O27 W9 120.2(6) . . ?
Co1 O28 Co2 118.3(6) . . ?
Co1 O28 Fe2 117.6(6) . 5_666 ?
Co1 O28 Fe2 117.9(6) . . ?
Fe2 O28 Co2 100.4(5) . . ?
Fe2 O28 Co2 99.5(5) 5_666 . ?
Fe2 O28 Fe2 99.5(5) . 5_666 ?
W4 O29 Co2 127.6(6) . 5_666 ?
W4 O29 Fe2 136.1(7) . . ?
Fe2 O29 Co2 93.3(5) . 5_666 ?
W5 O30 Fe2 141.5(7) . . ?
W6 O31 Co2 139.5(7) . . ?
W7 O32 Co2 140.2(7) . . ?
W8 O33 Fe2 142.6(7) . 5_666 ?
W9 O34 Co2 127.4(7) . 5_666 ?
W9 O34 Fe2 135.9(7) . 5_666 ?
Fe2 O34 Co2 93.5(5) 5_666 5_666 ?
Co2 O35 Na41 116.5(7) . 4_566 ?
Na2 O37 Na1 110.1(7) . 8_656 ?
Na3 O39 Na4 97.6(9) . . ?
Na3 O40 Na6 118.3(8) 3_646 . ?
O18 Na41 O21 111.9(7) . 4_466 ?
O18 Na41 Na1 36.4(3) . . ?
O18 Na41 Na5 89.0(7) . 4_466 ?
O21 Na41 Na1 84.3(5) 4_466 . ?
O21 Na41 Na5 49.2(6) 4_466 4_466 ?
O35 Na41 O18 118.6(7) 4_466 . ?
O35 Na41 O21 89.0(6) 4_466 4_466 ?
O35 Na41 Na1 96.4(5) 4_466 . ?
O35 Na41 Na5 137.4(8) 4_466 4_466 ?
O57 Na41 O18 111.6(11) . . ?
O57 Na41 O21 127.8(11) . 4_466 ?
O57 Na41 O35 94.4(11) . 4_466 ?
O57 Na41 Na1 146.3(11) . . ?
O57 Na41 Na5 105.2(12) . 4_466 ?
Na5 Na41 Na1 87.9(8) 4_466 . ?
Na5 O52 Na5 176(4) . 2_655 ?
Na5 O52 Na6 85.6(10) 2_655 2_655 ?
Na5 O52 Na6 94.7(9) . 2_655 ?
Na5 O52 Na6 85.6(10) . . ?
Na5 O52 Na6 94.7(9) 2_655 . ?
Na6 O52 Na6 171(3) . 2_655 ?
Na6 O54 Na5 91.2(14) 2_655 . ?
W1 Na1 W4 57.46(11) . . ?
W1 Na1 W7 164.2(2) . 4_466 ?
W1 Na1 W9 92.87(16) . . ?
W3 Na1 W1 65.96(12) . . ?
W3 Na1 W4 92.75(16) . . ?
W3 Na1 W7 119.1(2) . 4_466 ?
W3 Na1 W9 57.76(11) . . ?
W4 Na1 W7 133.34(19) . 4_466 ?
W9 Na1 W4 64.97(12) . . ?
W9 Na1 W7 102.41(18) . 4_466 ?
O7 Na1 W1 173.6(5) 4_466 . ?
O7 Na1 W3 117.0(4) 4_466 . ?
O7 Na1 W4 116.2(4) 4_466 . ?
O7 Na1 W7 20.4(4) 4_466 4_466 ?
O7 Na1 W9 84.6(4) 4_466 . ?
O7 Na1 O10 141.2(6) 4_466 . ?
O7 Na1 O13 150.4(6) 4_466 . ?
O7 Na1 O18 86.7(5) 4_466 . ?
O7 Na1 O24 98.9(5) 4_466 . ?
O7 Na1 O36 91.8(6) 4_466 . ?
O7 Na1 O37 82.8(6) 4_466 8_655 ?
O10 Na1 W1 33.1(3) . . ?
O10 Na1 W3 94.4(3) . . ?
O10 Na1 W4 34.9(3) . . ?
O10 Na1 W7 146.5(4) . 4_466 ?
O10 Na1 W9 94.7(3) . . ?
O13 Na1 W1 32.9(3) . . ?
O13 Na1 W3 33.4(3) . . ?
O13 Na1 W4 75.6(3) . . ?
O13 Na1 W7 148.2(4) . 4_466 ?
O13 Na1 W9 76.1(3) . . ?
O13 Na1 O10 63.9(4) . . ?
O13 Na1 O18 64.6(5) . . ?
O13 Na1 O37 126.7(5) . 8_655 ?
O18 Na1 W1 94.7(4) . . ?
O18 Na1 W3 33.3(3) . . ?
O18 Na1 W4 95.1(4) . . ?
O18 Na1 W7 95.4(4) . 4_466 ?
O18 Na1 W9 35.4(3) . . ?
O18 Na1 O10 114.5(5) . . ?
O24 Na1 W1 76.1(3) . . ?
O24 Na1 W3 76.4(3) . . ?
O24 Na1 W4 32.5(3) . . ?
O24 Na1 W7 119.3(4) . 4_466 ?
O24 Na1 W9 32.9(3) . . ?
O24 Na1 O10 65.2(4) . . ?
O24 Na1 O13 76.8(5) . . ?
O24 Na1 O18 66.0(5) . . ?
O24 Na1 O37 105.1(5) . 8_655 ?
O36 Na1 W1 94.4(4) . . ?
O36 Na1 W3 79.7(4) . . ?
O36 Na1 W4 151.1(5) . . ?
O36 Na1 W7 72.9(4) . 4_466 ?
O36 Na1 W9 128.8(5) . . ?
O36 Na1 O10 117.2(6) . . ?
O36 Na1 O13 83.4(5) . . ?
O36 Na1 O18 93.5(6) . . ?
O36 Na1 O24 156.1(6) . . ?
O36 Na1 O37 97.3(6) . 8_655 ?
O37 Na1 W1 94.6(4) 8_655 . ?
O37 Na1 W3 159.9(5) 8_655 . ?
O37 Na1 W4 80.2(4) 8_655 . ?
O37 Na1 W7 78.1(4) 8_655 4_466 ?
O37 Na1 W9 132.4(4) 8_655 . ?
O37 Na1 O10 69.1(5) 8_655 . ?
O37 Na1 O18 165.1(6) 8_655 . ?
O3 Na2 O4 83.4(6) . 8_656 ?
O3 Na2 O37 160.6(9) . . ?
O3 Na2 O46 100.6(8) . . ?
O3 Na2 O51 75.4(13) . . ?
O3 Na2 Na1 144.9(6) . 8_656 ?
O4 Na2 O46 166.0(9) 8_656 . ?
O4 Na2 Na1 66.8(4) 8_656 8_656 ?
O37 Na2 O4 82.9(6) . 8_656 ?
O37 Na2 O46 96.0(8) . . ?
O37 Na2 Na1 35.1(4) . 8_656 ?
O46 Na2 Na1 104.5(7) . 8_656 ?
O47 Na2 O3 94.9(8) . . ?
O47 Na2 O4 83.6(7) . 8_656 ?
O47 Na2 O37 97.1(7) . . ?
O47 Na2 O46 82.7(9) . . ?
O47 Na2 O51 168.2(15) . . ?
O47 Na2 Na1 65.0(6) . 8_656 ?
O51 Na2 O4 88.6(14) . 8_656 ?
O51 Na2 O37 90.6(13) . . ?
O51 Na2 O46 105.4(15) . . ?
O51 Na2 Na1 119.7(12) . 8_656 ?
O8 Na3 Na4 43.8(5) . . ?
O38 Na3 O8 172.6(7) . . ?
O38 Na3 O40 87.7(7) . 3_656 ?
O38 Na3 O45 88.1(8) . . ?
O38 Na3 Na4 133.0(7) . . ?
O39 Na3 O8 85.7(7) . . ?
O39 Na3 O38 90.6(7) . . ?
O39 Na3 O40 86.5(7) . 3_656 ?
O39 Na3 O44 163.9(9) . . ?
O39 Na3 O45 80.6(9) . . ?
O39 Na3 Na4 42.4(7) . . ?
O40 Na3 O8 85.7(6) 3_656 . ?
O40 Na3 O45 166.3(9) 3_656 . ?
O40 Na3 Na4 89.6(7) 3_656 . ?
O44 Na3 O8 102.7(8) . . ?
O44 Na3 O38 82.4(8) . . ?
O44 Na3 O40 107.6(8) . 3_656 ?
O44 Na3 O45 84.7(9) . . ?
O44 Na3 Na4 142.1(8) . . ?
O45 Na3 O8 97.7(8) . . ?
O45 Na3 Na4 83.8(8) . . ?
O8 Na4 O43 89.9(11) . . ?
O8 Na4 O49 174.3(14) . . ?
O8 Na4 O50 91.1(11) . . ?
O8 Na4 Na3 47.1(6) . . ?
O39 Na4 O8 86.6(10) . . ?
O39 Na4 O43 87.2(13) . . ?
O39 Na4 O49 99.0(12) . . ?
O39 Na4 O50 168.4(17) . . ?
O39 Na4 Na3 40.0(6) . . ?
O43 Na4 O49 89.1(12) . . ?
O43 Na4 O50 81.4(12) . . ?
O43 Na4 Na3 92.9(10) . . ?
O48 Na4 O8 93.1(13) . . ?
O48 Na4 O39 84.8(14) . . ?
O48 Na4 O43 171.2(17) . . ?
O48 Na4 O49 88.7(15) . . ?
O48 Na4 O50 106.8(18) . . ?
O48 Na4 Na3 83.2(12) . . ?
O49 Na4 Na3 138.6(12) . . ?
O50 Na4 O49 83.2(13) . . ?
O50 Na4 Na3 138.0(11) . . ?
O9 Na5 O21 107.6(10) 4_566 . ?
O9 Na5 Na41 75.9(8) 4_566 4_566 ?
O9 Na5 O54 103.4(14) 4_566 . ?
O9 Na5 Na6 80.7(8) 4_566 2_655 ?
O9 Na5 Na6 153.2(18) 4_566 . ?
O21 Na5 Na41 54.1(7) . 4_566 ?
O21 Na5 O54 107.0(16) . . ?
O21 Na5 Na6 83.4(8) . . ?
O21 Na5 Na6 147.8(17) . 2_655 ?
Na41 Na5 Na6 100.6(12) 4_566 2_655 ?
O52 Na5 O9 126.6(13) . 4_566 ?
O52 Na5 O21 124.3(16) . . ?
O52 Na5 Na41 124(2) . 4_566 ?
O52 Na5 O54 52.7(16) . . ?
O52 Na5 Na6 54.7(7) . . ?
O52 Na5 Na6 49.0(7) . 2_655 ?
O54 Na5 Na41 73.2(13) . 4_566 ?
O54 Na5 Na6 41.4(10) . 2_655 ?
O54 Na5 Na6 96.2(14) . . ?
Na6 Na5 Na41 128.0(11) . 4_566 ?
Na6 Na5 Na6 103.2(9) . 2_655 ?
O14 Na6 O40 98.3(8) . . ?
O14 Na6 O52 115.6(11) . . ?
O14 Na6 Na5 142.9(14) . 2_655 ?
O14 Na6 Na5 79.9(7) . . ?
O40 Na6 Na5 168.9(16) . . ?
O40 Na6 Na5 110.4(8) . 2_655 ?
O52 Na6 O40 145.4(9) . . ?
O52 Na6 Na5 36.3(5) . 2_655 ?
O52 Na6 Na5 39.8(7) . . ?
O54 Na6 O14 97.5(14) 2_655 . ?
O54 Na6 O40 122.2(15) 2_655 . ?
O54 Na6 O52 49.8(14) 2_655 . ?
O54 Na6 O59 106.2(17) 2_655 . ?
O54 Na6 Na5 68.9(13) 2_655 . ?
O54 Na6 Na5 47.4(11) 2_655 2_655 ?
O59 Na6 O14 119.0(15) . . ?
O59 Na6 O40 113.4(17) . . ?
O59 Na6 O52 56.6(16) . . ?
O59 Na6 Na5 70.9(14) . 2_655 ?
O59 Na6 Na5 59.3(14) . . ?
Na5 Na6 Na5 76.0(10) . 2_655 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 W2 O14 W6 -172.6(7) . . . . ?
O2 W2 O14 Na6 -23.3(10) . . . . ?
O2 W2 O15 W7 172.6(8) . . . . ?
O3 W3 O17 W8 -174.1(7) . . . . ?
O4 W4 O29 Co2 60.1(9) . . . 5_666 ?
O4 W4 O29 Fe2 -145.1(10) . . . . ?
O5 W5 O20 W6 125.4(16) . . . . ?
O5 W5 O30 Fe2 149.1(11) . . . . ?
O6 W6 O31 Co2 -149.8(11) . . . . ?
O7 W7 O32 Co2 145.7(10) . . . . ?
O8 W8 O22 W7 -124.8(14) . . . . ?
O8 W8 O33 Fe2 -146.0(11) . . . 5_666 ?
O9 W9 O34 Co2 -61.5(9) . . . 5_666 ?
O9 W9 O34 Fe2 144.7(10) . . . 5_666 ?
O10 W4 O4 Na2 46.6(13) . . . 8_655 ?
O10 W4 O29 Co2 -116.8(16) . . . 5_666 ?
O10 W4 O29 Fe2 38(2) . . . . ?
O11 W5 O20 W6 -140.6(17) . . . . ?
O11 W5 O30 Fe2 -15(3) . . . . ?
O12 W2 O14 W6 88.7(7) . . . . ?
O12 W2 O14 Na6 -122.0(9) . . . . ?
O12 W2 O15 W7 -21(2) . . . . ?
O13 W3 O3 Na2 114.8(17) . . . . ?
O13 W3 O17 W8 10.8(19) . . . . ?
O14 W2 O15 W7 73.1(7) . . . . ?
O14 W6 O31 Co2 28(2) . . . . ?
O15 W2 O14 W6 -71.8(7) . . . . ?
O15 W2 O14 Na6 77.5(10) . . . . ?
O15 W7 O7 Na1 -149.6(10) . . . 4_566 ?
O15 W7 O32 Co2 -28(2) . . . . ?
O16 W2 O14 W6 22(2) . . . . ?
O16 W2 O14 Na6 171.4(14) . . . . ?
O16 W2 O15 W7 -87.2(7) . . . . ?
O16 W3 O3 Na2 27.8(19) . . . . ?
O16 W3 O17 W8 85.6(7) . . . . ?
O17 W3 O3 Na2 -63.4(18) . . . . ?
O17 W8 O8 Na3 -153.8(8) . . . . ?
O17 W8 O8 Na4 -35.8(14) . . . . ?
O17 W8 O22 W7 140.2(14) . . . . ?
O17 W8 O33 Fe2 19(2) . . . 5_666 ?
O18 W3 O3 Na2 -157.1(17) . . . . ?
O18 W3 O17 W8 -75.6(7) . . . . ?
O18 W9 O9 Na5 37.8(19) . . . 4_466 ?
O18 W9 O34 Co2 118.6(16) . . . 5_666 ?
O18 W9 O34 Fe2 -35(2) . . . 5_666 ?
O19 W4 O4 Na2 132.7(12) . . . 8_655 ?
O19 W4 O29 Co2 159.7(8) . . . 5_666 ?
O19 W4 O29 Fe2 -45.5(10) . . . . ?
O19 W5 O20 W6 -79(2) . . . . ?
O19 W5 O30 Fe2 52.4(12) . . . . ?
O20 W5 O30 Fe2 -109.0(12) . . . . ?
O20 W6 O31 Co2 110.3(11) . . . . ?
O21 W6 O31 Co2 -50.0(11) . . . . ?
O21 W7 O7 Na1 126.5(10) . . . 4_566 ?
O21 W7 O32 Co2 48.4(11) . . . . ?
O22 W7 O7 Na1 -62.9(11) . . . 4_566 ?
O22 W7 O32 Co2 -113.4(11) . . . . ?
O22 W8 O8 Na3 119.5(8) . . . . ?
O22 W8 O8 Na4 -122.5(13) . . . . ?
O22 W8 O33 Fe2 111.8(12) . . . 5_666 ?
O23 W8 O8 Na3 -71.0(8) . . . . ?
O23 W8 O8 Na4 47.1(14) . . . . ?
O23 W8 O22 W7 88(2) . . . . ?
O23 W8 O33 Fe2 -49.7(12) . . . 5_666 ?
O23 W9 O9 Na5 -47.9(19) . . . 4_466 ?
O23 W9 O34 Co2 -159.5(8) . . . 5_666 ?
O23 W9 O34 Fe2 46.7(10) . . . 5_666 ?
O24 W4 O4 Na2 -39.0(13) . . . 8_655 ?
O24 W4 O29 Co2 -39.9(9) . . . 5_666 ?
O24 W4 O29 Fe2 114.9(10) . . . . ?
O24 W9 O9 Na5 123.9(19) . . . 4_466 ?
O24 W9 O34 Co2 39.6(8) . . . 5_666 ?
O24 W9 O34 Fe2 -114.2(10) . . . 5_666 ?
O25 W4 O4 Na2 76(3) . . . 8_655 ?
O25 W4 O29 Co2 -126.6(8) . . . 5_666 ?
O25 W4 O29 Fe2 28.3(10) . . . . ?
O25 W5 O20 W6 -66.7(16) . . . . ?
O25 W5 O30 Fe2 -22.0(11) . . . . ?
O25 Co1 O26 W2 -57.5(8) . . . . ?
O25 Co1 O26 W6 65.7(8) . . . . ?
O25 Co1 O26 W7 -178.8(7) . . . . ?
O25 Co1 O27 W3 58.7(8) . . . . ?
O25 Co1 O27 W8 178.5(6) . . . . ?
O25 Co1 O27 W9 -64.2(8) . . . . ?
O25 Co1 O28 Co2 -120.0(7) . . . . ?
O25 Co1 O28 Fe2 1.2(8) . . . . ?
O25 Co1 O28 Fe2 120.3(7) . . . 5_666 ?
O26 W2 O14 W6 1.2(6) . . . . ?
O26 W2 O14 Na6 150.5(10) . . . . ?
O26 W2 O15 W7 0.1(6) . . . . ?
O26 W6 O31 Co2 24.9(10) . . . . ?
O26 W7 O7 Na1 178.9(17) . . . 4_566 ?
O26 W7 O32 Co2 -26.1(10) . . . . ?
O26 Co1 O25 W1 57.1(8) . . . . ?
O26 Co1 O25 W4 178.2(7) . . . . ?
O26 Co1 O25 W5 -64.9(8) . . . . ?
O26 Co1 O27 W3 -54.9(8) . . . . ?
O26 Co1 O27 W8 64.9(8) . . . . ?
O26 Co1 O27 W9 -177.8(6) . . . . ?
O26 Co1 O28 Co2 -0.9(9) . . . . ?
O26 Co1 O28 Fe2 -120.6(7) . . . 5_666 ?
O26 Co1 O28 Fe2 120.2(7) . . . . ?
O27 W3 O3 Na2 -116(3) . . . . ?
O27 W3 O17 W8 -2.4(6) . . . . ?
O27 W8 O8 Na3 -116(2) . . . . ?
O27 W8 O8 Na4 2(3) . . . . ?
O27 W8 O22 W7 67.2(14) . . . . ?
O27 W8 O33 Fe2 24.0(12) . . . 5_666 ?
O27 W9 O9 Na5 4(4) . . . 4_466 ?
O27 W9 O34 Co2 126.2(8) . . . 5_666 ?
O27 W9 O34 Fe2 -27.6(10) . . . 5_666 ?
O27 Co1 O25 W1 -57.7(8) . . . . ?
O27 Co1 O25 W4 63.4(8) . . . . ?
O27 Co1 O25 W5 -179.7(6) . . . . ?
O27 Co1 O26 W2 56.2(8) . . . . ?
O27 Co1 O26 W6 179.5(6) . . . . ?
O27 Co1 O26 W7 -65.0(8) . . . . ?
O27 Co1 O28 Co2 120.6(7) . . . . ?
O27 Co1 O28 Fe2 0.9(8) . . . 5_666 ?
O27 Co1 O28 Fe2 -118.3(7) . . . . ?
O28 Co1 O25 W1 179.5(6) . . . . ?
O28 Co1 O25 W4 -59.3(8) . . . . ?
O28 Co1 O25 W5 57.6(8) . . . . ?
O28 Co1 O26 W2 -179.9(6) . . . . ?
O28 Co1 O26 W6 -56.6(8) . . . . ?
O28 Co1 O26 W7 58.9(8) . . . . ?
O28 Co1 O27 W3 -178.7(6) . . . . ?
O28 Co1 O27 W8 -58.9(8) . . . . ?
O28 Co1 O27 W9 58.4(8) . . . . ?
O29 W4 O4 Na2 -132.4(12) . . . 8_655 ?
O30 W5 O20 W6 21.8(17) . . . . ?
O32 W7 O7 Na1 32.3(11) . . . 4_566 ?
O33 W8 O8 Na3 21.1(9) . . . . ?
O33 W8 O8 Na4 139.2(13) . . . . ?
O33 W8 O22 W7 -20.5(15) . . . . ?
O34 W9 O9 Na5 -142.2(18) . . . 4_466 ?
Na1 W3 O3 Na2 157.9(17) . . . . ?
Na1 W3 O17 W8 -73.4(9) . . . . ?
Na1 W4 O4 Na2 1.4(12) . . . 8_655 ?
Na1 W4 O29 Co2 -38.4(11) . . . 5_666 ?
Na1 W4 O29 Fe2 116.4(9) . . . . ?
Na1 W7 O32 Co2 160.2(11) 4_566 . . . ?
Na1 W9 O9 Na5 82.8(19) . . . 4_466 ?
Na1 W9 O34 Co2 37.9(11) . . . 5_666 ?
Na1 W9 O34 Fe2 -115.9(8) . . . 5_666 ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Co2Fe2rod
_database_code_depnum_ccdc_archive 'CCDC 2068500'
_audit_update_record             
;
2023-09-29 deposited with the CCDC.	2023-10-30 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_PLAT430_Co2Fe2rod           
;
PROBLEM: Short Inter D...A Contact  O1       ..O42      .       2.28 Ang.  
RESPONSE: This is a "short contact" between a terminal oxo group of 
the lacunary Keggin structure and a water molecule bridgin two sodium
ions. There is neither a hydrogen bond, nor any other
;
_vrf_PLAT971_Co2Fe2rod           
;
PROBLEM: Check Calcd Resid. Dens.  1.61A   From O40             5.07 eA-3  
RESPONSE: Being a polyoxotungstate, the structure suffers from strong
absorption, which causes these absorption artefacts.
;
_vrf_PLAT972_Co2Fe2rod           
;
PROBLEM: Check Calcd Resid. Dens.  0.64A   From W6             -6.18 eA-3  
RESPONSE: Being a polyoxotungstate, the structure suffers from strong
absorption, which causes these absorption artefacts.
;
_vrf_PLAT973_Co2Fe2rod           
;
PROBLEM: Check Calcd Positive Resid. Density on        W8       3.27 eA-3  
RESPONSE: Being a polyoxotungstate, the structure suffers from strong
absorption, which causes these absorption artefacts.
;
_vrf_PLAT306_Co2Fe2rod           
;
PROBLEM: Isolated Oxygen Atom (H-atoms Missing ?) .......       O1AA Check 
RESPONSE: This belongs to a water molecule. Hydrogen atoms could not
be refined satisfactorily and where thus omitted.
;
# end Validation Reply Form
_audit_creation_date             2020-08-26
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.07.31 svn.rc2a77460 for OlexSys, GUI svn.r6145)
;
_shelx_SHELXL_version_number     2018/3
loop_
_audit_author_email
sorianoj@tcd.ie
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
College
Dublin
;
_audit_contact_author_email        schmittw@tcd.ie
_audit_contact_author_name         'Schmitt, W.'
_audit_contact_author_phone        +353-1-8963495
_publ_contact_author_id_orcid      0000-0002-0058-9404
_publ_requested_journal            ''
_publ_section_references
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Co4 Fe2 H75 Na14 O105.5 W18'
_chemical_formula_sum            'Co4 H75 Fe2 Na14 O105.5 W18'
_chemical_formula_weight         5741.93
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   12.2859(6)
_cell_length_b                   13.6630(6)
_cell_length_c                   14.9308(6)
_cell_angle_alpha                99.3780(10)
_cell_angle_beta                 104.1870(10)
_cell_angle_gamma                101.318(2)
_cell_volume                     2323.17(18)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    9915
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      33.20
_cell_measurement_theta_min      2.35
_shelx_estimated_absorpt_T_max   0.400
_shelx_estimated_absorpt_T_min   0.060
_exptl_absorpt_coefficient_mu    23.369
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_correction_T_min  0.2149
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1382 before and 0.0619 after correction. The Ratio of minimum to maximum transmission is 0.2879. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            brown
_exptl_crystal_colour_primary    brown
_exptl_crystal_density_diffrn    4.087
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       rod
_exptl_crystal_F_000             2541
_exptl_crystal_size_max          0.276
_exptl_crystal_size_mid          0.097
_exptl_crystal_size_min          0.048
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0627
_diffrn_reflns_av_unetI/netI     0.0736
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            54956
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         33.201
_diffrn_reflns_theta_min         1.559
_diffrn_ambient_temperature      100.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                12429
_reflns_number_total             17691
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'XT (Sheldrick, 2015)'
_refine_diff_density_max         5.598
_refine_diff_density_min         -5.698
_refine_diff_density_rms         0.568
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.057
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     692
_refine_ls_number_reflns         17691
_refine_ls_number_restraints     30
_refine_ls_R_factor_all          0.0950
_refine_ls_R_factor_gt           0.0570
_refine_ls_restrained_S_all      1.058
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0519P)²+88.9756P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1250
_refine_ls_wR_factor_ref         0.1462
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.5 times of:
  All O(H,H) groups
2. Uiso/Uaniso restraints and constraints
Uanis(O49B) \\sim Ueq, Uanis(O48B) \\sim Ueq, Uanis(O48A) \\sim Ueq: with sigma
of 0.01 and sigma for terminal atoms of 0.02
Uanis(Na5) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O38) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
3. Others
 Fixed Sof: Na4(0.5) Na5(0.5) Na7(0.5) O42(0.5) O44(0.5) O49B(0.75) O48A(0.5)
 O48B(0.5) Na6(0.75) Na9(0.75) O0AA(0.5)
4.a Rotating group:
 O35(H35A,H35B)
;
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.28792(4) 0.14776(4) 0.11134(3) 0.01628(10) Uani 1 1 d . . . . .
W2 W 0.14465(4) 0.36710(4) 0.11894(3) 0.01446(9) Uani 1 1 d . . . . .
W3 W 0.08257(4) 0.16901(4) 0.25870(3) 0.01553(9) Uani 1 1 d . . . . .
W4 W 0.49335(4) 0.14431(3) 0.30183(3) 0.01398(9) Uani 1 1 d . . . . .
W5 W 0.54394(4) 0.31659(4) 0.17983(3) 0.01455(9) Uani 1 1 d . . . . .
W6 W 0.40181(4) 0.53220(4) 0.19051(3) 0.01459(9) Uani 1 1 d . . . . .
W7 W 0.21827(4) 0.54954(4) 0.31508(3) 0.01424(9) Uani 1 1 d . . . . .
W8 W 0.15729(4) 0.35244(4) 0.45551(3) 0.01443(9) Uani 1 1 d . . . . .
W9 W 0.28911(4) 0.16572(3) 0.44804(3) 0.01397(9) Uani 1 1 d . . . . .
Co1 Co 0.36221(12) 0.34920(11) 0.32382(10) 0.0099(3) Uani 1 1 d . . . . .
Co2 Co 0.64623(13) 0.40298(11) 0.43601(11) 0.0116(3) Uani 1 1 d . . . . .
Fe1 Fe 0.47429(13) 0.41883(11) 0.55680(11) 0.0099(3) Uani 1 1 d . . . . .
Na1 Na 0.7272(7) 0.4410(8) 0.0313(7) 0.064(3) Uani 1 1 d . . . . .
Na2 Na 0.8222(9) 0.6554(9) 0.2053(6) 0.068(3) Uani 1 1 d . . . . .
Na3 Na 0.9566(9) 0.3818(8) 0.2580(8) 0.074(3) Uani 1 1 d . . . . .
Na4 Na 0.7688(13) -0.0454(11) 0.1476(10) 0.039(3) Uani 0.5 1 d . . P A .
Na5 Na 0.946(2) 0.1230(18) -0.0660(18) 0.088(7) Uani 0.5 1 d . U P A .
Na7 Na 0.6087(16) -0.1205(12) 0.2856(19) 0.077(7) Uani 0.5 1 d . . P A .
Na8 Na 0.7753(9) 0.0661(7) 0.4212(7) 0.064(2) Uani 1 1 d . . . . .
O10 O 0.8068(9) 0.2010(8) 0.3433(8) 0.029(2) Uani 1 1 d . . . . .
O1 O 0.2100(9) 0.0598(7) 0.0075(7) 0.026(2) Uani 1 1 d . . . . .
O1AA O 0.7955(11) 0.3224(11) -0.0691(11) 0.053(4) Uani 1 1 d . . . . .
O2 O 0.0282(8) 0.3369(7) 0.0151(6) 0.0218(19) Uani 1 1 d . . . . .
O3 O -0.0514(8) 0.0849(7) 0.1948(7) 0.026(2) Uani 1 1 d . . . . .
O4 O 0.2213(8) 0.2632(6) 0.0888(6) 0.0176(17) Uani 1 1 d . . . . .
O5 O 0.0807(7) 0.2783(6) 0.1923(6) 0.0167(16) Uani 1 1 d . . . . .
O6 O 0.1786(7) 0.1259(7) 0.1851(6) 0.0190(17) Uani 1 1 d . . . . .
O7 O 0.3707(8) 0.0667(7) 0.1771(7) 0.0199(18) Uani 1 1 d . . . . .
O8 O 0.4148(8) 0.2115(7) 0.0732(7) 0.0217(18) Uani 1 1 d . . . . .
O9 O 0.2506(8) 0.4625(7) 0.0837(7) 0.0218(18) Uani 1 1 d . . . . .
O2AA O 0.0995(7) 0.4738(6) 0.1906(6) 0.0177(17) Uani 1 1 d . . . . .
O11 O 0.0286(7) 0.2504(6) 0.3492(6) 0.0160(16) Uani 1 1 d . . . . .
O12 O 0.1378(8) 0.0914(6) 0.3467(7) 0.0207(18) Uani 1 1 d . . . . .
O13 O 0.4105(7) 0.2551(6) 0.2416(6) 0.0126(14) Uani 1 1 d . . . . .
O14 O 0.2926(7) 0.4338(6) 0.2502(6) 0.0125(14) Uani 1 1 d . . . . .
O15 O 0.2424(7) 0.2738(6) 0.3622(6) 0.0143(15) Uani 1 1 d . . . . .
O16 O 0.5818(7) 0.1927(7) 0.2184(6) 0.0173(16) Uani 1 1 d . . . . .
O17 O 0.6355(9) 0.3322(7) 0.1067(7) 0.0222(19) Uani 1 1 d . . . . .
O18 O 0.4567(7) 0.4164(6) 0.1499(6) 0.0162(16) Uani 1 1 d . . . . .
O19 O 0.4508(8) 0.6133(7) 0.1220(7) 0.0210(18) Uani 1 1 d . . . . .
O20 O 0.3021(7) 0.6158(6) 0.2364(6) 0.0158(16) Uani 1 1 d . . . . .
O21 O 0.1434(8) 0.6429(7) 0.3368(7) 0.0202(18) Uani 1 1 d . . . . .
O22 O 0.1468(8) 0.4463(6) 0.3703(6) 0.0162(16) Uani 1 1 d . . . . .
O23 O 0.0641(8) 0.3870(7) 0.5190(7) 0.0209(18) Uani 1 1 d . . . . .
O24 O 0.1863(8) 0.2355(6) 0.5076(6) 0.0166(16) Uani 1 1 d . . . . .
O25 O 0.2882(9) 0.0690(7) 0.5106(7) 0.025(2) Uani 1 1 d . . . . .
O26 O 0.3678(7) 0.1185(6) 0.3599(6) 0.0161(16) Uani 1 1 d . . . . .
O27 O 0.5505(9) 0.0391(7) 0.3202(7) 0.0231(19) Uani 1 1 d . . . . .
O28 O 0.5805(7) 0.2436(6) 0.4003(6) 0.0132(15) Uani 1 1 d . . . . .
O29 O 0.6292(7) 0.3954(6) 0.2928(6) 0.0164(16) Uani 1 1 d . . . . .
O30 O 0.5096(7) 0.5739(7) 0.3030(6) 0.0156(16) Uani 1 1 d . . . . .
O31 O 0.3487(7) 0.5894(6) 0.4173(6) 0.0154(16) Uani 1 1 d . . . . .
O32 O 0.2997(7) 0.4331(6) 0.5263(6) 0.0136(15) Uani 1 1 d . . . . .
O33 O 0.4153(7) 0.2650(6) 0.5212(6) 0.0155(16) Uani 1 1 d . . . . .
O34 O 0.4888(7) 0.4282(6) 0.4261(6) 0.0126(15) Uani 1 1 d . . . . .
O35 O 0.8098(8) 0.3784(7) 0.4520(7) 0.0226(19) Uani 1 1 d . . . . .
H35A H 0.859738 0.426654 0.497099 0.034 Uiso 1 1 d R U . . .
H35B H 0.830916 0.385623 0.401271 0.034 Uiso 1 1 d R U . . .
O36 O 0.8370(19) 0.7976(15) 0.1298(14) 0.089(6) Uani 1 1 d . . . . .
O37 O 0.7026(13) 0.7256(10) 0.2998(8) 0.051(4) Uani 1 1 d . . . . .
O38 O 0.992(2) 0.769(2) 0.317(2) 0.127(9) Uani 1 1 d . U . . .
O39 O 0.9148(10) 0.5540(9) 0.1194(8) 0.035(3) Uani 1 1 d . . . . .
O40 O 0.8460(15) 0.5054(14) 0.2910(11) 0.073(5) Uani 1 1 d . . . . .
O41 O 0.8305(14) 0.2611(15) 0.1428(14) 0.082(6) Uani 1 1 d . . . . .
O42 O 0.812(3) 0.107(2) 0.0625(19) 0.062(10) Uani 0.5 1 d . . P . .
O43 O 0.6244(18) 0.0465(13) 0.0885(13) 0.075(5) Uani 1 1 d . . . . .
O44 O 0.560(3) -0.174(3) 0.110(3) 0.074(10) Uani 0.5 1 d . . P A .
O45 O 0.6503(12) 0.5912(17) 0.0658(9) 0.079(6) Uani 1 1 d . . . . .
O47 O 0.188(2) -0.0922(12) 0.2580(13) 0.086(6) Uani 1 1 d . . . . .
O49B O 0.9764(18) 0.0984(19) 0.5025(19) 0.076(7) Uani 0.75 1 d . U P A 2
O50 O 0.2648(17) -0.1689(11) 0.4614(13) 0.076(5) Uani 1 1 d . . . . .
O51 O 0.786(3) -0.038(2) 0.290(2) 0.132(10) Uani 1 1 d . . . . .
O52 O 0.500000 0.000000 0.500000 0.076(8) Uani 1 2 d S . P . .
O48A O 0.457(2) -0.1947(17) 0.3310(18) 0.033(5) Uani 0.5 1 d . U P A 1
O48B O 0.408(4) -0.182(2) 0.294(2) 0.068(9) Uani 0.5 1 d . U P A 2
Na6 Na 0.5889(13) 0.2021(9) 0.5525(9) 0.067(3) Uani 0.75 1 d . . P A -1
Na9 Na 0.3635(10) -0.0649(9) 0.3753(8) 0.057(3) Uani 0.75 1 d . . P A -1
O46 O 0.342(2) -0.1280(12) 0.0763(14) 0.091(7) Uani 1 1 d . . . . .
O0AA O -0.001(5) 0.015(4) 0.026(2) 0.071(14) Uani 0.5 1 d . . P B -1


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.726(10) . ?
W1 O4 1.954(8) . ?
W1 O6 1.945(9) . ?
W1 O7 1.879(8) . ?
W1 O8 1.891(10) . ?
W1 O13 2.229(8) . ?
W2 O2 1.759(9) . ?
W2 O4 1.904(9) . ?
W2 O5 1.942(9) . ?
W2 O9 1.887(10) . ?
W2 O2AA 1.918(9) . ?
W2 O14 2.235(8) . ?
W3 O3 1.752(9) . ?
W3 O5 1.923(8) . ?
W3 O6 1.908(9) . ?
W3 O11 1.934(8) . ?
W3 O12 1.901(9) . ?
W3 O15 2.232(8) . ?
W4 O7 2.054(9) . ?
W4 O13 2.176(8) . ?
W4 O16 1.954(9) . ?
W4 O26 1.948(9) . ?
W4 O27 1.750(9) . ?
W4 O28 1.777(8) . ?
W5 O8 2.058(10) . ?
W5 O13 2.168(8) . ?
W5 O16 1.978(9) . ?
W5 O17 1.757(9) . ?
W5 O18 1.936(8) . ?
W5 O29 1.789(9) . ?
W6 O9 2.064(9) . ?
W6 O14 2.162(8) . ?
W6 O18 1.905(8) . ?
W6 O19 1.745(9) . ?
W6 O20 1.995(9) . ?
W6 O30 1.789(8) . ?
W7 O2AA 2.026(8) . ?
W7 O14 2.185(8) . ?
W7 O20 1.958(9) . ?
W7 O21 1.746(8) . ?
W7 O22 1.921(9) . ?
W7 O31 1.839(8) . ?
W8 O11 2.036(8) . ?
W8 O15 2.204(8) . ?
W8 O22 1.948(8) . ?
W8 O23 1.741(9) . ?
W8 O24 1.944(8) . ?
W8 O32 1.830(8) . ?
W9 O12 2.039(9) . ?
W9 O15 2.177(8) . ?
W9 O24 2.010(9) . ?
W9 O25 1.738(9) . ?
W9 O26 1.917(9) . ?
W9 O33 1.816(8) . ?
Co1 O13 1.911(8) . ?
Co1 O14 1.902(8) . ?
Co1 O15 1.889(9) . ?
Co1 O34 1.886(8) . ?
Co2 O28 2.097(8) . ?
Co2 O29 2.080(9) . ?
Co2 O31 2.161(8) 2_666 ?
Co2 O32 2.143(8) 2_666 ?
Co2 O34 2.005(8) . ?
Co2 O35 2.065(9) . ?
Fe1 O30 2.038(8) 2_666 ?
Fe1 O31 2.142(9) 2_666 ?
Fe1 O32 2.136(8) . ?
Fe1 O33 2.019(8) . ?
Fe1 O34 2.025(8) . ?
Fe1 O34 2.009(8) 2_666 ?
Na1 Na2 3.374(16) . ?
Na1 Na3 4.143(13) . ?
Na1 O1AA 2.44(2) . ?
Na1 O9 2.364(12) 2_665 ?
Na1 O17 2.292(12) . ?
Na1 O19 2.632(13) 2_665 ?
Na1 O39 2.425(15) . ?
Na1 O45 2.46(2) . ?
Na2 O36 2.40(2) . ?
Na2 O37 2.490(18) . ?
Na2 O38 2.39(3) . ?
Na2 O39 2.369(15) . ?
Na2 O40 2.61(2) . ?
Na2 O45 2.467(16) . ?
Na3 O5 2.532(15) 1_655 ?
Na3 O2AA 2.468(15) 1_655 ?
Na3 O11 2.586(13) 1_655 ?
Na3 O22 2.417(13) 1_655 ?
Na3 O40 2.43(2) . ?
Na3 O41 2.20(2) . ?
Na4 Na7 3.32(2) . ?
Na4 Na8 4.097(17) . ?
Na4 O1 2.375(17) 2_655 ?
Na4 O3 2.415(17) 1_655 ?
Na4 O36 2.45(2) 1_545 ?
Na4 O42 2.64(3) . ?
Na4 O43 2.44(2) . ?
Na4 O44 2.68(4) . ?
Na4 O51 2.07(3) . ?
Na5 O2 2.85(3) 1_655 ?
Na5 O42 2.82(5) . ?
Na5 O47 2.85(3) 2_655 ?
Na5 O0AA 2.25(7) 2_655 ?
Na7 Na8 3.01(2) . ?
Na7 O25 2.90(3) 2_656 ?
Na7 O27 2.442(19) . ?
Na7 O37 2.60(2) 1_545 ?
Na7 O44 2.49(4) . ?
Na7 O51 2.23(3) . ?
Na7 O48A 2.25(3) . ?
Na7 O48B 2.48(4) . ?
Na7 Na6 3.96(2) 2_656 ?
Na7 Na9 3.74(2) . ?
Na8 O10 2.354(14) . ?
Na8 O25 2.343(12) 2_656 ?
Na8 O27 2.723(15) . ?
Na8 O49B 2.39(2) . ?
Na8 O50 2.28(2) 2_656 ?
Na8 O51 2.28(3) . ?
Na8 Na6 3.902(18) . ?
O25 Na9 2.942(17) . ?
O26 Na9 2.544(13) . ?
O27 Na9 2.828(16) . ?
O28 Na6 2.415(15) . ?
O33 Na6 2.422(17) . ?
O35 H35A 0.8712 . ?
O35 H35B 0.8719 . ?
O47 Na9 2.34(2) . ?
O50 Na6 1.99(3) 2_656 ?
O50 Na9 2.41(2) . ?
O52 Na6 2.668(12) . ?
O52 Na6 2.668(12) 2_656 ?
O52 Na9 2.100(12) . ?
O48A Na9 2.38(3) . ?
Na6 Na9 4.155(18) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O4 99.3(4) . . ?
O1 W1 O6 99.4(4) . . ?
O1 W1 O7 100.7(4) . . ?
O1 W1 O8 99.9(5) . . ?
O1 W1 O13 172.0(4) . . ?
O4 W1 O13 86.2(3) . . ?
O6 W1 O4 83.4(4) . . ?
O6 W1 O13 87.1(3) . . ?
O7 W1 O4 159.3(4) . . ?
O7 W1 O6 88.3(4) . . ?
O7 W1 O8 94.0(4) . . ?
O7 W1 O13 74.5(3) . . ?
O8 W1 O4 87.6(4) . . ?
O8 W1 O6 159.9(4) . . ?
O8 W1 O13 74.3(4) . . ?
O2 W2 O4 99.9(4) . . ?
O2 W2 O5 100.6(4) . . ?
O2 W2 O9 98.8(4) . . ?
O2 W2 O2AA 98.5(4) . . ?
O2 W2 O14 170.0(4) . . ?
O4 W2 O5 85.0(4) . . ?
O4 W2 O2AA 160.8(4) . . ?
O4 W2 O14 88.1(3) . . ?
O5 W2 O14 86.0(3) . . ?
O9 W2 O4 90.5(4) . . ?
O9 W2 O5 160.6(4) . . ?
O9 W2 O2AA 92.0(4) . . ?
O9 W2 O14 75.0(3) . . ?
O2AA W2 O5 86.3(4) . . ?
O2AA W2 O14 74.3(3) . . ?
O3 W3 O5 100.5(4) . . ?
O3 W3 O6 100.4(4) . . ?
O3 W3 O11 97.6(4) . . ?
O3 W3 O12 99.9(4) . . ?
O3 W3 O15 170.0(4) . . ?
O5 W3 O11 86.4(4) . . ?
O5 W3 O15 85.6(3) . . ?
O6 W3 O5 85.5(4) . . ?
O6 W3 O11 161.3(4) . . ?
O6 W3 O15 87.9(3) . . ?
O11 W3 O15 74.7(3) . . ?
O12 W3 O5 159.6(4) . . ?
O12 W3 O6 89.3(4) . . ?
O12 W3 O11 92.4(4) . . ?
O12 W3 O15 74.5(3) . . ?
O7 W4 O13 72.5(3) . . ?
O16 W4 O7 83.9(4) . . ?
O16 W4 O13 74.2(3) . . ?
O26 W4 O7 85.5(4) . . ?
O26 W4 O13 86.5(3) . . ?
O26 W4 O16 160.1(4) . . ?
O27 W4 O7 94.7(4) . . ?
O27 W4 O13 165.5(4) . . ?
O27 W4 O16 98.3(4) . . ?
O27 W4 O26 99.3(4) . . ?
O27 W4 O28 103.4(4) . . ?
O28 W4 O7 161.9(3) . . ?
O28 W4 O13 89.5(3) . . ?
O28 W4 O16 92.4(4) . . ?
O28 W4 O26 92.5(4) . . ?
O8 W5 O13 72.6(3) . . ?
O16 W5 O8 83.2(4) . . ?
O16 W5 O13 74.0(3) . . ?
O17 W5 O8 92.4(4) . . ?
O17 W5 O13 163.5(4) . . ?
O17 W5 O16 97.8(4) . . ?
O17 W5 O18 100.0(4) . . ?
O17 W5 O29 104.2(4) . . ?
O18 W5 O8 86.7(4) . . ?
O18 W5 O13 86.5(3) . . ?
O18 W5 O16 159.9(4) . . ?
O29 W5 O8 163.1(4) . . ?
O29 W5 O13 90.5(3) . . ?
O29 W5 O16 91.5(4) . . ?
O29 W5 O18 93.3(4) . . ?
O9 W6 O14 73.3(3) . . ?
O18 W6 O9 86.3(4) . . ?
O18 W6 O14 87.3(3) . . ?
O18 W6 O20 160.6(4) . . ?
O19 W6 O9 92.0(4) . . ?
O19 W6 O14 163.2(4) . . ?
O19 W6 O18 100.1(4) . . ?
O19 W6 O20 96.3(4) . . ?
O19 W6 O30 104.3(4) . . ?
O20 W6 O9 82.7(4) . . ?
O20 W6 O14 74.2(3) . . ?
O30 W6 O9 163.2(4) . . ?
O30 W6 O14 90.0(3) . . ?
O30 W6 O18 94.8(4) . . ?
O30 W6 O20 91.2(4) . . ?
O2AA W7 O14 73.4(3) . . ?
O20 W7 O2AA 85.1(4) . . ?
O20 W7 O14 74.4(3) . . ?
O21 W7 O2AA 94.3(4) . . ?
O21 W7 O14 165.3(4) . . ?
O21 W7 O20 97.0(4) . . ?
O21 W7 O22 100.3(4) . . ?
O21 W7 O31 102.9(4) . . ?
O22 W7 O2AA 86.6(4) . . ?
O22 W7 O14 87.2(3) . . ?
O22 W7 O20 161.3(4) . . ?
O31 W7 O2AA 162.8(4) . . ?
O31 W7 O14 89.4(3) . . ?
O31 W7 O20 91.4(4) . . ?
O31 W7 O22 91.6(4) . . ?
O11 W8 O15 73.4(3) . . ?
O22 W8 O11 85.7(4) . . ?
O22 W8 O15 85.8(3) . . ?
O23 W8 O11 94.3(4) . . ?
O23 W8 O15 166.1(4) . . ?
O23 W8 O22 99.8(4) . . ?
O23 W8 O24 98.4(4) . . ?
O23 W8 O32 103.7(4) . . ?
O24 W8 O11 86.6(4) . . ?
O24 W8 O15 75.0(3) . . ?
O24 W8 O22 160.7(4) . . ?
O32 W8 O11 162.0(4) . . ?
O32 W8 O15 88.9(3) . . ?
O32 W8 O22 89.7(4) . . ?
O32 W8 O24 92.2(4) . . ?
O12 W9 O15 73.2(3) . . ?
O24 W9 O12 83.7(4) . . ?
O24 W9 O15 74.4(3) . . ?
O25 W9 O12 94.6(4) . . ?
O25 W9 O15 165.3(4) . . ?
O25 W9 O24 96.6(4) . . ?
O25 W9 O26 99.5(4) . . ?
O25 W9 O33 102.9(4) . . ?
O26 W9 O12 87.3(4) . . ?
O26 W9 O15 88.3(3) . . ?
O26 W9 O24 162.1(3) . . ?
O33 W9 O12 162.0(3) . . ?
O33 W9 O15 88.9(3) . . ?
O33 W9 O24 90.2(4) . . ?
O33 W9 O26 93.7(4) . . ?
O14 Co1 O13 107.5(3) . . ?
O15 Co1 O13 108.0(3) . . ?
O15 Co1 O14 105.7(4) . . ?
O34 Co1 O13 111.0(3) . . ?
O34 Co1 O14 111.1(3) . . ?
O34 Co1 O15 113.4(4) . . ?
O28 Co2 O31 92.2(3) . 2_666 ?
O28 Co2 O32 175.5(3) . 2_666 ?
O29 Co2 O28 87.2(3) . . ?
O29 Co2 O31 176.0(3) . 2_666 ?
O29 Co2 O32 93.9(3) . 2_666 ?
O32 Co2 O31 86.4(3) 2_666 2_666 ?
O34 Co2 O28 92.6(3) . . ?
O34 Co2 O29 93.3(3) . . ?
O34 Co2 O31 82.7(3) . 2_666 ?
O34 Co2 O32 83.0(3) . 2_666 ?
O34 Co2 O35 177.7(4) . . ?
O35 Co2 O28 88.0(3) . . ?
O35 Co2 O29 88.9(4) . . ?
O35 Co2 O31 95.1(4) . 2_666 ?
O35 Co2 O32 96.4(3) . 2_666 ?
O30 Fe1 O31 88.8(3) 2_666 2_666 ?
O30 Fe1 O32 93.4(3) 2_666 . ?
O32 Fe1 O31 176.8(3) . 2_666 ?
O33 Fe1 O30 93.4(3) . 2_666 ?
O33 Fe1 O31 92.5(3) . 2_666 ?
O33 Fe1 O32 89.6(3) . . ?
O33 Fe1 O34 93.5(3) . . ?
O34 Fe1 O30 93.1(3) 2_666 2_666 ?
O34 Fe1 O30 169.3(3) . 2_666 ?
O34 Fe1 O31 94.5(3) 2_666 2_666 ?
O34 Fe1 O31 82.8(3) . 2_666 ?
O34 Fe1 O32 94.7(3) . . ?
O34 Fe1 O32 83.1(3) 2_666 . ?
O34 Fe1 O33 170.5(3) 2_666 . ?
O34 Fe1 O34 81.1(4) 2_666 . ?
W6 Na1 Na3 162.1(3) 2_665 . ?
Na2 Na1 W6 116.7(3) . 2_665 ?
Na2 Na1 Na3 72.3(3) . . ?
O1AA Na1 W6 77.6(4) . 2_665 ?
O1AA Na1 Na2 142.0(5) . . ?
O1AA Na1 Na3 86.2(4) . . ?
O1AA Na1 O19 80.1(5) . 2_665 ?
O1AA Na1 O45 153.4(6) . . ?
O9 Na1 W6 36.4(3) 2_665 2_665 ?
O9 Na1 Na2 91.2(4) 2_665 . ?
O9 Na1 Na3 133.9(4) 2_665 . ?
O9 Na1 O1AA 81.4(5) 2_665 . ?
O9 Na1 O19 66.5(4) 2_665 2_665 ?
O9 Na1 O39 82.4(4) 2_665 . ?
O9 Na1 O45 72.7(5) 2_665 . ?
O17 Na1 W6 122.5(4) . 2_665 ?
O17 Na1 Na2 99.5(4) . . ?
O17 Na1 Na3 67.7(3) . . ?
O17 Na1 O1AA 100.8(5) . . ?
O17 Na1 O9 158.3(5) . 2_665 ?
O17 Na1 O19 92.4(4) . 2_665 ?
O17 Na1 O39 118.3(5) . . ?
O17 Na1 O45 101.0(6) . . ?
O19 Na1 W6 30.2(2) 2_665 2_665 ?
O19 Na1 Na2 130.7(4) 2_665 . ?
O19 Na1 Na3 153.3(4) 2_665 . ?
O39 Na1 W6 118.8(4) . 2_665 ?
O39 Na1 Na2 44.6(4) . . ?
O39 Na1 Na3 55.4(3) . . ?
O39 Na1 O1AA 97.4(5) . . ?
O39 Na1 O19 148.9(5) . 2_665 ?
O39 Na1 O45 85.5(6) . . ?
O45 Na1 W6 77.9(4) . 2_665 ?
O45 Na1 Na2 46.9(4) . . ?
O45 Na1 Na3 116.3(5) . . ?
O45 Na1 O19 84.0(4) . 2_665 ?
O36 Na2 Na1 106.9(6) . . ?
O36 Na2 O37 92.0(7) . . ?
O36 Na2 O40 169.7(8) . . ?
O36 Na2 O45 79.2(8) . . ?
O37 Na2 Na1 125.1(5) . . ?
O37 Na2 O40 95.3(6) . . ?
O38 Na2 Na1 143.5(7) . . ?
O38 Na2 O36 80.7(9) . . ?
O38 Na2 O37 89.3(8) . . ?
O38 Na2 O40 92.1(8) . . ?
O38 Na2 O45 159.9(10) . . ?
O39 Na2 Na1 45.9(4) . . ?
O39 Na2 O36 99.1(7) . . ?
O39 Na2 O37 167.5(7) . . ?
O39 Na2 O38 98.0(8) . . ?
O39 Na2 O40 74.4(5) . . ?
O39 Na2 O45 86.4(6) . . ?
O40 Na2 Na1 74.6(5) . . ?
O45 Na2 Na1 46.6(5) . . ?
O45 Na2 O37 90.2(6) . . ?
O45 Na2 O40 107.9(7) . . ?
W2 Na3 W3 64.5(2) 1_655 1_655 ?
W2 Na3 W8 92.5(2) 1_655 1_655 ?
W2 Na3 Na1 87.9(3) 1_655 . ?
W3 Na3 Na1 127.3(3) 1_655 . ?
W7 Na3 W2 57.93(18) 1_655 1_655 ?
W7 Na3 W3 92.2(2) 1_655 1_655 ?
W7 Na3 W8 66.07(17) 1_655 1_655 ?
W7 Na3 Na1 110.6(3) 1_655 . ?
W8 Na3 W3 56.60(15) 1_655 1_655 ?
W8 Na3 Na1 175.5(3) 1_655 . ?
O5 Na3 W2 33.2(2) 1_655 1_655 ?
O5 Na3 W3 31.5(2) 1_655 1_655 ?
O5 Na3 W7 76.2(3) 1_655 1_655 ?
O5 Na3 W8 74.6(3) 1_655 1_655 ?
O5 Na3 Na1 107.8(4) 1_655 . ?
O5 Na3 O11 62.1(4) 1_655 1_655 ?
O2AA Na3 W2 32.3(3) 1_655 1_655 ?
O2AA Na3 W3 92.8(4) 1_655 1_655 ?
O2AA Na3 W7 36.4(2) 1_655 1_655 ?
O2AA Na3 W8 96.3(3) 1_655 1_655 ?
O2AA Na3 Na1 81.7(3) 1_655 . ?
O2AA Na3 O5 63.7(4) 1_655 1_655 ?
O2AA Na3 O11 114.2(5) 1_655 1_655 ?
O11 Na3 W2 92.9(4) 1_655 1_655 ?
O11 Na3 W3 32.1(2) 1_655 1_655 ?
O11 Na3 W7 95.8(3) 1_655 1_655 ?
O11 Na3 W8 35.4(2) 1_655 1_655 ?
O11 Na3 Na1 149.0(4) 1_655 . ?
O22 Na3 W2 76.0(4) 1_655 1_655 ?
O22 Na3 W3 74.5(3) 1_655 1_655 ?
O22 Na3 W7 33.7(2) 1_655 1_655 ?
O22 Na3 W8 32.6(2) 1_655 1_655 ?
O22 Na3 Na1 143.7(4) 1_655 . ?
O22 Na3 O5 75.6(4) 1_655 1_655 ?
O22 Na3 O2AA 67.3(4) 1_655 1_655 ?
O22 Na3 O11 65.5(4) 1_655 1_655 ?
O22 Na3 O40 106.4(6) 1_655 . ?
O40 Na3 W2 132.5(5) . 1_655 ?
O40 Na3 W3 163.0(6) . 1_655 ?
O40 Na3 W7 97.4(5) . 1_655 ?
O40 Na3 W8 115.1(5) . 1_655 ?
O40 Na3 Na1 61.8(5) . . ?
O40 Na3 O5 165.4(6) . 1_655 ?
O40 Na3 O2AA 103.3(5) . 1_655 ?
O40 Na3 O11 132.2(6) . 1_655 ?
O41 Na3 W2 85.6(6) . 1_655 ?
O41 Na3 W3 76.4(5) . 1_655 ?
O41 Na3 W7 142.9(7) . 1_655 ?
O41 Na3 W8 128.0(6) . 1_655 ?
O41 Na3 Na1 56.5(6) . . ?
O41 Na3 O5 76.2(6) . 1_655 ?
O41 Na3 O2AA 107.9(8) . 1_655 ?
O41 Na3 O11 92.6(6) . 1_655 ?
O41 Na3 O22 150.2(7) . 1_655 ?
O41 Na3 O40 103.3(7) . . ?
Na7 Na4 Na8 46.3(4) . . ?
O1 Na4 Na7 147.8(8) 2_655 . ?
O1 Na4 Na8 163.4(6) 2_655 . ?
O1 Na4 O3 85.1(6) 2_655 1_655 ?
O1 Na4 O36 79.4(7) 2_655 1_545 ?
O1 Na4 O42 53.6(8) 2_655 . ?
O1 Na4 O43 83.1(6) 2_655 . ?
O1 Na4 O44 100.3(9) 2_655 . ?
O3 Na4 Na7 127.1(7) 1_655 . ?
O3 Na4 Na8 81.3(5) 1_655 . ?
O3 Na4 O36 101.7(8) 1_655 1_545 ?
O3 Na4 O42 55.3(7) 1_655 . ?
O3 Na4 O43 103.0(7) 1_655 . ?
O3 Na4 O44 172.6(10) 1_655 . ?
O36 Na4 Na7 93.7(7) 1_545 . ?
O36 Na4 Na8 112.5(6) 1_545 . ?
O36 Na4 O42 126.4(11) 1_545 . ?
O36 Na4 O44 84.4(11) 1_545 . ?
O42 Na4 Na7 139.6(10) . . ?
O42 Na4 Na8 110.3(8) . . ?
O42 Na4 O44 124.1(12) . . ?
O43 Na4 Na7 87.1(7) . . ?
O43 Na4 Na8 90.8(6) . . ?
O43 Na4 O36 148.2(9) . 1_545 ?
O43 Na4 O42 57.2(9) . . ?
O43 Na4 O44 72.8(11) . . ?
O44 Na4 Na7 47.5(9) . . ?
O44 Na4 Na8 92.6(8) . . ?
O51 Na4 Na7 41.2(10) . . ?
O51 Na4 Na8 20.5(8) . . ?
O51 Na4 O1 167.4(12) . 2_655 ?
O51 Na4 O3 87.5(10) . 1_655 ?
O51 Na4 O36 92.1(11) . 1_545 ?
O51 Na4 O42 128.4(12) . . ?
O51 Na4 O43 108.6(11) . . ?
O51 Na4 O44 88.1(12) . . ?
O42 Na5 O2 89.0(9) . 1_655 ?
O42 Na5 O47 114.1(11) . 2_655 ?
O47 Na5 O2 109.4(8) 2_655 1_655 ?
O0AA Na5 O2 133.2(13) 2_655 1_655 ?
O0AA Na5 O42 86.0(16) 2_655 . ?
O0AA Na5 O47 115.1(12) 2_655 2_655 ?
Na4 Na7 Na6 177.8(7) . 2_656 ?
Na4 Na7 Na9 141.5(7) . . ?
Na8 Na7 Na4 80.5(5) . . ?
Na8 Na7 Na6 99.2(7) . 2_656 ?
Na8 Na7 Na9 91.5(6) . . ?
O25 Na7 Na4 119.0(7) 2_656 . ?
O25 Na7 Na8 46.7(5) 2_656 . ?
O25 Na7 Na6 61.7(5) 2_656 2_656 ?
O25 Na7 Na9 77.7(5) 2_656 . ?
O27 Na7 Na4 96.3(6) . . ?
O27 Na7 Na8 58.9(5) . . ?
O27 Na7 O25 82.0(7) . 2_656 ?
O27 Na7 O37 163.6(13) . 1_545 ?
O27 Na7 O44 106.7(13) . . ?
O27 Na7 O48B 77.6(10) . . ?
O27 Na7 Na6 81.7(6) . 2_656 ?
O27 Na7 Na9 49.1(4) . . ?
O37 Na7 Na4 90.0(6) 1_545 . ?
O37 Na7 Na8 107.7(8) 1_545 . ?
O37 Na7 O25 81.8(7) 1_545 2_656 ?
O37 Na7 Na6 92.2(6) 1_545 2_656 ?
O37 Na7 Na9 128.0(7) 1_545 . ?
O44 Na7 Na4 52.6(9) . . ?
O44 Na7 Na8 130.5(10) . . ?
O44 Na7 O25 167.9(12) . 2_656 ?
O44 Na7 O37 89.1(11) . 1_545 ?
O44 Na7 Na6 127.0(10) . 2_656 ?
O44 Na7 Na9 114.4(11) . . ?
O51 Na7 Na4 37.6(8) . . ?
O51 Na7 Na8 48.9(8) . . ?
O51 Na7 O25 81.5(11) . 2_656 ?
O51 Na7 O27 92.5(9) . . ?
O51 Na7 O37 83.3(10) . 1_545 ?
O51 Na7 O44 89.6(13) . . ?
O51 Na7 O48A 161.7(17) . . ?
O51 Na7 O48B 169.9(14) . . ?
O51 Na7 Na6 143.2(13) . 2_656 ?
O51 Na7 Na9 138.2(10) . . ?
O48A Na7 Na4 160.6(13) . . ?
O48A Na7 Na8 116.8(11) . . ?
O48A Na7 O25 80.3(10) . 2_656 ?
O48A Na7 O27 86.5(8) . . ?
O48A Na7 O37 92.5(8) . 1_545 ?
O48A Na7 O44 108.2(13) . . ?
O48A Na7 Na6 18.8(7) . 2_656 ?
O48A Na7 Na9 37.4(6) . . ?
O48B Na7 Na4 144.7(13) . . ?
O48B Na7 Na8 122.3(11) . . ?
O48B Na7 O44 95.4(14) . . ?
Na9 Na7 Na6 36.3(3) . 2_656 ?
Na7 Na8 Na4 53.2(5) . . ?
Na7 Na8 Na6 105.5(5) . . ?
O10 Na8 Na4 69.6(4) . . ?
O10 Na8 Na7 110.4(6) . . ?
O10 Na8 O27 83.1(4) . . ?
O10 Na8 O49B 92.7(6) . . ?
O10 Na8 Na6 90.8(4) . . ?
O25 Na8 Na4 110.0(4) 2_656 . ?
O25 Na8 Na7 64.3(5) 2_656 . ?
O25 Na8 O10 170.6(6) 2_656 . ?
O25 Na8 O27 87.7(4) 2_656 . ?
O25 Na8 O49B 96.5(6) 2_656 . ?
O25 Na8 Na6 83.5(4) 2_656 . ?
O27 Na8 Na4 76.0(4) . . ?
O27 Na8 Na7 50.2(4) . . ?
O27 Na8 Na6 64.5(3) . . ?
O49B Na8 Na4 101.7(8) . . ?
O49B Na8 Na7 131.4(8) . . ?
O49B Na8 O27 175.7(6) . . ?
O50 Na8 Na4 155.4(6) 2_656 . ?
O50 Na8 Na7 125.6(7) 2_656 . ?
O50 Na8 O10 91.5(6) 2_656 . ?
O50 Na8 O25 86.1(5) 2_656 2_656 ?
O50 Na8 O27 86.5(6) 2_656 . ?
O50 Na8 O49B 94.5(9) 2_656 . ?
O50 Na8 O51 171.0(11) 2_656 . ?
O50 Na8 Na6 22.2(5) 2_656 . ?
O51 Na8 Na4 18.6(8) . . ?
O51 Na8 Na7 47.5(8) . . ?
O51 Na8 O10 86.7(8) . . ?
O51 Na8 O25 94.2(8) . 2_656 ?
O51 Na8 O27 84.5(9) . . ?
O51 Na8 O49B 94.4(11) . . ?
O51 Na8 Na6 148.9(9) . . ?
Na6 Na8 Na4 137.8(4) . . ?
W1 O1 Na4 130.3(6) . 2_655 ?
W2 O2 Na5 113.5(6) . 1_455 ?
W3 O3 Na4 164.2(7) . 1_455 ?
W2 O4 W1 154.3(5) . . ?
W2 O5 Na3 101.2(4) . 1_455 ?
W3 O5 W2 152.1(5) . . ?
W3 O5 Na3 104.9(5) . 1_455 ?
W3 O6 W1 153.9(5) . . ?
W1 O7 W4 115.2(4) . . ?
W1 O8 W5 114.7(5) . . ?
W2 O9 W6 113.9(5) . . ?
W2 O9 Na1 144.5(5) . 2_665 ?
W6 O9 Na1 100.7(4) . 2_665 ?
W2 O2AA W7 114.8(4) . . ?
W2 O2AA Na3 104.2(4) . 1_455 ?
W7 O2AA Na3 97.2(4) . 1_455 ?
W3 O11 W8 114.4(4) . . ?
W3 O11 Na3 102.7(4) . 1_455 ?
W8 O11 Na3 97.2(4) . 1_455 ?
W3 O12 W9 114.7(4) . . ?
W4 O13 W1 97.9(3) . . ?
W5 O13 W1 98.3(3) . . ?
W5 O13 W4 97.2(3) . . ?
Co1 O13 W1 122.7(4) . . ?
Co1 O13 W4 117.8(4) . . ?
Co1 O13 W5 118.0(4) . . ?
W6 O14 W2 97.8(3) . . ?
W6 O14 W7 97.8(3) . . ?
W7 O14 W2 97.5(3) . . ?
Co1 O14 W2 121.5(4) . . ?
Co1 O14 W6 117.4(4) . . ?
Co1 O14 W7 120.0(4) . . ?
W8 O15 W3 97.6(3) . . ?
W9 O15 W3 97.6(3) . . ?
W9 O15 W8 97.0(3) . . ?
Co1 O15 W3 122.4(4) . . ?
Co1 O15 W8 120.5(4) . . ?
Co1 O15 W9 116.5(4) . . ?
W4 O16 W5 112.0(4) . . ?
W5 O17 Na1 146.4(6) . . ?
W6 O18 W5 149.8(5) . . ?
W6 O19 Na1 100.6(4) . 2_665 ?
W7 O20 W6 111.9(4) . . ?
W7 O22 W8 151.0(5) . . ?
W7 O22 Na3 101.9(4) . 1_455 ?
W8 O22 Na3 105.5(4) . 1_455 ?
W8 O24 W9 112.1(4) . . ?
W9 O25 Na7 119.6(5) . 2_656 ?
W9 O25 Na8 162.1(7) . 2_656 ?
W9 O25 Na9 94.3(4) . . ?
Na7 O25 Na9 124.7(5) 2_656 . ?
Na8 O25 Na7 69.0(5) 2_656 2_656 ?
Na8 O25 Na9 92.2(4) 2_656 . ?
W4 O26 Na9 100.1(5) . . ?
W9 O26 W4 149.6(5) . . ?
W9 O26 Na9 103.6(5) . . ?
W4 O27 Na7 159.9(8) . . ?
W4 O27 Na8 120.8(5) . . ?
W4 O27 Na9 95.5(5) . . ?
Na7 O27 Na8 70.9(6) . . ?
Na7 O27 Na9 90.1(5) . . ?
Na8 O27 Na9 122.2(4) . . ?
W4 O28 Co2 140.2(4) . . ?
W4 O28 Na6 114.4(5) . . ?
Co2 O28 Na6 102.7(5) . . ?
W5 O29 Co2 139.6(5) . . ?
W6 O30 Fe1 140.3(5) . 2_666 ?
W7 O31 Co2 126.3(5) . 2_666 ?
W7 O31 Fe1 136.3(5) . 2_666 ?
Fe1 O31 Co2 92.6(3) 2_666 2_666 ?
W8 O32 Co2 128.0(4) . 2_666 ?
W8 O32 Fe1 136.2(4) . . ?
Fe1 O32 Co2 92.4(3) . 2_666 ?
W9 O33 Fe1 140.6(5) . . ?
W9 O33 Na6 112.0(5) . . ?
Fe1 O33 Na6 104.4(5) . . ?
Co1 O34 Co2 119.1(4) . . ?
Co1 O34 Fe1 115.6(4) . . ?
Co1 O34 Fe1 118.1(4) . 2_666 ?
Co2 O34 Fe1 101.1(4) . . ?
Co2 O34 Fe1 100.6(4) . 2_666 ?
Fe1 O34 Fe1 98.9(4) 2_666 . ?
Co2 O35 H35A 109.3 . . ?
Co2 O35 H35B 109.4 . . ?
H35A O35 H35B 104.5 . . ?
Na2 O36 Na4 133.2(11) . 1_565 ?
Na2 O37 Na7 129.3(7) . 1_565 ?
Na2 O39 Na1 89.5(5) . . ?
Na3 O40 Na2 125.3(7) . . ?
Na4 O42 Na5 127.7(13) . . ?
Na7 O44 Na4 79.8(11) . . ?
Na1 O45 Na2 86.5(6) . . ?
Na9 O47 Na5 152.3(12) . 2_655 ?
Na8 O50 Na9 109.6(7) 2_656 . ?
Na6 O50 Na8 132.3(10) 2_656 2_656 ?
Na6 O50 Na9 65.5(7) 2_656 . ?
Na4 O51 Na7 101.3(15) . . ?
Na4 O51 Na8 140.9(16) . . ?
Na7 O51 Na8 83.5(11) . . ?
Na6 O52 Na6 180.0 2_656 . ?
Na9 O52 Na6 120.8(4) . . ?
Na9 O52 Na6 59.2(4) . 2_656 ?
Na7 O48A Na9 107.5(10) . . ?
W4 Na6 Na8 63.4(3) . . ?
W4 Na6 Na9 52.8(2) . . ?
W9 Na6 W4 63.7(2) . . ?
W9 Na6 Co2 89.7(3) . . ?
W9 Na6 Na8 121.0(4) . . ?
W9 Na6 Na9 53.9(2) . . ?
Co2 Na6 W4 62.0(2) . . ?
Co2 Na6 Na8 87.4(3) . . ?
Co2 Na6 Na9 113.9(4) . . ?
Fe1 Na6 W4 89.6(3) . . ?
Fe1 Na6 W9 61.7(2) . . ?
Fe1 Na6 Co2 52.40(17) . . ?
Fe1 Na6 Na8 139.5(4) . . ?
Fe1 Na6 Na9 114.3(4) . . ?
Na8 Na6 Na9 74.1(3) . . ?
O28 Na6 W4 27.2(2) . . ?
O28 Na6 W9 77.0(4) . . ?
O28 Na6 Co2 35.4(3) . . ?
O28 Na6 Fe1 74.9(4) . . ?
O28 Na6 Na8 67.6(4) . . ?
O28 Na6 O33 78.3(5) . . ?
O28 Na6 O52 100.6(5) . . ?
O28 Na6 Na9 80.0(4) . . ?
O33 Na6 W4 77.8(4) . . ?
O33 Na6 W9 28.5(3) . . ?
O33 Na6 Co2 74.2(4) . . ?
O33 Na6 Fe1 33.8(3) . . ?
O33 Na6 Na8 141.1(5) . . ?
O33 Na6 O52 101.5(5) . . ?
O33 Na6 Na9 82.4(4) . . ?
O52 Na6 W4 74.2(3) . . ?
O52 Na6 W9 73.8(3) . . ?
O52 Na6 Co2 136.0(4) . . ?
O52 Na6 Fe1 135.2(5) . . ?
O52 Na6 Na8 68.6(3) . . ?
O52 Na6 Na9 25.7(2) . . ?
W4 Na9 W9 64.47(19) . . ?
W4 Na9 Na7 69.8(3) . . ?
W4 Na9 Na6 54.4(2) . . ?
W9 Na9 Na7 132.3(4) . . ?
W9 Na9 Na6 53.9(3) . . ?
Na7 Na9 Na6 88.7(4) . . ?
O25 Na9 W4 91.0(3) . . ?
O25 Na9 W9 29.4(2) . . ?
O25 Na9 Na7 147.2(6) . . ?
O25 Na9 Na6 58.7(4) . . ?
O26 Na9 W4 33.6(2) . . ?
O26 Na9 W9 31.9(3) . . ?
O26 Na9 Na7 103.4(5) . . ?
O26 Na9 O25 60.7(4) . . ?
O26 Na9 O27 63.1(4) . . ?
O26 Na9 Na6 52.4(3) . . ?
O27 Na9 W4 30.2(2) . . ?
O27 Na9 W9 91.8(3) . . ?
O27 Na9 Na7 40.8(3) . . ?
O27 Na9 O25 113.4(5) . . ?
O27 Na9 Na6 59.9(4) . . ?
O47 Na9 W4 92.9(5) . . ?
O47 Na9 W9 80.9(5) . . ?
O47 Na9 Na7 114.9(8) . . ?
O47 Na9 O25 91.7(7) . . ?
O47 Na9 O26 80.1(5) . . ?
O47 Na9 O27 111.0(7) . . ?
O47 Na9 O50 89.6(8) . . ?
O47 Na9 O48A 108.0(9) . . ?
O47 Na9 Na6 131.4(6) . . ?
O50 Na9 W4 162.2(7) . . ?
O50 Na9 W9 98.6(6) . . ?
O50 Na9 Na7 124.7(7) . . ?
O50 Na9 O25 71.3(6) . . ?
O50 Na9 O26 130.3(8) . . ?
O50 Na9 O27 158.3(7) . . ?
O50 Na9 Na6 111.9(6) . . ?
O52 Na9 W4 82.4(3) . . ?
O52 Na9 W9 80.2(4) . . ?
O52 Na9 Na7 81.1(5) . . ?
O52 Na9 O25 69.8(4) . . ?
O52 Na9 O26 85.8(4) . . ?
O52 Na9 O27 73.5(4) . . ?
O52 Na9 O47 160.7(8) . . ?
O52 Na9 O50 89.5(6) . . ?
O52 Na9 O48A 91.4(7) . . ?
O52 Na9 Na6 33.5(3) . . ?
O48A Na9 W4 104.4(8) . . ?
O48A Na9 W9 166.6(8) . . ?
O48A Na9 Na7 35.1(7) . . ?
O48A Na9 O25 154.1(8) . . ?
O48A Na9 O26 137.9(9) . . ?
O48A Na9 O27 75.8(7) . . ?
O48A Na9 O50 91.6(9) . . ?
O48A Na9 Na6 114.1(7) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O1 W1 O7 W4 172.9(5) . . . . ?
O1 W1 O8 W5 -174.4(5) . . . . ?
O2 W2 O9 W6 174.9(5) . . . . ?
O2 W2 O9 Na1 9.0(10) . . . 2_665 ?
O4 W1 O1 Na4 77.2(8) . . . 2_655 ?
O4 W1 O7 W4 -21.7(14) . . . . ?
O4 W1 O8 W5 86.5(5) . . . . ?
O4 W2 O2 Na5 34.4(8) . . . 1_455 ?
O4 W2 O9 W6 -85.0(5) . . . . ?
O4 W2 O9 Na1 109.1(9) . . . 2_665 ?
O5 W2 O2 Na5 -52.3(8) . . . 1_455 ?
O5 W2 O9 W6 -8.8(14) . . . . ?
O5 W2 O9 Na1 -174.7(9) . . . 2_665 ?
O5 W3 O3 Na4 -154(2) . . . 1_455 ?
O6 W1 O1 Na4 162.0(8) . . . 2_655 ?
O6 W1 O7 W4 -87.9(5) . . . . ?
O6 W1 O8 W5 23.1(13) . . . . ?
O6 W3 O3 Na4 119(2) . . . 1_455 ?
O7 W1 O1 Na4 -108.0(8) . . . 2_655 ?
O7 W1 O8 W5 -72.8(5) . . . . ?
O7 W4 O27 Na7 31.2(19) . . . . ?
O7 W4 O27 Na8 152.7(5) . . . . ?
O7 W4 O27 Na9 -74.4(4) . . . . ?
O7 W4 O28 Co2 -28.2(17) . . . . ?
O7 W4 O28 Na6 128.9(11) . . . . ?
O8 W1 O1 Na4 -12.0(8) . . . 2_655 ?
O8 W1 O7 W4 72.1(5) . . . . ?
O8 W5 O17 Na1 113.9(10) . . . . ?
O8 W5 O29 Co2 18.0(17) . . . . ?
O9 W2 O2 Na5 126.4(7) . . . 1_455 ?
O9 W6 O19 Na1 2.7(4) . . . 2_665 ?
O9 W6 O30 Fe1 -14.8(18) . . . 2_666 ?
O2AA W2 O2 Na5 -140.2(7) . . . 1_455 ?
O2AA W2 O9 W6 76.0(5) . . . . ?
O2AA W2 O9 Na1 -90.0(9) . . . 2_665 ?
O2AA W7 O31 Co2 -120.9(12) . . . 2_666 ?
O2AA W7 O31 Fe1 27.4(16) . . . 2_666 ?
O11 W3 O3 Na4 -66(2) . . . 1_455 ?
O11 W8 O32 Co2 115.1(11) . . . 2_666 ?
O11 W8 O32 Fe1 -37.8(15) . . . . ?
O12 W3 O3 Na4 28(3) . . . 1_455 ?
O12 W9 O25 Na7 -149.1(6) . . . 2_656 ?
O12 W9 O25 Na8 -34(2) . . . 2_656 ?
O12 W9 O25 Na9 76.6(4) . . . . ?
O12 W9 O33 Fe1 17.7(18) . . . . ?
O12 W9 O33 Na6 -138.6(12) . . . . ?
O13 W1 O7 W4 -0.4(4) . . . . ?
O13 W1 O8 W5 -0.2(4) . . . . ?
O13 W4 O27 Na7 5(3) . . . . ?
O13 W4 O27 Na8 126.1(14) . . . . ?
O13 W4 O27 Na9 -101.1(15) . . . . ?
O13 W4 O28 Co2 -24.7(7) . . . . ?
O13 W4 O28 Na6 132.4(5) . . . . ?
O13 W5 O17 Na1 138.7(11) . . . . ?
O13 W5 O29 Co2 20.9(7) . . . . ?
O13 Co1 O15 W3 -54.8(5) . . . . ?
O13 Co1 O15 W8 -178.5(4) . . . . ?
O13 Co1 O15 W9 64.7(5) . . . . ?
O13 Co1 O34 Co2 -1.1(5) . . . . ?
O13 Co1 O34 Fe1 -121.9(4) . . . . ?
O13 Co1 O34 Fe1 121.3(4) . . . 2_666 ?
O14 W2 O9 W6 2.9(4) . . . . ?
O14 W2 O9 Na1 -163.1(10) . . . 2_665 ?
O14 W6 O19 Na1 -25.8(15) . . . 2_665 ?
O14 W6 O30 Fe1 -20.7(7) . . . 2_666 ?
O14 W7 O31 Co2 -124.5(5) . . . 2_666 ?
O14 W7 O31 Fe1 23.8(6) . . . 2_666 ?
O14 Co1 O15 W3 60.0(5) . . . . ?
O14 Co1 O15 W8 -63.8(5) . . . . ?
O14 Co1 O15 W9 179.4(4) . . . . ?
O14 Co1 O34 Co2 -120.6(4) . . . . ?
O14 Co1 O34 Fe1 1.8(6) . . . 2_666 ?
O14 Co1 O34 Fe1 118.6(4) . . . . ?
O15 W3 O3 Na4 -27(4) . . . 1_455 ?
O15 W8 O32 Co2 125.8(5) . . . 2_666 ?
O15 W8 O32 Fe1 -27.1(6) . . . . ?
O15 W9 O25 Na7 -116.0(15) . . . 2_656 ?
O15 W9 O25 Na8 -1(3) . . . 2_656 ?
O15 W9 O25 Na9 109.6(15) . . . . ?
O15 W9 O33 Fe1 22.2(8) . . . . ?
O15 W9 O33 Na6 -134.1(5) . . . . ?
O15 Co1 O34 Co2 120.6(4) . . . . ?
O15 Co1 O34 Fe1 -117.0(4) . . . 2_666 ?
O15 Co1 O34 Fe1 -0.1(5) . . . . ?
O16 W4 O27 Na7 -53.3(19) . . . . ?
O16 W4 O27 Na8 68.2(6) . . . . ?
O16 W4 O27 Na9 -158.9(4) . . . . ?
O16 W4 O28 Co2 49.5(7) . . . . ?
O16 W4 O28 Na6 -153.4(6) . . . . ?
O16 W5 O17 Na1 -162.6(10) . . . . ?
O16 W5 O29 Co2 -53.1(7) . . . . ?
O17 W5 O29 Co2 -151.5(7) . . . . ?
O18 W5 O17 Na1 26.9(11) . . . . ?
O18 W5 O29 Co2 107.4(7) . . . . ?
O18 W6 O19 Na1 89.3(4) . . . 2_665 ?
O18 W6 O30 Fe1 -107.9(7) . . . 2_666 ?
O19 W6 O30 Fe1 150.4(7) . . . 2_666 ?
O20 W6 O19 Na1 -80.2(4) . . . 2_665 ?
O20 W6 O30 Fe1 53.5(7) . . . 2_666 ?
O20 W7 O31 Co2 161.2(5) . . . 2_666 ?
O20 W7 O31 Fe1 -50.5(6) . . . 2_666 ?
O21 W7 O31 Co2 63.6(6) . . . 2_666 ?
O21 W7 O31 Fe1 -148.1(6) . . . 2_666 ?
O22 W7 O31 Co2 -37.3(5) . . . 2_666 ?
O22 W7 O31 Fe1 111.0(6) . . . 2_666 ?
O22 W8 O32 Co2 40.1(6) . . . 2_666 ?
O22 W8 O32 Fe1 -112.8(6) . . . . ?
O23 W8 O32 Co2 -60.0(6) . . . 2_666 ?
O23 W8 O32 Fe1 147.1(6) . . . . ?
O24 W8 O32 Co2 -159.2(6) . . . 2_666 ?
O24 W8 O32 Fe1 47.9(6) . . . . ?
O24 W9 O25 Na7 -64.9(7) . . . 2_656 ?
O24 W9 O25 Na8 50(2) . . . 2_656 ?
O24 W9 O25 Na9 160.8(4) . . . . ?
O24 W9 O33 Fe1 -52.2(8) . . . . ?
O24 W9 O33 Na6 151.6(5) . . . . ?
O25 W9 O33 Fe1 -149.0(8) . . . . ?
O25 W9 O33 Na6 54.7(6) . . . . ?
O26 W4 O27 Na7 117.4(19) . . . . ?
O26 W4 O27 Na8 -121.1(5) . . . . ?
O26 W4 O27 Na9 11.7(5) . . . . ?
O26 W4 O28 Co2 -111.2(7) . . . . ?
O26 W4 O28 Na6 45.8(6) . . . . ?
O26 W9 O25 Na7 122.9(6) . . . 2_656 ?
O26 W9 O25 Na8 -122(2) . . . 2_656 ?
O26 W9 O25 Na9 -11.4(4) . . . . ?
O26 W9 O33 Fe1 110.4(8) . . . . ?
O26 W9 O33 Na6 -45.9(5) . . . . ?
O27 W4 O28 Co2 148.7(7) . . . . ?
O27 W4 O28 Na6 -54.3(6) . . . . ?
O28 W4 O27 Na7 -147.8(19) . . . . ?
O28 W4 O27 Na8 -26.3(6) . . . . ?
O28 W4 O27 Na9 106.6(4) . . . . ?
O29 W5 O17 Na1 -69.1(11) . . . . ?
O30 W6 O19 Na1 -173.1(4) . . . 2_665 ?
O33 W9 O25 Na7 26.8(7) . . . 2_656 ?
O33 W9 O25 Na8 142(2) . . . 2_656 ?
O33 W9 O25 Na9 -107.5(4) . . . . ?
O34 Co1 O15 W3 -178.2(4) . . . . ?
O34 Co1 O15 W8 58.1(5) . . . . ?
O34 Co1 O15 W9 -58.7(5) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Co3W
_database_code_depnum_ccdc_archive 'CCDC 2068502'
_audit_update_record             
;
2023-09-29 deposited with the CCDC.	2023-10-30 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_PLAT971_Co3W                
;
PROBLEM: Check Calcd Resid. Dens.  1.89A   From O35             3.61 eA-3  
RESPONSE: Every atom in the viscinity of this Q peak is fully occupied
not allowing for this to be part of a disorder. It is most likely
an abosprtion artefact.
;
_vrf_PLAT306_Co3W                
;
PROBLEM: Isolated Oxygen Atom (H-atoms Missing ?) .......       O7AA Check 
RESPONSE: As a hydrogen bond network could not be modelled to satisfaction,
hydrogen atoms were omitted in the refinement. These oxygen atoms belong
to water molecules.
;
_vrf_PLAT972_Co3W                
;
PROBLEM: Check Calcd Resid. Dens.  0.68A   From W2             -2.70 eA-3  
RESPONSE: The structure suffers from strong absorption due to being a 
polyoxotungstate. This is an absorption artefact.
;
# end Validation Reply Form
_audit_creation_date             2020-08-27
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.07.31 svn.rc2a77460 for OlexSys, GUI svn.r6145)
;
_shelx_SHELXL_version_number     2018/3
loop_
_audit_author_email
sorianoj@tcd.ie
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
College
Dublin
;
_audit_contact_author_email        schmittw@tcd.ie
_audit_contact_author_name         'Schmitt, W.'
_audit_contact_author_phone        +353-1-8963495
_publ_contact_author_id_orcid      0000-0002-0058-9404
_publ_requested_journal            ''
_publ_section_references
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Co5 Na12 H82 O109 W19'
_chemical_formula_sum            'Co5 Na12 H82 O109 W19'
_chemical_formula_weight         5807.49
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   13.063(11)
_cell_length_b                   17.764(15)
_cell_length_c                   21.118(18)
_cell_angle_alpha                90
_cell_angle_beta                 93.152(9)
_cell_angle_gamma                90
_cell_volume                     4893(7)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    4601
_cell_measurement_temperature    100.0
_cell_measurement_theta_max      29.490
_cell_measurement_theta_min      2.252
_shelx_estimated_absorpt_T_max   0.390
_shelx_estimated_absorpt_T_min   0.090
_exptl_absorpt_coefficient_mu    23.232
_exptl_absorpt_correction_T_max  0.7459
_exptl_absorpt_correction_T_min  0.3877
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1086 before and 0.0604 after correction.
The Ratio of minimum to maximum transmission is 0.5198.
The λ/2 correction factor is 0.00150.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'greenish blue'
_exptl_crystal_colour_modifier   greenish
_exptl_crystal_colour_primary    blue
_exptl_crystal_density_diffrn    3.942
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       needle
_exptl_crystal_F_000             5090
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.05
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.1017
_diffrn_reflns_av_unetI/netI     0.1182
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            46062
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.624
_diffrn_reflns_theta_min         1.499
_diffrn_ambient_temperature      100.0
_diffrn_detector                 'Bruker APEX2 area detector'
_diffrn_detector_area_resol_mean 7.9
_diffrn_detector_type            'CCD area detector'
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  'mirror optics'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'microfocus sealed X-ray tube'
_diffrn_source_current           45.0
_diffrn_source_power             2.25
_diffrn_source_type              'Incoatec I\ms'
_diffrn_source_voltage           50.0
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                8719
_reflns_number_total             13682
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.38A (Bruker, 2018)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.38A (Bruker, 2018)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'XT (Sheldrick, 2015)'
_refine_diff_density_max         3.866
_refine_diff_density_min         -3.246
_refine_diff_density_rms         0.510
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.020
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     676
_refine_ls_number_reflns         13682
_refine_ls_number_restraints     102
_refine_ls_R_factor_all          0.1152
_refine_ls_R_factor_gt           0.0570
_refine_ls_restrained_S_all      1.019
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0398P)²+25.9747P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1003
_refine_ls_wR_factor_ref         0.1167
_refine_special_details          ?
_olex2_refinement_description    
;
1. Shared sites
{Co3, W10}
2. Uiso/Uaniso restraints and constraints
Uanis(O15) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(Na6) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O1) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O13) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O01J) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O27) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O55) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O30) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O46) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O14) \\sim Ueq: with sigma of 0.0025 and sigma for terminal atoms of 0.005
Uanis(O53) \\sim Ueq, Uanis(O50) \\sim Ueq, Uanis(O45) \\sim Ueq, Uanis(O43)
\\sim Ueq, Uanis(O42) \\sim Ueq: with sigma of 0.01 and sigma for terminal
atoms of 0.02
Uanis(O7) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O18) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(Co3) = Uanis(W10)
3. Others
 Fixed Sof: W10(0.5) Co3(0.5) Na54(0.5) O44(0.75) Na6(0.5) O43(0.75)
 O55(0.66667) O53(0.33333)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W2 W 0.27720(5) 0.24361(4) 0.67329(3) 0.01543(14) Uani 1 1 d . . . . .
W6 W 0.27630(5) 0.05669(4) 0.68831(3) 0.01382(13) Uani 1 1 d . . . . .
W9 W 0.57774(5) 0.22188(4) 0.46014(3) 0.01341(13) Uani 1 1 d . . . . .
W3 W 0.56460(5) 0.24199(4) 0.69879(3) 0.01492(14) Uani 1 1 d . . . . .
W8 W 0.70037(4) 0.13410(4) 0.60849(3) 0.01245(13) Uani 1 1 d . . . . .
W7 W 0.56178(5) 0.05884(4) 0.71542(3) 0.01493(13) Uani 1 1 d . . . . .
W4 W 0.32850(5) 0.22437(4) 0.44356(3) 0.01450(13) Uani 1 1 d . . . . .
W5 W 0.16724(5) 0.13302(4) 0.56293(3) 0.01494(13) Uani 1 1 d . . . . .
W1 W 0.44360(5) 0.32872(4) 0.55311(3) 0.01592(14) Uani 1 1 d . . . . .
W10 W 0.55047(7) -0.03811(5) 0.56206(4) 0.01055(18) Uani 0.5 1 d . . P A 6
Co2 Co 0.30963(15) -0.03631(12) 0.53892(9) 0.0136(4) Uani 1 1 d . . . . .
Co1 Co 0.43538(15) 0.12873(12) 0.57559(8) 0.0116(4) Uani 1 1 d . . . . .
Co3 Co 0.55047(7) -0.03811(5) 0.56206(4) 0.01055(18) Uani 0.5 1 d . . P A 5
O29 O 0.3007(7) -0.0193(6) 0.6355(4) 0.014(2) Uani 1 1 d . . . . .
O26 O 0.6762(8) 0.2486(6) 0.4128(5) 0.021(3) Uani 1 1 d . . . . .
O32 O 0.5665(7) 0.1166(6) 0.4455(4) 0.012(2) Uani 1 1 d . . . . .
O17 O 0.1437(7) 0.0794(6) 0.6399(4) 0.016(2) Uani 1 1 d . . . . .
O5 O 0.5386(8) 0.3028(6) 0.6217(5) 0.020(2) Uani 1 1 d . . . . .
O1 O 0.4420(9) 0.4260(6) 0.5613(5) 0.021(2) Uani 1 1 d . U . . .
O52 O 0.3462(8) 0.3260(6) 0.4785(5) 0.019(2) Uani 1 1 d . . . . .
O6 O 0.5575(8) 0.3214(6) 0.4965(5) 0.018(2) Uani 1 1 d . . . . .
O24 O 0.5962(8) 0.0035(7) 0.7801(5) 0.024(3) Uani 1 1 d . . . . .
O15 O 0.4622(7) 0.2390(6) 0.4033(4) 0.013(2) Uani 1 1 d . U . . .
O34 O 0.1744(8) -0.1061(7) 0.5339(5) 0.025(3) Uani 1 1 d . . . . .
O25 O 0.8327(8) 0.1363(6) 0.6011(4) 0.018(2) Uani 1 1 d . . . . .
O14 O 0.5475(7) 0.1401(6) 0.6385(4) 0.010(2) Uani 1 1 d . U . . .
O23 O 0.2254(8) 0.0123(6) 0.7531(5) 0.021(2) Uani 1 1 d . . . . .
O2 O 0.2392(8) 0.3199(6) 0.7189(5) 0.020(2) Uani 1 1 d . . . . .
O19 O 0.6998(8) 0.0713(6) 0.6853(5) 0.019(2) Uani 1 1 d . . . . .
O27 O 0.4356(7) 0.0321(6) 0.5342(4) 0.013(2) Uani 1 1 d . U . . .
O30 O 0.5416(7) -0.0161(6) 0.6508(4) 0.013(2) Uani 1 1 d . U . . .
O13 O 0.3096(7) 0.1385(6) 0.6173(4) 0.011(2) Uani 1 1 d . U . . .
O01J O 0.4228(8) 0.2388(6) 0.7033(4) 0.016(2) Uani 1 1 d . U . . .
O21 O 0.2487(8) 0.2478(7) 0.3774(5) 0.022(3) Uani 1 1 d . . . . .
O12 O 0.4471(7) 0.2127(6) 0.5183(4) 0.011(2) Uani 1 1 d . . . . .
O18 O 0.4165(8) 0.0662(6) 0.7198(5) 0.020(2) Uani 1 1 d . U . . .
O28 O 0.2048(8) 0.0503(7) 0.5211(5) 0.023(3) Uani 1 1 d . . . . .
O4 O 0.3385(8) 0.2993(7) 0.6041(5) 0.023(3) Uani 1 1 d . . . . .
O16 O 0.2307(8) 0.1994(6) 0.5031(4) 0.018(2) Uani 1 1 d . . . . .
O20 O 0.6579(8) 0.1949(6) 0.5374(5) 0.019(2) Uani 1 1 d . . . . .
O8 O 0.1601(8) 0.2310(6) 0.6199(5) 0.020(2) Uani 1 1 d . . . . .
O11 O 0.6998(8) 0.2215(7) 0.6670(5) 0.025(3) Uani 1 1 d . . . . .
O33 O 0.3498(9) 0.1188(6) 0.4289(5) 0.022(3) Uani 1 1 d . . . . .
O10 O 0.5801(8) 0.1584(7) 0.7577(5) 0.022(3) Uani 1 1 d . . . . .
O9 O 0.2534(8) 0.1635(6) 0.7286(5) 0.019(2) Uani 1 1 d . . . . .
O3 O 0.6013(9) 0.3123(6) 0.7516(4) 0.022(3) Uani 1 1 d . . . . .
O31 O 0.6606(8) 0.0476(6) 0.5596(4) 0.019(2) Uani 1 1 d . . . . .
O22 O 0.0389(8) 0.1435(6) 0.5351(5) 0.019(2) Uani 1 1 d . . . . .
O35 O 0.0906(11) -0.2722(9) 0.4942(6) 0.050(4) Uani 1 1 d . . . B 1
O37 O 0.1479(10) -0.1327(7) 0.6717(5) 0.034(3) Uani 1 1 d . . . . .
O47 O 0.0863(9) 0.1594(7) 0.8062(6) 0.032(3) Uani 1 1 d . . . . .
O51 O -0.2030(13) 0.3466(10) 0.5994(7) 0.061(5) Uani 1 1 d . . . . .
Na54 Na -0.1048(12) -0.3445(10) 0.4847(8) 0.045(4) Uani 0.5 1 d . . P . .
O46 O -0.1731(8) 0.1555(7) 0.7872(5) 0.022(2) Uani 1 1 d . U . . .
O41 O 0.0496(9) -0.0528(7) 0.7914(5) 0.024(3) Uani 1 1 d . . . . .
O44 O -0.2051(15) -0.0626(11) 1.0001(9) 0.052(6) Uani 0.75 1 d . . P . .
O7AA O -0.0376(8) 0.0538(7) 0.6922(5) 0.026(3) Uani 1 1 d . . . . .
O45 O -0.0209(13) 0.0611(9) 0.9105(6) 0.055(4) Uani 1 1 d . U . . .
O42 O -0.1857(13) -0.0233(11) 0.8252(8) 0.074(5) Uani 1 1 d . U . . .
O50 O 0.0577(8) 0.3622(6) 0.7746(5) 0.022(3) Uani 1 1 d . U . . .
O48 O -0.0282(8) 0.2480(7) 0.6716(5) 0.023(3) Uani 1 1 d . . . . .
O49 O -0.1779(9) 0.3360(7) 0.7524(7) 0.038(3) Uani 1 1 d . . . . .
O38 O -0.0439(10) -0.2014(9) 0.6039(5) 0.043(4) Uani 1 1 d . . . . .
O40 O -0.2095(10) -0.0688(8) 0.6682(6) 0.036(3) Uani 1 1 d . . . . .
Na3 Na -0.0455(5) 0.0612(4) 0.8018(3) 0.0245(15) Uani 1 1 d . . . . .
Na4 Na -0.0421(5) 0.2527(4) 0.7863(3) 0.0232(15) Uani 1 1 d . . . . .
Na5 Na -0.0615(5) 0.3818(4) 0.6783(3) 0.0295(16) Uani 1 1 d . . . . .
Na2 Na -0.0304(5) -0.0890(4) 0.6818(3) 0.0316(17) Uani 1 1 d . . . . .
Na6 Na -0.1873(9) 0.0477(7) 0.9344(5) 0.015(3) Uani 0.5 1 d . U P . .
O39 O -0.0079(11) -0.0328(9) 0.5694(6) 0.048(4) Uani 1 1 d . . . C 1
O36 O 0.1114(11) -0.3271(8) 0.6617(6) 0.046(4) Uani 1 1 d . . . D 1
Na1 Na 0.1405(5) -0.2258(4) 0.5962(3) 0.0323(17) Uani 1 1 d . . . . .
O43 O -0.3569(18) 0.0748(15) 0.9076(10) 0.074(7) Uani 0.75 1 d . U P . .
O55 O 0.0210(19) 0.4465(15) 0.5988(11) 0.060(6) Uani 0.6667 1 d . U P E 1
O53 O 0.101(3) 0.417(3) 0.6317(19) 0.044(10) Uani 0.3333 1 d . U P E 2
O7 O 0.193(2) 0.5410(15) 0.6120(13) 0.141(10) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W2 O2 1.751(10) . ?
W2 O13 2.262(10) . ?
W2 O01J 1.974(10) . ?
W2 O4 1.970(10) . ?
W2 O8 1.862(11) . ?
W2 O9 1.878(11) . ?
W6 O29 1.791(10) . ?
W6 O17 2.003(10) . ?
W6 O23 1.743(10) . ?
W6 O13 2.150(9) . ?
W6 O18 1.921(11) . ?
W6 O9 2.108(10) . ?
W9 O26 1.737(10) . ?
W9 O32 1.900(10) . ?
W9 O6 1.952(11) . ?
W9 O15 1.900(10) . ?
W9 O12 2.163(9) . ?
W9 O20 1.950(10) . ?
W3 O5 1.969(11) . ?
W3 O14 2.217(10) . ?
W3 O01J 1.860(10) . ?
W3 O11 1.958(10) . ?
W3 O10 1.941(11) . ?
W3 O3 1.725(11) . ?
W8 O25 1.744(10) . ?
W8 O14 2.131(9) . ?
W8 O19 1.969(10) . ?
W8 O20 1.907(11) . ?
W8 O11 1.984(12) . ?
W8 O31 1.907(11) . ?
W7 O24 1.721(11) . ?
W7 O14 2.173(9) . ?
W7 O19 1.957(10) . ?
W7 O30 1.915(10) . ?
W7 O18 1.910(11) . ?
W7 O10 1.990(11) . ?
W4 O52 1.958(11) . ?
W4 O15 2.001(9) . ?
W4 O21 1.747(11) . ?
W4 O12 2.160(9) . ?
W4 O16 1.894(9) . ?
W4 O33 1.923(11) . ?
W5 O17 1.924(10) . ?
W5 O13 2.133(10) . ?
W5 O28 1.797(11) . ?
W5 O16 1.946(10) . ?
W5 O8 2.122(11) . ?
W5 O22 1.755(11) . ?
W1 O5 1.911(11) . ?
W1 O1 1.737(11) . ?
W1 O52 1.972(11) . ?
W1 O6 1.964(10) . ?
W1 O12 2.189(10) . ?
W1 O4 1.866(10) . ?
W10 O32 2.068(10) 3_656 ?
W10 O27 2.053(9) 3_656 ?
W10 O27 2.014(10) . ?
W10 O30 1.924(10) . ?
W10 O33 1.939(12) 3_656 ?
W10 O31 2.097(11) . ?
Co2 O29 2.071(9) . ?
Co2 O32 2.169(10) 3_656 ?
Co2 O34 2.156(11) . ?
Co2 O27 2.053(10) . ?
Co2 O28 2.080(12) . ?
Co2 O31 2.148(10) 3_656 ?
Co1 O14 1.933(9) . ?
Co1 O27 1.926(10) . ?
Co1 O13 1.915(9) . ?
Co1 O12 1.932(9) . ?
Co3 O32 2.068(10) 3_656 ?
Co3 O27 2.053(9) 3_656 ?
Co3 O27 2.014(10) . ?
Co3 O30 1.924(10) . ?
Co3 O33 1.939(12) 3_656 ?
Co3 O31 2.097(11) . ?
O26 Na1 2.447(13) 3_656 ?
O52 Na6 2.458(16) 4_665 ?
O24 Na5 2.387(14) 2_546 ?
O15 Na4 2.473(11) 4_665 ?
O34 Na1 2.553(14) . ?
O3 Na2 2.459(13) 2_556 ?
O35 Na54 2.85(2) . ?
O35 Na1 2.364(15) . ?
O37 Na2 2.476(15) . ?
O37 Na1 2.296(14) . ?
O47 Na3 2.449(14) . ?
O47 Na4 2.379(14) . ?
O51 Na5 2.499(18) . ?
Na54 Na6 3.804(19) 2_446 ?
Na54 O43 2.76(3) 2_446 ?
Na54 O55 2.79(3) 3_556 ?
Na54 O53 2.77(4) 3_556 ?
O46 Na3 2.371(13) . ?
O46 Na4 2.431(13) . ?
O41 Na3 2.392(14) . ?
O41 Na2 2.569(13) . ?
O44 Na6 2.42(2) . ?
O7AA Na3 2.325(12) . ?
O7AA Na2 2.549(15) . ?
O45 Na3 2.300(14) . ?
O45 Na6 2.27(2) . ?
O42 Na3 2.440(18) . ?
O42 Na6 2.63(2) . ?
O50 Na4 2.364(13) . ?
O50 Na5 2.517(13) . ?
O48 Na4 2.439(12) . ?
O48 Na5 2.421(14) . ?
O49 Na4 2.390(14) . ?
O49 Na5 2.385(14) . ?
O38 Na2 2.587(16) . ?
O38 Na1 2.462(15) . ?
O40 Na2 2.368(15) . ?
Na3 Na4 3.417(10) . ?
Na3 Na2 3.692(10) . ?
Na3 Na6 3.451(13) . ?
Na4 Na5 3.235(10) . ?
Na5 O55 2.35(2) . ?
Na5 O53 2.46(4) . ?
Na2 O39 2.606(16) . ?
Na2 Na1 3.822(10) . ?
Na6 O43 2.31(3) . ?
O36 Na1 2.313(16) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 W2 O13 173.5(4) . . ?
O2 W2 O01J 98.9(5) . . ?
O2 W2 O4 99.1(5) . . ?
O2 W2 O8 100.2(5) . . ?
O2 W2 O9 100.5(5) . . ?
O01J W2 O13 85.8(4) . . ?
O4 W2 O13 86.1(4) . . ?
O4 W2 O01J 80.6(4) . . ?
O8 W2 O13 75.9(4) . . ?
O8 W2 O01J 159.1(4) . . ?
O8 W2 O4 88.0(5) . . ?
O8 W2 O9 97.3(5) . . ?
O9 W2 O13 75.0(4) . . ?
O9 W2 O01J 87.5(4) . . ?
O9 W2 O4 158.4(4) . . ?
O29 W6 O17 90.7(4) . . ?
O29 W6 O13 91.5(4) . . ?
O29 W6 O18 94.8(4) . . ?
O29 W6 O9 164.6(4) . . ?
O17 W6 O13 73.2(4) . . ?
O17 W6 O9 83.5(4) . . ?
O23 W6 O29 103.7(5) . . ?
O23 W6 O17 97.7(5) . . ?
O23 W6 O13 162.6(5) . . ?
O23 W6 O18 99.5(5) . . ?
O23 W6 O9 91.2(5) . . ?
O18 W6 O17 160.1(4) . . ?
O18 W6 O13 87.5(4) . . ?
O18 W6 O9 86.2(4) . . ?
O9 W6 O13 73.2(4) . . ?
O26 W9 O32 103.2(5) . . ?
O26 W9 O6 95.7(5) . . ?
O26 W9 O15 100.4(4) . . ?
O26 W9 O12 168.3(5) . . ?
O26 W9 O20 99.7(5) . . ?
O32 W9 O6 160.9(4) . . ?
O32 W9 O15 90.2(4) . . ?
O32 W9 O12 87.8(4) . . ?
O32 W9 O20 85.8(4) . . ?
O6 W9 O12 73.5(4) . . ?
O15 W9 O6 89.0(4) . . ?
O15 W9 O12 75.3(4) . . ?
O15 W9 O20 159.9(4) . . ?
O20 W9 O6 88.4(4) . . ?
O20 W9 O12 84.8(4) . . ?
O5 W3 O14 88.0(4) . . ?
O01J W3 O5 86.1(4) . . ?
O01J W3 O14 86.3(4) . . ?
O01J W3 O11 158.6(5) . . ?
O01J W3 O10 90.7(4) . . ?
O11 W3 O5 86.3(4) . . ?
O11 W3 O14 73.5(4) . . ?
O10 W3 O5 163.3(4) . . ?
O10 W3 O14 75.4(4) . . ?
O10 W3 O11 90.8(5) . . ?
O3 W3 O5 99.6(5) . . ?
O3 W3 O14 168.0(5) . . ?
O3 W3 O01J 103.3(5) . . ?
O3 W3 O11 97.6(5) . . ?
O3 W3 O10 97.1(5) . . ?
O25 W8 O14 167.1(4) . . ?
O25 W8 O19 97.8(4) . . ?
O25 W8 O20 99.4(4) . . ?
O25 W8 O11 94.3(5) . . ?
O25 W8 O31 102.2(5) . . ?
O19 W8 O14 74.7(4) . . ?
O19 W8 O11 86.0(5) . . ?
O20 W8 O14 88.2(4) . . ?
O20 W8 O19 162.8(4) . . ?
O20 W8 O11 92.0(5) . . ?
O20 W8 O31 88.4(4) . . ?
O11 W8 O14 74.9(4) . . ?
O31 W8 O14 88.2(4) . . ?
O31 W8 O19 88.6(4) . . ?
O31 W8 O11 163.1(4) . . ?
O24 W7 O14 168.5(5) . . ?
O24 W7 O19 96.8(5) . . ?
O24 W7 O30 100.8(5) . . ?
O24 W7 O18 102.6(5) . . ?
O24 W7 O10 97.6(5) . . ?
O19 W7 O14 74.0(4) . . ?
O19 W7 O10 87.5(4) . . ?
O30 W7 O14 85.8(4) . . ?
O30 W7 O19 86.5(4) . . ?
O30 W7 O10 161.2(4) . . ?
O18 W7 O14 86.9(4) . . ?
O18 W7 O19 160.7(4) . . ?
O18 W7 O30 89.1(4) . . ?
O18 W7 O10 90.7(4) . . ?
O10 W7 O14 75.4(4) . . ?
O52 W4 O15 87.3(4) . . ?
O52 W4 O12 75.4(4) . . ?
O15 W4 O12 73.4(4) . . ?
O21 W4 O52 97.7(5) . . ?
O21 W4 O15 97.2(4) . . ?
O21 W4 O12 168.4(4) . . ?
O21 W4 O16 101.1(5) . . ?
O21 W4 O33 100.9(5) . . ?
O16 W4 O52 92.1(4) . . ?
O16 W4 O15 161.6(4) . . ?
O16 W4 O12 88.6(4) . . ?
O16 W4 O33 89.2(5) . . ?
O33 W4 O52 160.7(5) . . ?
O33 W4 O15 85.5(4) . . ?
O33 W4 O12 85.4(4) . . ?
O17 W5 O13 75.1(4) . . ?
O17 W5 O16 160.4(4) . . ?
O17 W5 O8 85.0(4) . . ?
O28 W5 O17 94.1(5) . . ?
O28 W5 O13 92.8(4) . . ?
O28 W5 O16 92.2(5) . . ?
O28 W5 O8 166.4(4) . . ?
O16 W5 O13 86.1(4) . . ?
O16 W5 O8 84.6(4) . . ?
O8 W5 O13 73.8(4) . . ?
O22 W5 O17 98.1(4) . . ?
O22 W5 O13 164.5(4) . . ?
O22 W5 O28 101.7(5) . . ?
O22 W5 O16 98.7(4) . . ?
O22 W5 O8 91.9(5) . . ?
O5 W1 O52 164.5(4) . . ?
O5 W1 O6 87.9(4) . . ?
O5 W1 O12 90.2(4) . . ?
O1 W1 O5 100.1(5) . . ?
O1 W1 O52 95.4(5) . . ?
O1 W1 O6 98.0(5) . . ?
O1 W1 O12 166.0(4) . . ?
O1 W1 O4 102.0(5) . . ?
O52 W1 O12 74.5(4) . . ?
O6 W1 O52 89.4(4) . . ?
O6 W1 O12 72.7(4) . . ?
O4 W1 O5 87.9(5) . . ?
O4 W1 O52 89.5(5) . . ?
O4 W1 O6 160.0(5) . . ?
O4 W1 O12 87.7(4) . . ?
O32 W10 O31 172.9(4) 3_656 . ?
O27 W10 O32 93.6(4) 3_656 3_656 ?
O27 W10 O32 82.0(4) . 3_656 ?
O27 W10 O27 77.5(4) . 3_656 ?
O27 W10 O31 80.8(4) 3_656 . ?
O27 W10 O31 92.5(4) . . ?
O30 W10 O32 97.4(4) . 3_656 ?
O30 W10 O27 94.3(4) . . ?
O30 W10 O27 165.2(4) . 3_656 ?
O30 W10 O33 97.5(4) . 3_656 ?
O30 W10 O31 87.4(4) . . ?
O33 W10 O32 89.9(4) 3_656 3_656 ?
O33 W10 O27 92.3(4) 3_656 3_656 ?
O33 W10 O27 166.4(4) 3_656 . ?
O33 W10 O31 94.7(4) 3_656 . ?
O29 Co2 O32 91.6(4) . 3_656 ?
O29 Co2 O34 92.4(4) . . ?
O29 Co2 O28 89.9(4) . . ?
O29 Co2 O31 172.2(4) . 3_656 ?
O34 Co2 O32 103.4(4) . 3_656 ?
O27 Co2 O29 92.9(4) . . ?
O27 Co2 O32 78.6(4) . 3_656 ?
O27 Co2 O34 174.3(4) . . ?
O27 Co2 O28 94.3(4) . . ?
O27 Co2 O31 79.6(4) . 3_656 ?
O28 Co2 O32 172.8(4) . 3_656 ?
O28 Co2 O34 83.5(4) . . ?
O28 Co2 O31 92.6(4) . 3_656 ?
O31 Co2 O32 84.9(4) 3_656 3_656 ?
O31 Co2 O34 95.2(4) 3_656 . ?
O27 Co1 O14 112.6(4) . . ?
O27 Co1 O12 113.7(4) . . ?
O13 Co1 O14 108.1(4) . . ?
O13 Co1 O27 108.2(4) . . ?
O13 Co1 O12 108.5(4) . . ?
O12 Co1 O14 105.5(4) . . ?
O32 Co3 O31 172.9(4) 3_656 . ?
O27 Co3 O32 93.6(4) 3_656 3_656 ?
O27 Co3 O32 82.0(4) . 3_656 ?
O27 Co3 O27 77.5(4) . 3_656 ?
O27 Co3 O31 80.8(4) 3_656 . ?
O27 Co3 O31 92.5(4) . . ?
O30 Co3 O32 97.4(4) . 3_656 ?
O30 Co3 O27 165.2(4) . 3_656 ?
O30 Co3 O27 94.3(4) . . ?
O30 Co3 O33 97.5(4) . 3_656 ?
O30 Co3 O31 87.4(4) . . ?
O33 Co3 O32 89.9(4) 3_656 3_656 ?
O33 Co3 O27 166.4(4) 3_656 . ?
O33 Co3 O27 92.3(4) 3_656 3_656 ?
O33 Co3 O31 94.7(4) 3_656 . ?
W6 O29 Co2 138.1(6) . . ?
W9 O26 Na1 139.3(6) . 3_656 ?
W9 O32 W10 136.6(5) . 3_656 ?
W9 O32 Co2 124.9(5) . 3_656 ?
W5 O17 W6 110.9(5) . . ?
W1 O5 W3 146.5(6) . . ?
W4 O52 W1 112.4(5) . . ?
W4 O52 Na6 133.2(6) . 4_665 ?
W1 O52 Na6 111.9(5) . 4_665 ?
W9 O6 W1 115.0(5) . . ?
W7 O24 Na5 139.7(6) . 2_546 ?
W9 O15 W4 113.1(4) . . ?
W9 O15 Na4 127.9(4) . 4_665 ?
W4 O15 Na4 117.4(4) . 4_665 ?
Co2 O34 Na1 128.2(6) . . ?
W8 O14 W3 98.3(4) . . ?
W8 O14 W7 98.4(4) . . ?
W7 O14 W3 96.4(3) . . ?
Co1 O14 W3 121.9(5) . . ?
Co1 O14 W8 118.5(4) . . ?
Co1 O14 W7 118.4(5) . . ?
W7 O19 W8 112.2(5) . . ?
W10 O27 Co2 101.2(4) 3_656 . ?
W10 O27 Co2 101.8(5) . . ?
Co1 O27 W10 113.9(5) . 3_656 ?
Co1 O27 W10 116.0(5) . . ?
Co1 O27 Co2 119.0(5) . . ?
Co1 O27 Co3 116.0(5) . . ?
Co3 O27 Co2 101.8(5) . . ?
W7 O30 W10 145.3(6) . . ?
W7 O30 Co3 145.3(6) . . ?
W6 O13 W2 98.2(3) . . ?
W5 O13 W2 97.8(4) . . ?
W5 O13 W6 98.1(4) . . ?
Co1 O13 W2 120.3(5) . . ?
Co1 O13 W6 118.1(5) . . ?
Co1 O13 W5 119.5(4) . . ?
W3 O01J W2 157.9(5) . . ?
W9 O12 W1 98.7(4) . . ?
W4 O12 W9 97.7(4) . . ?
W4 O12 W1 97.3(4) . . ?
Co1 O12 W9 120.4(5) . . ?
Co1 O12 W4 117.0(5) . . ?
Co1 O12 W1 120.9(4) . . ?
W7 O18 W6 155.3(6) . . ?
W5 O28 Co2 135.3(6) . . ?
W1 O4 W2 155.6(7) . . ?
W4 O16 W5 154.1(6) . . ?
W8 O20 W9 156.6(6) . . ?
W2 O8 W5 112.4(5) . . ?
W3 O11 W8 113.2(5) . . ?
W4 O33 W10 143.9(6) . 3_656 ?
W3 O10 W7 112.7(5) . . ?
W2 O9 W6 113.5(5) . . ?
W3 O3 Na2 141.8(6) . 2_556 ?
W8 O31 W10 137.6(5) . . ?
W8 O31 Co2 122.8(5) . 3_656 ?
W8 O31 Co3 137.6(5) . . ?
Na1 O35 Na54 114.9(6) . . ?
Na1 O37 Na2 106.3(6) . . ?
Na4 O47 Na3 90.1(5) . . ?
O35 Na54 Na6 148.5(6) . 2_446 ?
O43 Na54 O35 112.2(8) 2_446 . ?
O43 Na54 Na6 37.0(6) 2_446 2_446 ?
O43 Na54 O55 106.2(9) 2_446 3_556 ?
O43 Na54 O53 120.2(12) 2_446 3_556 ?
O55 Na54 O35 87.5(7) 3_556 . ?
O55 Na54 Na6 105.7(7) 3_556 2_446 ?
Na3 O46 Na4 90.7(4) . . ?
Na3 O41 Na2 96.1(5) . . ?
Na3 O7AA Na2 98.4(5) . . ?
Na6 O45 Na3 98.0(7) . . ?
Na3 O42 Na6 85.7(6) . . ?
Na4 O50 Na5 83.0(4) . . ?
Na5 O48 Na4 83.5(4) . . ?
Na5 O49 Na4 85.3(4) . . ?
Na1 O38 Na2 98.4(5) . . ?
O47 Na3 Na4 44.1(3) . . ?
O47 Na3 Na2 118.5(4) . . ?
O47 Na3 Na6 115.2(4) . . ?
O46 Na3 O47 89.4(5) . . ?
O46 Na3 O41 162.0(5) . . ?
O46 Na3 O42 86.0(6) . . ?
O46 Na3 Na4 45.4(3) . . ?
O46 Na3 Na2 119.0(4) . . ?
O46 Na3 Na6 75.5(4) . . ?
O41 Na3 O47 103.8(5) . . ?
O41 Na3 O42 84.1(6) . . ?
O41 Na3 Na4 145.5(4) . . ?
O41 Na3 Na2 43.8(3) . . ?
O41 Na3 Na6 108.7(4) . . ?
O7AA Na3 O47 90.5(5) . . ?
O7AA Na3 O46 88.8(4) . . ?
O7AA Na3 O41 79.0(4) . . ?
O7AA Na3 O42 104.0(6) . . ?
O7AA Na3 Na4 87.7(4) . . ?
O7AA Na3 Na2 43.1(4) . . ?
O7AA Na3 Na6 149.2(4) . . ?
O45 Na3 O47 84.5(6) . . ?
O45 Na3 O46 100.9(5) . . ?
O45 Na3 O41 92.6(5) . . ?
O45 Na3 O7AA 168.9(6) . . ?
O45 Na3 O42 82.1(6) . . ?
O45 Na3 Na4 95.5(5) . . ?
O45 Na3 Na2 132.4(5) . . ?
O45 Na3 Na6 40.7(5) . . ?
O42 Na3 O47 164.7(6) . . ?
O42 Na3 Na4 130.2(5) . . ?
O42 Na3 Na2 76.3(5) . . ?
O42 Na3 Na6 49.5(5) . . ?
Na4 Na3 Na2 130.7(2) . . ?
Na4 Na3 Na6 99.0(3) . . ?
Na6 Na3 Na2 123.9(3) . . ?
O15 Na4 Na3 87.9(3) 4_566 . ?
O15 Na4 Na5 131.2(4) 4_566 . ?
O47 Na4 O15 83.6(4) . 4_566 ?
O47 Na4 O46 89.7(5) . . ?
O47 Na4 O48 93.5(4) . . ?
O47 Na4 O49 171.5(5) . . ?
O47 Na4 Na3 45.8(3) . . ?
O47 Na4 Na5 130.2(4) . . ?
O46 Na4 O15 90.7(4) . 4_566 ?
O46 Na4 O48 94.3(4) . . ?
O46 Na4 Na3 43.9(3) . . ?
O46 Na4 Na5 118.8(4) . . ?
O50 Na4 O15 94.1(4) . 4_566 ?
O50 Na4 O47 101.8(5) . . ?
O50 Na4 O46 168.0(5) . . ?
O50 Na4 O48 81.5(4) . . ?
O50 Na4 O49 82.1(5) . . ?
O50 Na4 Na3 147.1(4) . . ?
O50 Na4 Na5 50.6(3) . . ?
O48 Na4 O15 174.2(5) . 4_566 ?
O48 Na4 Na3 93.7(4) . . ?
O48 Na4 Na5 48.0(3) . . ?
O49 Na4 O15 103.8(5) . 4_566 ?
O49 Na4 O46 86.0(5) . . ?
O49 Na4 O48 79.5(5) . . ?
O49 Na4 Na3 129.2(4) . . ?
O49 Na4 Na5 47.3(3) . . ?
Na5 Na4 Na3 140.6(3) . . ?
O24 Na5 O51 108.9(6) 2_556 . ?
O24 Na5 O50 87.1(4) 2_556 . ?
O24 Na5 O48 161.6(5) 2_556 . ?
O24 Na5 Na4 113.1(4) 2_556 . ?
O24 Na5 O53 96.0(11) 2_556 . ?
O51 Na5 O50 155.0(6) . . ?
O51 Na5 Na4 108.6(5) . . ?
O50 Na5 Na4 46.5(3) . . ?
O48 Na5 O51 81.1(5) . . ?
O48 Na5 O50 78.8(4) . . ?
O48 Na5 Na4 48.5(3) . . ?
O48 Na5 O53 93.5(11) . . ?
O49 Na5 O24 85.8(4) . 2_556 ?
O49 Na5 O51 82.9(5) . . ?
O49 Na5 O50 79.1(5) . . ?
O49 Na5 O48 80.0(4) . . ?
O49 Na5 Na4 47.4(3) . . ?
O49 Na5 O53 160.3(11) . . ?
O55 Na5 O24 85.6(7) . 2_556 ?
O55 Na5 O51 89.9(7) . . ?
O55 Na5 O50 111.0(7) . . ?
O55 Na5 O48 110.4(7) . . ?
O55 Na5 O49 166.4(8) . . ?
O55 Na5 Na4 146.2(7) . . ?
O53 Na5 O51 114.6(11) . . ?
O53 Na5 O50 81.4(11) . . ?
O53 Na5 Na4 115.1(11) . . ?
O3 Na2 O37 102.2(5) 2_546 . ?
O3 Na2 O41 79.1(4) 2_546 . ?
O3 Na2 O7AA 130.0(4) 2_546 . ?
O3 Na2 O38 78.4(5) 2_546 . ?
O3 Na2 Na3 95.0(3) 2_546 . ?
O3 Na2 O39 149.1(5) 2_546 . ?
O3 Na2 Na1 93.7(4) 2_546 . ?
O37 Na2 O41 79.5(4) . . ?
O37 Na2 O7AA 111.0(5) . . ?
O37 Na2 O38 74.6(5) . . ?
O37 Na2 Na3 111.8(4) . . ?
O37 Na2 O39 83.5(5) . . ?
O37 Na2 Na1 35.2(3) . . ?
O41 Na2 O38 141.0(5) . . ?
O41 Na2 Na3 40.1(3) . . ?
O41 Na2 O39 131.6(5) . . ?
O41 Na2 Na1 111.5(4) . . ?
O7AA Na2 O41 71.8(4) . . ?
O7AA Na2 O38 145.2(5) . . ?
O7AA Na2 Na3 38.5(3) . . ?
O7AA Na2 O39 72.8(4) . . ?
O7AA Na2 Na1 134.4(3) . . ?
O38 Na2 Na3 171.8(4) . . ?
O38 Na2 O39 73.9(5) . . ?
O38 Na2 Na1 39.6(3) . . ?
O40 Na2 O3 77.1(5) . 2_546 ?
O40 Na2 O37 164.7(5) . . ?
O40 Na2 O41 114.9(5) . . ?
O40 Na2 O7AA 79.6(5) . . ?
O40 Na2 O38 90.4(5) . . ?
O40 Na2 Na3 83.4(4) . . ?
O40 Na2 O39 89.5(5) . . ?
O40 Na2 Na1 129.6(4) . . ?
Na3 Na2 Na1 147.0(3) . . ?
O39 Na2 Na3 111.2(4) . . ?
O39 Na2 Na1 73.4(4) . . ?
W1 Na6 Na54 73.2(3) 4_566 2_456 ?
O52 Na6 W1 29.8(3) 4_566 4_566 ?
O52 Na6 Na54 59.2(4) 4_566 2_456 ?
O52 Na6 O42 139.4(7) 4_566 . ?
O52 Na6 Na3 98.7(4) 4_566 . ?
O44 Na6 W1 98.6(6) . 4_566 ?
O44 Na6 O52 122.9(7) . 4_566 ?
O44 Na6 Na54 93.3(6) . 2_456 ?
O44 Na6 O42 96.9(8) . . ?
O44 Na6 Na3 126.5(6) . . ?
O45 Na6 W1 71.1(5) . 4_566 ?
O45 Na6 O52 80.6(6) . 4_566 ?
O45 Na6 Na54 139.8(6) . 2_456 ?
O45 Na6 O44 109.6(8) . . ?
O45 Na6 O42 78.5(6) . . ?
O45 Na6 Na3 41.3(4) . . ?
O45 Na6 O43 147.3(9) . . ?
O42 Na6 W1 149.0(6) . 4_566 ?
O42 Na6 Na54 132.5(6) . 2_456 ?
O42 Na6 Na3 44.8(4) . . ?
Na3 Na6 W1 105.2(3) . 4_566 ?
Na3 Na6 Na54 139.3(5) . 2_456 ?
O43 Na6 W1 116.5(7) . 4_566 ?
O43 Na6 O52 92.9(8) . 4_566 ?
O43 Na6 Na54 46.0(6) . 2_456 ?
O43 Na6 O44 100.8(9) . . ?
O43 Na6 O42 86.5(8) . . ?
O43 Na6 Na3 109.7(7) . . ?
O26 Na1 O34 84.2(4) 3_656 . ?
O26 Na1 O38 179.0(6) 3_656 . ?
O26 Na1 Na2 137.9(4) 3_656 . ?
O34 Na1 Na2 80.6(3) . . ?
O35 Na1 O26 95.3(5) . 3_656 ?
O35 Na1 O34 82.4(5) . . ?
O35 Na1 O38 84.3(5) . . ?
O35 Na1 Na2 120.9(4) . . ?
O37 Na1 O26 99.7(5) . 3_656 ?
O37 Na1 O34 75.9(5) . . ?
O37 Na1 O35 152.0(6) . . ?
O37 Na1 O38 80.3(5) . . ?
O37 Na1 Na2 38.4(4) . . ?
O37 Na1 O36 98.5(5) . . ?
O38 Na1 O34 94.9(5) . . ?
O38 Na1 Na2 42.1(4) . . ?
O36 Na1 O26 96.4(5) . 3_656 ?
O36 Na1 O34 174.3(5) . . ?
O36 Na1 O35 103.2(6) . . ?
O36 Na1 O38 84.5(5) . . ?
O36 Na1 Na2 95.3(4) . . ?
Na6 O43 Na54 97.0(9) . 2_456 ?
Na5 O55 Na54 110.2(10) . 3_556 ?
Na5 O53 Na54 107.3(16) . 3_556 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O26 W9 O32 W10 -143.9(7) . . . 3_656 ?
O26 W9 O32 Co2 57.1(6) . . . 3_656 ?
O32 W9 O26 Na1 -63.7(9) . . . 3_656 ?
O17 W6 O29 Co2 54.5(8) . . . . ?
O17 W5 O28 Co2 -51.6(8) . . . . ?
O5 W3 O01J W2 22.5(16) . . . . ?
O5 W3 O3 Na2 80.3(9) . . . 2_556 ?
O5 W1 O4 W2 -24.7(16) . . . . ?
O1 W1 O4 W2 -124.6(16) . . . . ?
O52 W4 O16 W5 -138.6(14) . . . . ?
O52 W1 O4 W2 140.1(16) . . . . ?
O6 W9 O26 Na1 113.6(9) . . . 3_656 ?
O6 W9 O32 W10 44.4(16) . . . 3_656 ?
O6 W9 O32 Co2 -114.6(12) . . . 3_656 ?
O6 W1 O4 W2 53(2) . . . . ?
O15 W9 O26 Na1 -156.4(9) . . . 3_656 ?
O15 W9 O32 W10 -43.2(7) . . . 3_656 ?
O15 W9 O32 Co2 157.8(5) . . . 3_656 ?
O15 W4 O16 W5 -51(2) . . . . ?
O14 W3 O01J W2 -65.8(16) . . . . ?
O14 W3 O3 Na2 -150.7(15) . . . 2_556 ?
O14 W7 O24 Na5 -157.2(16) . . . 2_546 ?
O23 W6 O29 Co2 152.6(8) . . . . ?
O2 W2 O8 W5 -172.8(5) . . . . ?
O2 W2 O9 W6 174.4(5) . . . . ?
O19 W7 O24 Na5 -120.9(9) . . . 2_546 ?
O30 W7 O24 Na5 -33.1(9) . . . 2_546 ?
O13 W2 O8 W5 1.8(4) . . . . ?
O13 W2 O9 W6 -0.7(5) . . . . ?
O13 W6 O29 Co2 -18.7(8) . . . . ?
O13 W5 O28 Co2 23.6(8) . . . . ?
O01J W2 O8 W5 31.6(15) . . . . ?
O01J W2 O9 W6 -87.0(5) . . . . ?
O01J W3 O3 Na2 -7.9(10) . . . 2_556 ?
O21 W4 O16 W5 123.1(14) . . . . ?
O12 W9 O26 Na1 136.3(18) . . . 3_656 ?
O12 W9 O32 W10 32.1(7) . . . 3_656 ?
O12 W9 O32 Co2 -126.9(5) . . . 3_656 ?
O12 W4 O16 W5 -63.2(14) . . . . ?
O12 W1 O4 W2 65.6(16) . . . . ?
O18 W6 O29 Co2 -106.3(8) . . . . ?
O18 W7 O24 Na5 58.4(9) . . . 2_546 ?
O4 W2 O8 W5 88.3(5) . . . . ?
O4 W2 O9 W6 -30.7(15) . . . . ?
O16 W5 O28 Co2 109.9(8) . . . . ?
O20 W9 O26 Na1 24.3(10) . . . 3_656 ?
O20 W9 O32 W10 117.1(7) . . . 3_656 ?
O20 W9 O32 Co2 -41.9(5) . . . 3_656 ?
O8 W2 O9 W6 72.5(6) . . . . ?
O8 W5 O28 Co2 34(2) . . . . ?
O11 W3 O01J W2 -47(2) . . . . ?
O11 W3 O3 Na2 167.9(9) . . . 2_556 ?
O33 W4 O16 W5 22.2(14) . . . . ?
O10 W3 O01J W2 -141.1(16) . . . . ?
O10 W3 O3 Na2 -100.4(9) . . . 2_556 ?
O10 W7 O24 Na5 150.8(8) . . . 2_546 ?
O9 W2 O8 W5 -70.7(5) . . . . ?
O9 W6 O29 Co2 -13(2) . . . . ?
O3 W3 O01J W2 121.4(16) . . . . ?
O22 W5 O28 Co2 -150.8(7) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Co2Fe2plate
_database_code_depnum_ccdc_archive 'CCDC 2068501'
loop_
_audit_author_name
_audit_author_address
'Friedrich Steuber'
;Trinity College Dublin
Ireland
;
_audit_update_record             
;
2021-03-07 deposited with the CCDC.	2023-10-30 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_PLAT306_Co2Fe2plate         
;
PROBLEM: Isolated Oxygen Atom (H-atoms Missing ?) .......       O01E Check 
RESPONSE: As a hydrogen bond network could not be modelled to satisfaction,
hydrogen atoms were omitted in the refinement. These oxygen atoms belong
to water molecules.
;
# end Validation Reply Form
_audit_creation_date             2020-08-27
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.07.31 svn.rc2a77460 for OlexSys, GUI svn.r6145)
;
_shelx_SHELXL_version_number     2018/3
loop_
_audit_author_email
sorianoj@tcd.ie
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
SFI
Dublin
Ireland
College
of
College
Dublin
;
_audit_contact_author_email        schmittw@tcd.ie
_audit_contact_author_name         'Schmitt, W.'
_audit_contact_author_phone        +353-1-8963495
_publ_contact_author_id_orcid      0000-0002-0058-9404
_publ_requested_journal            ''
_publ_section_references
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Co4 Fe2 Na14 O90 W18, 5(H2O)'
_chemical_formula_sum            'Co4 Fe2 Na14 O97 W18'
_chemical_formula_weight         5530.58
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           18
_space_group_name_H-M_alt        'P 21 21 2'
_space_group_name_Hall           'P 2 2ab'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'

_cell_length_a                   26.056(3)
_cell_length_b                   20.996(3)
_cell_length_c                   17.747(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     9709(2)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    9951
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      26.24
_cell_measurement_theta_min      2.167
_shelx_estimated_absorpt_T_max   0.185
_shelx_estimated_absorpt_T_min   0.071
_exptl_absorpt_coefficient_mu    22.355
_exptl_absorpt_correction_T_max  0.7454
_exptl_absorpt_correction_T_min  0.1699
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1796 before and 0.0906 after correction. The Ratio of minimum to maximum transmission is 0.2279. The λ/2 correction factor is 0.00150.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            orange
_exptl_crystal_colour_primary    orange
_exptl_crystal_density_diffrn    3.784
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       oval
_exptl_crystal_F_000             9688
_exptl_crystal_size_max          0.252
_exptl_crystal_size_mid          0.199
_exptl_crystal_size_min          0.114
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.1042
_diffrn_reflns_av_unetI/netI     0.0988
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_limit_h_max       32
_diffrn_reflns_limit_h_min       -32
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            106183
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.985
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.514
_diffrn_reflns_theta_min         1.502
_diffrn_ambient_temperature      100.01
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.842
_reflns_Friedel_fraction_full    0.999
_reflns_Friedel_fraction_max     0.983
_reflns_number_gt                13340
_reflns_number_total             19876
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences. Completness statistics refer to single and
 composite reflections containing twin component 1 only.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.38A (?, 2016)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.38A (?, 2016)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         6.309
_refine_diff_density_min         -6.518
_refine_diff_density_rms         0.667
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.45(5)
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.032
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     700
_refine_ls_number_reflns         19876
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1452
_refine_ls_R_factor_gt           0.0934
_refine_ls_restrained_S_all      1.032
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.1178P)²+1495.3499P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2410
_refine_ls_wR_factor_ref         0.2896
_refine_special_details          'Refined as a 2-component inversion twin.,Twin'
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.55(5)
 0.45(5)
2. Others
 Fixed Sof: Na02(0.5) Na2(0.5) Na6(0.5) Na8(0.5) Na9(0.5) Na10(0.5) Na03(0.5)
 Na11(0.5) Na12(0.5) O2AA(0.5) Na1B(0.5) Na3B(0.25) O7AA(0.5) O5BA(0.5)
 O4BA(0.5) Na0A(0.5) Na6B(0.5) Na6A(0.5) Na7B(0.25) Na5A(0.5) O73(0.5) Na73(0.5)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W7 W 0.82099(13) 0.07676(11) 0.30160(18) 0.0352(7) Uani 1 1 d . . . . .
W14 W 0.79864(13) 0.37610(11) 0.09549(17) 0.0361(7) Uani 1 1 d . . . . .
W16 W 0.69731(13) 0.12757(11) 0.00490(18) 0.0385(7) Uani 1 1 d . . . . .
W13 W 0.67881(12) 0.41553(11) 0.20117(18) 0.0363(7) Uani 1 1 d . . . . .
W8 W 0.70136(13) 0.11506(12) 0.40704(17) 0.0380(7) Uani 1 1 d . . . . .
W15 W 0.80609(14) 0.23912(12) 0.00665(17) 0.0395(7) Uani 1 1 d . . . . .
W4 W 0.80152(14) 0.36404(12) 0.49868(19) 0.0422(8) Uani 1 1 d . . . . .
W6 W 0.91498(13) 0.18013(12) 0.3017(2) 0.0405(7) Uani 1 1 d . . . . .
W11 W 0.72995(15) 0.35299(12) -0.06052(18) 0.0422(8) Uani 1 1 d . . . . .
W5 W 0.90557(13) 0.33288(12) 0.4062(2) 0.0428(8) Uani 1 1 d . . . . .
W2 W 0.88990(14) 0.09833(12) 0.45770(19) 0.0427(8) Uani 1 1 d . . . . .
W18 W 0.58487(13) 0.31320(13) 0.2021(2) 0.0442(8) Uani 1 1 d . . . . .
W3 W 0.76948(15) 0.13736(13) 0.56339(18) 0.0431(8) Uani 1 1 d . . . . .
W1 W 0.87983(14) 0.25243(13) 0.56355(19) 0.0430(8) Uani 1 1 d . . . . .
W12 W 0.61907(15) 0.23942(13) -0.0591(2) 0.0460(8) Uani 1 1 d . . . . .
W9 W 0.69355(14) 0.25131(14) 0.4969(2) 0.0462(8) Uani 1 1 d . . . . .
W17 W 0.59376(13) 0.16013(13) 0.0988(2) 0.0463(8) Uani 1 1 d . . . . .
W10 W 0.60944(14) 0.39362(12) 0.0467(2) 0.0433(8) Uani 1 1 d . . . . .
Co3 Co 0.6960(4) 0.2680(4) 0.1098(6) 0.032(2) Uani 1 1 d . . . . .
Co2 Co 0.7910(4) 0.3580(4) 0.2941(6) 0.035(2) Uani 1 1 d . . . . .
Co1 Co 0.8045(4) 0.2239(4) 0.3955(5) 0.031(2) Uani 1 1 d . . . . .
Fe1 Fe 0.7014(4) 0.2627(4) 0.2945(6) 0.032(2) Uani 1 1 d . . . . .
Co4 Co 0.7083(4) 0.1343(4) 0.2084(6) 0.036(2) Uani 1 1 d . . . . .
Fe2 Fe 0.7989(4) 0.2297(4) 0.2071(6) 0.033(2) Uani 1 1 d . . . . .
Na7 Na 0.7127(11) 0.4932(11) 0.0380(14) 0.032(5) Uiso 1 1 d . . . . .
Na1 Na 0.7846(12) -0.0034(12) 0.4671(16) 0.042(7) Uiso 1 1 d . . . . .
Na4 Na 0.9355(15) 0.1636(17) 0.037(2) 0.063(9) Uiso 1 1 d . . . . .
O58 O 0.7385(17) 0.4176(18) 0.131(2) 0.028(9) Uiso 1 1 d . . . . .
O4 O 0.9003(18) 0.1746(19) 0.513(3) 0.034(10) Uiso 1 1 d . . . . .
O41 O 0.6731(19) 0.3964(19) -0.008(3) 0.035(10) Uiso 1 1 d . . . . .
O33 O 0.788(2) 0.132(2) 0.241(3) 0.040(11) Uiso 1 1 d . . . . .
O8 O 0.8586(18) 0.039(2) 0.389(3) 0.034(10) Uiso 1 1 d . . . . .
O9 O 0.9406(19) 0.125(2) 0.385(3) 0.039(11) Uiso 1 1 d . . . . .
O31 O 0.687(2) 0.284(2) 0.406(3) 0.042(11) Uiso 1 1 d . . . . .
O62 O 0.7229(19) 0.229(2) 0.194(3) 0.038(11) Uiso 1 1 d . . . . .
O60 O 0.7485(18) 0.3051(19) 0.046(3) 0.033(10) Uiso 1 1 d . . . . .
O67 O 0.6303(16) 0.0983(17) 0.039(2) 0.026(9) Uiso 1 1 d . . . . .
O52 O 0.687(2) 0.487(2) 0.246(3) 0.036(10) Uiso 1 1 d . . . . .
O39 O 0.6801(17) 0.2865(19) -0.077(3) 0.034(10) Uiso 1 1 d . . . . .
O61 O 0.6574(18) 0.210(2) 0.049(3) 0.036(10) Uiso 1 1 d . . . . .
O42 O 0.7828(18) 0.294(2) -0.082(3) 0.037(11) Uiso 1 1 d . . . . .
O28 O 0.874(2) 0.223(2) 0.245(3) 0.044(12) Uiso 1 1 d . . . . .
O29 O 0.867(2) 0.350(2) 0.327(3) 0.044(12) Uiso 1 1 d . . . . .
O53 O 0.846(2) 0.435(2) 0.109(3) 0.042(12) Uiso 1 1 d . . . . .
O57 O 0.612(2) 0.395(2) 0.246(3) 0.039(11) Uiso 1 1 d . . . . .
O11 O 0.842(2) 0.327(3) 0.591(3) 0.056(14) Uiso 1 1 d . . . . .
O55 O 0.7534(19) 0.186(2) -0.026(3) 0.034(11) Uiso 1 1 d . . . . .
O65 O 0.807(2) 0.327(2) 0.179(3) 0.043(11) Uiso 1 1 d . . . . .
O24 O 0.658(2) 0.168(3) 0.464(3) 0.060(15) Uiso 1 1 d . . . . .
O01E O 0.829(2) -0.088(2) 0.393(3) 0.048(13) Uiso 1 1 d . . . . .
O20 O 0.8871(18) 0.0970(19) 0.264(3) 0.032(10) Uiso 1 1 d . . . . .
O32 O 0.6980(17) 0.1634(18) 0.321(2) 0.031(9) Uiso 1 1 d . . . . .
O48 O 0.8606(19) 0.206(2) -0.039(3) 0.039(11) Uiso 1 1 d . . . . .
O10 O 0.9319(19) 0.298(2) 0.506(3) 0.040(11) Uiso 1 1 d . . . . .
O47 O 0.778(3) 0.406(3) -0.007(4) 0.068(17) Uiso 1 1 d . . . . .
O40 O 0.599(2) 0.315(2) -0.006(3) 0.044(12) Uiso 1 1 d . . . . .
O56 O 0.574(2) 0.243(2) 0.140(3) 0.044(12) Uiso 1 1 d . . . . .
O01M O 0.929(2) 0.266(3) 0.116(4) 0.061(16) Uiso 1 1 d . . . . .
O34 O 0.778(2) 0.262(2) 0.310(3) 0.045(12) Uiso 1 1 d . . . . .
O26 O 0.8428(19) 0.281(2) 0.460(3) 0.038(11) Uiso 1 1 d . . . . .
O69 O 0.6332(18) 0.1412(19) 0.181(3) 0.033(10) Uiso 1 1 d . . . . .
O63 O 0.6265(18) 0.269(2) 0.267(3) 0.035(10) Uiso 1 1 d . . . . .
O59 O 0.647(2) 0.335(2) 0.132(3) 0.047(13) Uiso 1 1 d . . . . .
O23 O 0.749(2) 0.308(2) 0.527(3) 0.049(14) Uiso 1 1 d . . . . .
O54 O 0.8456(19) 0.318(2) 0.037(3) 0.039(11) Uiso 1 1 d . . . . .
Na01 Na 0.659(2) -0.025(2) 0.103(3) 0.101(15) Uiso 1 1 d . . . . .
O50 O 0.5396(18) 0.118(2) 0.116(3) 0.038(11) Uiso 1 1 d . . . . .
O30 O 0.774(2) 0.377(2) 0.411(3) 0.046(12) Uiso 1 1 d . . . . .
O51 O 0.527(2) 0.316(2) 0.258(3) 0.052(14) Uiso 1 1 d . . . . .
O44 O 0.572(2) 0.196(3) -0.008(4) 0.053(14) Uiso 1 1 d . . . . .
O68 O 0.7240(18) 0.115(2) 0.098(3) 0.037(10) Uiso 1 1 d . . . . .
O15 O 0.974(2) 0.179(2) 0.253(3) 0.051(14) Uiso 1 1 d . . . . .
O21 O 0.922(2) 0.253(2) 0.368(3) 0.045(13) Uiso 1 1 d . . . . .
O16 O 0.963(2) 0.371(2) 0.396(3) 0.053(14) Uiso 1 1 d . . . . .
O38 O 0.725(2) 0.394(3) -0.145(3) 0.057(15) Uiso 1 1 d . . . . .
O43 O 0.656(2) 0.169(2) -0.082(3) 0.046(12) Uiso 1 1 d . . . . .
O25 O 0.8458(19) 0.158(2) 0.370(3) 0.039(11) Uiso 1 1 d . . . . .
O12 O 0.7146(19) 0.196(2) 0.587(3) 0.042(11) Uiso 1 1 d . . . . .
O22 O 0.870(2) 0.398(3) 0.468(3) 0.055(15) Uiso 1 1 d . . . . .
O19 O 0.763(2) 0.075(2) 0.368(3) 0.038(11) Uiso 1 1 d . . . . .
O17 O 0.783(2) 0.433(2) 0.550(3) 0.053(14) Uiso 1 1 d . . . . .
O02B O 0.702(2) 0.035(3) 0.223(4) 0.059(15) Uiso 1 1 d . . . . .
O35 O 0.797(2) 0.454(3) 0.281(3) 0.053(14) Uiso 1 1 d . . . . .
Na02 Na 0.493(3) 0.361(4) 0.386(5) 0.07(2) Uiso 0.5 1 d . . P . .
O64 O 0.714(2) 0.359(2) 0.262(3) 0.043(12) Uiso 1 1 d . . . . .
Na5 Na 0.806(2) 0.029(2) 0.084(3) 0.101(15) Uiso 1 1 d . . . . .
O02G O 0.825(2) 0.083(2) 0.900(3) 0.048(13) Uiso 1 1 d . . . . .
O1 O 0.7704(19) 0.094(2) 0.648(3) 0.037(10) Uiso 1 1 d . . . . .
O37 O 0.570(2) 0.445(3) -0.008(4) 0.062(16) Uiso 1 1 d . . . . .
O5 O 0.819(2) 0.201(2) 0.585(3) 0.051(13) Uiso 1 1 d . . . . .
O7 O 0.7239(19) 0.083(2) 0.509(3) 0.041(11) Uiso 1 1 d . . . . .
O02L O 0.788(2) 0.100(2) 0.774(3) 0.040(11) Uiso 1 1 d . . . . .
Na2 Na 0.845(2) 0.514(3) 0.403(3) 0.046(13) Uiso 0.5 1 d . . P . .
O14 O 0.8133(18) 0.0028(17) 0.258(2) 0.026(9) Uiso 1 1 d . . . . .
O45 O 0.558(2) 0.367(3) 0.108(3) 0.052(14) Uiso 1 1 d . . . . .
O66 O 0.811(2) 0.209(2) 0.104(3) 0.045(12) Uiso 1 1 d . . . . .
Na3 Na 0.4870(19) 0.281(2) 0.041(3) 0.095(13) Uiso 1 1 d . . . . .
O27 O 0.754(2) 0.187(2) 0.455(3) 0.043(12) Uiso 1 1 d . . . . .
O3 O 0.9125(19) 0.238(2) 0.649(3) 0.044(11) Uiso 1 1 d . . . . .
Na6 Na 1.207(7) 0.203(9) 0.272(11) 0.21(7) Uiso 0.5 1 d . . P . .
O2 O 0.927(2) 0.045(2) 0.511(3) 0.049(13) Uiso 1 1 d . . . . .
Na8 Na 0.573(3) 0.232(3) 0.394(4) 0.057(17) Uiso 0.5 1 d . . P . .
O46 O 0.637(2) 0.457(3) 0.119(3) 0.055(15) Uiso 1 1 d . . . . .
O02Y O 0.413(3) 0.146(3) 0.054(4) 0.08(2) Uiso 1 1 d . . . . .
O02Z O 0.744(4) 0.204(4) 0.812(6) 0.12(3) Uiso 1 1 d . . . . .
O030 O 1.010(3) 0.138(3) 0.112(4) 0.059(16) Uiso 1 1 d . . . . .
O18 O 0.644(3) 0.284(3) 0.543(4) 0.075(19) Uiso 1 1 d . . . . .
O032 O 0.540(3) 0.573(3) 0.048(4) 0.074(19) Uiso 1 1 d . . . . .
O033 O 0.716(3) 0.392(3) 0.722(4) 0.073(19) Uiso 1 1 d . . . . .
O13 O 0.654(2) 0.055(2) 0.394(3) 0.042(12) Uiso 1 1 d . . . . .
O035 O 0.925(4) 0.409(5) 0.206(6) 0.14(4) Uiso 1 1 d . . . . .
Na9 Na 1.019(4) 0.238(5) 0.449(6) 0.10(3) Uiso 0.5 1 d . . P . .
Na10 Na 0.762(3) 0.285(3) 0.679(4) 0.063(17) Uiso 0.5 1 d . . P . .
O038 O 0.890(4) 0.100(4) 0.104(5) 0.12(3) Uiso 1 1 d . . . . .
Na03 Na 0.600(3) 0.426(3) 0.384(4) 0.061(16) Uiso 0.5 1 d . . P . .
Na11 Na 0.497(3) 0.120(4) -0.059(4) 0.076(19) Uiso 0.5 1 d . . P . .
Na12 Na 1.020(3) 0.303(4) 0.283(4) 0.077(19) Uiso 0.5 1 d . . P . .
O03C O 1.000000 0.500000 0.558(5) 0.06(2) Uiso 1 2 d S . P . .
O36 O 0.582(2) 0.247(3) -0.136(4) 0.067(16) Uiso 1 1 d . . . . .
O3AA O 0.708(4) 0.048(4) 0.807(6) 0.12(3) Uiso 1 1 d . . . . .
O0BA O 0.919(2) 0.254(2) -0.127(3) 0.055(13) Uiso 1 1 d . . . . .
O2AA O 1.071(4) 0.159(5) 0.308(6) 0.05(2) Uiso 0.5 1 d . . P . .
O8AA O 0.792(4) 0.432(4) 0.698(6) 0.12(3) Uiso 1 1 d . . . . .
O49 O 0.7115(19) 0.057(2) -0.039(3) 0.044(12) Uiso 1 1 d . . . . .
O2BA O 0.582(3) 0.026(3) -0.064(4) 0.09(2) Uiso 1 1 d . . . . .
Na1B Na 1.045(3) 0.027(4) 0.142(5) 0.08(2) Uiso 0.5 1 d . . P . .
O9AA O 0.804(3) -0.038(3) 0.589(4) 0.08(2) Uiso 1 1 d . . . . .
Na3B Na 0.841(5) 0.306(6) -0.204(8) 0.06(3) Uiso 0.25 1 d . . P . .
O7AA O 0.539(5) 0.419(5) 0.553(7) 0.06(3) Uiso 0.5 1 d . . P . .
O5BA O 1.148(6) 0.316(7) 0.303(9) 0.09(4) Uiso 0.5 1 d . . P . .
O4BA O 0.884(4) 0.385(5) 0.705(6) 0.06(3) Uiso 0.5 1 d . . P . .
O1AA O 1.066(3) 0.168(3) 0.535(4) 0.08(2) Uiso 1 1 d . . . . .
Na0A Na 0.544(4) 0.506(4) 0.208(5) 0.10(3) Uiso 0.5 1 d . . P . .
Na6B Na 1.107(3) 0.408(4) 0.315(5) 0.09(2) Uiso 0.5 1 d . . P . .
Na6A Na 1.021(3) 0.435(3) 0.477(4) 0.072(18) Uiso 0.5 1 d . . P . .
Na7B Na 0.477(5) 0.015(7) 0.074(8) 0.07(4) Uiso 0.25 1 d . . P . .
O8BA O 0.495(3) 0.161(4) -0.166(4) 0.09(2) Uiso 1 1 d . . . . .
Na5A Na 0.860(3) 0.038(4) 0.643(4) 0.077(19) Uiso 0.5 1 d . . P . .
O6 O 0.8245(19) 0.097(2) 0.509(3) 0.037(10) Uiso 1 1 d . . . . .
O71 O 1.082(4) 0.370(5) 0.440(7) 0.15(4) Uiso 1 1 d . . . . .
O70 O 1.004(5) 0.359(6) 0.593(7) 0.17(5) Uiso 1 1 d . . . . .
O82 O 1.060(5) 0.488(6) 0.299(7) 0.16(4) Uiso 1 1 d . . . . .
O72 O 0.870(5) 0.118(6) 0.714(7) 0.17(4) Uiso 1 1 d . . . . .
O73 O 0.524(4) 0.460(5) 0.442(6) 0.05(2) Uiso 0.5 1 d . . P . .
Na73 Na 0.573(3) 0.085(4) 0.278(5) 0.08(2) Uiso 0.5 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W7 O33 1.81(5) . ?
W7 O8 2.00(5) . ?
W7 O20 1.90(5) . ?
W7 O25 2.19(5) . ?
W7 O19 1.91(5) . ?
W7 O14 1.74(4) . ?
W14 O58 1.90(4) . ?
W14 O60 2.17(4) . ?
W14 O53 1.76(5) . ?
W14 O65 1.82(5) . ?
W14 O47 2.00(7) . ?
W14 O54 2.01(5) . ?
W16 O67 1.94(4) . ?
W16 O61 2.17(4) . ?
W16 O55 1.98(5) . ?
W16 O68 1.82(5) . ?
W16 O43 2.07(5) . ?
W16 O49 1.71(5) . ?
W13 O58 2.00(5) . ?
W13 O52 1.72(4) . ?
W13 O57 1.95(5) . ?
W13 O59 2.25(5) . ?
W13 O64 1.84(5) . ?
W13 O46 2.01(6) . ?
W8 O24 1.89(6) . ?
W8 O32 1.83(4) . ?
W8 O19 1.95(5) . ?
W8 O7 2.03(5) . ?
W8 O27 2.21(5) . ?
W8 O13 1.78(5) . ?
W15 O60 2.16(4) . ?
W15 O42 2.04(5) . ?
W15 O55 1.86(5) . ?
W15 O48 1.77(5) . ?
W15 O54 2.02(5) . ?
W15 O66 1.84(5) . ?
W4 O11 2.10(6) . ?
W4 O26 2.17(5) . ?
W4 O23 1.88(6) . ?
W4 O30 1.73(5) . ?
W4 O22 2.00(6) . ?
W4 O17 1.77(5) . ?
W6 O9 1.99(5) . ?
W6 O28 1.72(5) . ?
W6 O20 2.01(4) . ?
W6 O15 1.76(6) . ?
W6 O21 1.94(5) . ?
W6 O25 2.22(5) . ?
W11 O41 1.97(5) . ?
W11 O60 2.19(5) . ?
W11 O39 1.93(4) . ?
W11 O42 1.89(5) . ?
W11 O47 1.94(7) . ?
W11 O38 1.72(6) . ?
W5 O29 1.77(5) . ?
W5 O10 2.03(5) . ?
W5 O26 2.18(5) . ?
W5 O21 1.86(5) . ?
W5 O16 1.70(6) . ?
W5 O22 1.98(6) . ?
W2 O4 1.89(4) . ?
W2 O8 1.92(5) . ?
W2 O9 1.93(5) . ?
W2 O25 2.31(5) . ?
W2 O2 1.75(5) . ?
W2 O6 1.94(5) . ?
W18 O57 2.01(5) . ?
W18 O56 1.86(5) . ?
W18 O63 1.83(5) . ?
W18 O59 2.10(5) . ?
W18 O51 1.80(6) . ?
W18 O45 2.13(6) . ?
W3 O12 1.93(5) . ?
W3 O1 1.76(5) . ?
W3 O5 1.90(5) . ?
W3 O7 1.91(5) . ?
W3 O27 2.22(5) . ?
W3 O6 1.92(5) . ?
W1 O4 1.94(4) . ?
W1 O11 1.92(6) . ?
W1 O10 1.95(5) . ?
W1 O26 2.17(5) . ?
W1 O5 1.95(5) . ?
W1 O3 1.76(5) . ?
W12 O39 1.90(4) . ?
W12 O61 2.24(5) . ?
W12 O40 1.92(5) . ?
W12 O44 1.79(6) . ?
W12 O43 1.82(5) . ?
W12 O36 1.68(6) . ?
W9 O31 1.76(5) . ?
W9 O24 2.07(6) . ?
W9 O23 1.94(6) . ?
W9 O12 2.06(5) . ?
W9 O27 2.20(5) . ?
W9 O18 1.67(7) . ?
W17 O67 1.93(4) . ?
W17 O61 2.16(5) . ?
W17 O56 1.96(5) . ?
W17 O69 1.83(5) . ?
W17 O50 1.69(5) . ?
W17 O44 2.11(6) . ?
W10 O41 1.92(5) . ?
W10 O40 1.92(5) . ?
W10 O59 2.18(5) . ?
W10 O37 1.78(6) . ?
W10 O45 1.82(6) . ?
W10 O46 1.98(6) . ?
Co3 O62 1.84(5) . ?
Co3 O60 1.94(5) . ?
Co3 O61 1.91(5) . ?
Co3 O59 1.94(5) . ?
Co2 O29 2.07(5) . ?
Co2 O65 2.19(5) . ?
Co2 O34 2.06(5) . ?
Co2 O30 2.17(5) . ?
Co2 O35 2.04(5) . ?
Co2 O64 2.08(6) . ?
Co1 O34 1.86(5) . ?
Co1 O26 1.93(5) . ?
Co1 O25 1.81(5) . ?
Co1 O27 1.86(5) . ?
Fe1 O31 2.07(5) . ?
Fe1 O62 2.01(5) . ?
Fe1 O32 2.14(4) . ?
Fe1 O34 2.01(5) . ?
Fe1 O63 2.02(5) . ?
Fe1 O64 2.14(5) . ?
Co4 O33 2.15(5) . ?
Co4 O62 2.04(4) . ?
Co4 O32 2.11(4) . ?
Co4 O69 2.02(5) . ?
Co4 O68 2.04(5) . ?
Co4 O02B 2.10(6) . ?
Fe2 O33 2.15(5) . ?
Fe2 O62 1.99(5) . ?
Fe2 O28 2.07(5) . ?
Fe2 O65 2.10(5) . ?
Fe2 O34 2.02(6) . ?
Fe2 O66 1.91(5) . ?
Na7 O58 2.38(5) . ?
Na7 O41 2.42(5) . ?
Na7 O47 2.62(7) . ?
Na7 Na01 4.19(6) 3_655 ?
Na7 Na5 2.34(6) 3_655 ?
Na7 O02G 2.38(6) 3_656 ?
Na7 O46 2.55(6) . ?
Na7 O49 2.39(6) 3_655 ?
Na1 O8 2.54(5) . ?
Na1 O01E 2.50(6) . ?
Na1 O19 2.47(6) . ?
Na1 O17 2.23(6) 3_646 ?
Na1 O7 2.52(5) . ?
Na1 O9AA 2.34(8) . ?
Na1 O6 2.47(5) . ?
Na4 O48 2.53(6) . ?
Na4 O01M 2.57(7) . ?
Na4 Na3 2.26(6) 4 ?
Na4 O030 2.42(7) . ?
Na4 O032 2.51(8) 3_645 ?
Na4 O038 2.14(10) . ?
O67 Na01 2.92(6) . ?
O52 Na5A 2.55(9) 3_656 ?
O42 Na3B 2.64(14) . ?
O57 Na03 2.55(8) . ?
O57 Na0A 3.01(11) . ?
O11 Na10 2.75(9) . ?
O24 Na8 2.87(9) . ?
O10 Na9 2.78(12) . ?
O47 Na01 2.77(9) 3_655 ?
O56 Na3 2.97(7) . ?
O69 Na73 2.61(10) . ?
O63 Na8 2.78(8) . ?
O23 Na10 2.75(9) . ?
Na01 O02B 2.71(8) . ?
Na01 Na5 4.00(8) . ?
Na01 Na3B 3.99(14) 3_645 ?
Na01 Na7B 3.59(15) 2_655 ?
O50 Na7B 2.81(15) . ?
O50 Na7B 2.93(15) 2_655 ?
O51 Na02 2.61(10) . ?
O44 Na3 2.97(8) . ?
O44 Na11 2.68(10) . ?
O68 Na5 2.80(7) . ?
O15 Na12 2.92(9) . ?
O21 Na9 2.93(12) . ?
O16 Na12 2.88(9) . ?
O16 Na6A 2.49(9) . ?
O12 Na10 2.77(9) . ?
O22 Na2 2.78(8) . ?
O35 Na2 2.79(8) . ?
Na02 O3 3.02(9) 4_456 ?
Na02 Na8 3.41(10) . ?
Na02 Na9 3.65(13) 4_456 ?
Na02 Na03 3.10(11) . ?
Na02 O1AA 2.44(11) 4_456 ?
Na02 Na5A 4.10(11) 4_456 ?
Na02 O73 2.43(12) . ?
Na5 O038 2.68(11) . ?
Na5 Na1B 4.19(10) 2_755 ?
O1 Na5A 2.62(9) . ?
O37 Na1B 2.53(11) 4_455 ?
O5 Na10 2.85(9) . ?
O7 Na2 2.77(8) 3_646 ?
Na2 Na6B 2.60(10) 2_765 ?
Na2 Na6A 3.89(10) 2_765 ?
O45 Na3 2.84(7) . ?
Na3 Na11 3.82(9) . ?
Na3 O0BA 2.44(7) 4_455 ?
Na6 O02Z 2.7(2) 4_556 ?
Na6 O033 2.0(2) 4_556 ?
Na6 Na10 1.7(2) 4_556 ?
Na6 Na3B 3.7(2) 4 ?
Na6 O5BA 2.9(2) . ?
O2 Na5A 2.92(9) . ?
Na8 Na9 3.16(13) 4_456 ?
Na8 Na03 4.14(9) . ?
Na8 O1AA 2.44(10) 4_456 ?
Na8 O70 2.62(14) 4_456 ?
Na8 Na73 3.71(11) . ?
O02Y Na11 3.02(11) . ?
O02Z Na10 2.95(10) . ?
O030 Na1B 2.54(10) . ?
O033 Na10 2.66(10) . ?
O13 Na73 3.00(10) . ?
Na9 Na12 3.25(13) . ?
Na9 O1AA 2.43(13) . ?
Na9 Na6A 4.16(12) . ?
Na10 Na3B 2.96(16) 1_556 ?
Na03 O9AA 2.66(10) 3_656 ?
Na03 O1AA 2.62(10) 4_456 ?
Na03 Na0A 3.82(12) . ?
Na03 Na5A 2.62(10) 3_656 ?
Na03 O73 2.36(12) . ?
Na11 O2BA 2.98(10) . ?
Na11 Na7B 3.76(16) 2_655 ?
Na11 Na7B 3.27(16) . ?
Na11 O8BA 2.09(11) . ?
Na12 Na6B 3.21(11) . ?
Na12 O8BA 2.31(11) 4 ?
O03C Na6A 2.06(9) . ?
O03C Na6A 2.06(9) 2_765 ?
O0BA Na3B 2.68(15) . ?
Na1B Na1B 2.62(16) 2_755 ?
O9AA Na5A 2.37(11) . ?
Na3B O4BA 2.59(17) 1_554 ?
O5BA Na6B 2.22(17) . ?
Na0A Na0A 2.33(19) 2_665 ?
Na0A Na5A 3.70(12) 3_656 ?
Na6B Na6A 3.69(11) . ?
Na6B O71 2.45(14) . ?
Na6B O82 2.10(14) . ?
Na6A Na6A 2.96(14) 2_765 ?
Na6A O71 2.19(14) . ?
Na6A O70 2.64(14) . ?
Na7B Na7B 1.4(3) 2_655 ?
Na5A O6 2.82(9) . ?
Na5A O72 2.12(14) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O33 W7 O8 162(2) . . ?
O33 W7 O20 94(2) . . ?
O33 W7 O25 88(2) . . ?
O33 W7 O19 90(2) . . ?
O8 W7 O25 74.6(17) . . ?
O20 W7 O8 85.3(19) . . ?
O20 W7 O25 75.7(18) . . ?
O20 W7 O19 160(2) . . ?
O19 W7 O8 84(2) . . ?
O19 W7 O25 84.7(19) . . ?
O14 W7 O33 105(2) . . ?
O14 W7 O8 92.5(18) . . ?
O14 W7 O20 98.5(19) . . ?
O14 W7 O25 166.2(19) . . ?
O14 W7 O19 99(2) . . ?
O58 W14 O60 87.3(17) . . ?
O58 W14 O47 86(2) . . ?
O58 W14 O54 161.5(19) . . ?
O53 W14 O58 102(2) . . ?
O53 W14 O60 164(2) . . ?
O53 W14 O65 102(2) . . ?
O53 W14 O47 95(2) . . ?
O53 W14 O54 94(2) . . ?
O65 W14 O58 96(2) . . ?
O65 W14 O60 91(2) . . ?
O65 W14 O47 162(2) . . ?
O65 W14 O54 90(2) . . ?
O47 W14 O60 72(2) . . ?
O47 W14 O54 84(2) . . ?
O54 W14 O60 74.9(18) . . ?
O67 W16 O61 73.3(16) . . ?
O67 W16 O55 160.3(17) . . ?
O67 W16 O43 84.3(19) . . ?
O55 W16 O61 87.6(18) . . ?
O55 W16 O43 85(2) . . ?
O68 W16 O67 90.9(19) . . ?
O68 W16 O61 88.6(19) . . ?
O68 W16 O55 93(2) . . ?
O68 W16 O43 160(2) . . ?
O43 W16 O61 71.6(19) . . ?
O49 W16 O67 94(2) . . ?
O49 W16 O61 163(2) . . ?
O49 W16 O55 104(2) . . ?
O49 W16 O68 102(2) . . ?
O49 W16 O43 98(2) . . ?
O58 W13 O59 87.7(18) . . ?
O58 W13 O46 87(2) . . ?
O52 W13 O58 100(2) . . ?
O52 W13 O57 97(2) . . ?
O52 W13 O59 163(2) . . ?
O52 W13 O64 103(2) . . ?
O52 W13 O46 91(2) . . ?
O57 W13 O58 161.6(19) . . ?
O57 W13 O59 74.2(19) . . ?
O57 W13 O46 85(2) . . ?
O64 W13 O58 89(2) . . ?
O64 W13 O57 94(2) . . ?
O64 W13 O59 91(2) . . ?
O64 W13 O46 165(2) . . ?
O46 W13 O59 74(2) . . ?
O24 W8 O19 161(2) . . ?
O24 W8 O7 84(2) . . ?
O24 W8 O27 76(2) . . ?
O32 W8 O24 95(2) . . ?
O32 W8 O19 89(2) . . ?
O32 W8 O7 161.0(19) . . ?
O32 W8 O27 88.4(19) . . ?
O19 W8 O7 86(2) . . ?
O19 W8 O27 85.6(19) . . ?
O7 W8 O27 72.8(19) . . ?
O13 W8 O24 94(2) . . ?
O13 W8 O32 104(2) . . ?
O13 W8 O19 103(2) . . ?
O13 W8 O7 95(2) . . ?
O13 W8 O27 165(2) . . ?
O42 W15 O60 71.3(18) . . ?
O55 W15 O60 88.5(18) . . ?
O55 W15 O42 83.1(19) . . ?
O55 W15 O54 161.8(19) . . ?
O48 W15 O60 162.4(19) . . ?
O48 W15 O42 96(2) . . ?
O48 W15 O55 102(2) . . ?
O48 W15 O54 92(2) . . ?
O48 W15 O66 104(2) . . ?
O54 W15 O60 75.1(18) . . ?
O54 W15 O42 84.1(18) . . ?
O66 W15 O60 88(2) . . ?
O66 W15 O42 160(2) . . ?
O66 W15 O55 98(2) . . ?
O66 W15 O54 90(2) . . ?
O11 W4 O26 73(2) . . ?
O23 W4 O11 85(2) . . ?
O23 W4 O26 87(2) . . ?
O23 W4 O22 162(2) . . ?
O30 W4 O11 165(2) . . ?
O30 W4 O26 93(2) . . ?
O30 W4 O23 92(2) . . ?
O30 W4 O22 94(2) . . ?
O30 W4 O17 103(2) . . ?
O22 W4 O11 84(2) . . ?
O22 W4 O26 76(2) . . ?
O17 W4 O11 92(2) . . ?
O17 W4 O26 163(2) . . ?
O17 W4 O23 100(2) . . ?
O17 W4 O22 95(2) . . ?
O9 W6 O20 82.4(19) . . ?
O9 W6 O25 75.3(19) . . ?
O28 W6 O9 161(2) . . ?
O28 W6 O20 92(2) . . ?
O28 W6 O15 105(3) . . ?
O28 W6 O21 90(2) . . ?
O28 W6 O25 86(2) . . ?
O20 W6 O25 73.1(18) . . ?
O15 W6 O9 94(2) . . ?
O15 W6 O20 98(2) . . ?
O15 W6 O21 103(2) . . ?
O15 W6 O25 166(2) . . ?
O21 W6 O9 88(2) . . ?
O21 W6 O20 158(2) . . ?
O21 W6 O25 85(2) . . ?
O41 W11 O60 88.4(18) . . ?
O39 W11 O41 84.3(18) . . ?
O39 W11 O60 87.1(18) . . ?
O39 W11 O47 159(2) . . ?
O42 W11 O41 160.8(19) . . ?
O42 W11 O60 73.2(19) . . ?
O42 W11 O39 89.1(19) . . ?
O42 W11 O47 90(2) . . ?
O47 W11 O41 89(2) . . ?
O47 W11 O60 72(2) . . ?
O38 W11 O41 97(2) . . ?
O38 W11 O60 171(2) . . ?
O38 W11 O39 100(2) . . ?
O38 W11 O42 102(2) . . ?
O38 W11 O47 100(3) . . ?
O29 W5 O10 163(2) . . ?
O29 W5 O26 91(2) . . ?
O29 W5 O21 91(2) . . ?
O29 W5 O22 92(2) . . ?
O10 W5 O26 72.2(19) . . ?
O21 W5 O10 85(2) . . ?
O21 W5 O26 83(2) . . ?
O21 W5 O22 159(2) . . ?
O16 W5 O29 109(3) . . ?
O16 W5 O10 88(2) . . ?
O16 W5 O26 160(2) . . ?
O16 W5 O21 101(2) . . ?
O16 W5 O22 98(3) . . ?
O22 W5 O10 86(2) . . ?
O22 W5 O26 76(2) . . ?
O4 W2 O8 159.0(19) . . ?
O4 W2 O9 89.9(19) . . ?
O4 W2 O25 87.6(18) . . ?
O4 W2 O6 83.8(19) . . ?
O8 W2 O9 93(2) . . ?
O8 W2 O25 73.3(18) . . ?
O8 W2 O6 85(2) . . ?
O9 W2 O25 74.4(19) . . ?
O9 W2 O6 157(2) . . ?
O2 W2 O4 100(2) . . ?
O2 W2 O8 100(2) . . ?
O2 W2 O9 100(2) . . ?
O2 W2 O25 170(2) . . ?
O2 W2 O6 103(2) . . ?
O6 W2 O25 83.6(19) . . ?
O57 W18 O59 77(2) . . ?
O57 W18 O45 88(2) . . ?
O56 W18 O57 163(2) . . ?
O56 W18 O59 87(2) . . ?
O56 W18 O45 85(2) . . ?
O63 W18 O57 88.4(19) . . ?
O63 W18 O56 94(2) . . ?
O63 W18 O59 91(2) . . ?
O63 W18 O45 162(2) . . ?
O59 W18 O45 71(2) . . ?
O51 W18 O57 93(2) . . ?
O51 W18 O56 103(2) . . ?
O51 W18 O63 100(2) . . ?
O51 W18 O59 165(2) . . ?
O51 W18 O45 98(2) . . ?
O12 W3 O27 76(2) . . ?
O1 W3 O12 98(2) . . ?
O1 W3 O5 101(2) . . ?
O1 W3 O7 97(2) . . ?
O1 W3 O27 170(2) . . ?
O1 W3 O6 101(2) . . ?
O5 W3 O12 91(2) . . ?
O5 W3 O7 161(2) . . ?
O5 W3 O27 88(2) . . ?
O5 W3 O6 84(2) . . ?
O7 W3 O12 92(2) . . ?
O7 W3 O27 74.6(19) . . ?
O7 W3 O6 87(2) . . ?
O6 W3 O12 160(2) . . ?
O6 W3 O27 85(2) . . ?
O4 W1 O10 88.5(19) . . ?
O4 W1 O26 87.6(18) . . ?
O4 W1 O5 81(2) . . ?
O11 W1 O4 161(2) . . ?
O11 W1 O10 96(2) . . ?
O11 W1 O26 76(2) . . ?
O11 W1 O5 89(2) . . ?
O10 W1 O26 74(2) . . ?
O5 W1 O10 159(2) . . ?
O5 W1 O26 87(2) . . ?
O3 W1 O4 97(2) . . ?
O3 W1 O11 100(2) . . ?
O3 W1 O10 102(2) . . ?
O3 W1 O26 173.9(19) . . ?
O3 W1 O5 97(2) . . ?
O39 W12 O61 85.0(18) . . ?
O39 W12 O40 83(2) . . ?
O40 W12 O61 85.6(19) . . ?
O44 W12 O39 158(2) . . ?
O44 W12 O61 74(2) . . ?
O44 W12 O40 89(2) . . ?
O44 W12 O43 94(2) . . ?
O43 W12 O39 86(2) . . ?
O43 W12 O61 74(2) . . ?
O43 W12 O40 158(2) . . ?
O36 W12 O39 107(3) . . ?
O36 W12 O61 167(2) . . ?
O36 W12 O40 100(3) . . ?
O36 W12 O44 94(3) . . ?
O36 W12 O43 102(3) . . ?
O31 W9 O24 92(2) . . ?
O31 W9 O23 95(2) . . ?
O31 W9 O12 164(2) . . ?
O31 W9 O27 90(2) . . ?
O24 W9 O27 73(2) . . ?
O23 W9 O24 159(2) . . ?
O23 W9 O12 86(2) . . ?
O23 W9 O27 87(2) . . ?
O12 W9 O24 82(2) . . ?
O12 W9 O27 74(2) . . ?
O18 W9 O31 102(3) . . ?
O18 W9 O24 98(3) . . ?
O18 W9 O23 101(3) . . ?
O18 W9 O12 93(3) . . ?
O18 W9 O27 165(3) . . ?
O67 W17 O61 73.9(17) . . ?
O67 W17 O56 159.2(19) . . ?
O67 W17 O44 83(2) . . ?
O56 W17 O61 85.6(19) . . ?
O56 W17 O44 87(2) . . ?
O69 W17 O67 91.0(18) . . ?
O69 W17 O61 90.1(19) . . ?
O69 W17 O56 93(2) . . ?
O69 W17 O44 161(2) . . ?
O50 W17 O67 99(2) . . ?
O50 W17 O61 166(2) . . ?
O50 W17 O56 100(2) . . ?
O50 W17 O69 102(2) . . ?
O50 W17 O44 97(2) . . ?
O44 W17 O61 71(2) . . ?
O41 W10 O59 89(2) . . ?
O41 W10 O46 89(2) . . ?
O40 W10 O41 84(2) . . ?
O40 W10 O59 85(2) . . ?
O40 W10 O46 160(2) . . ?
O37 W10 O41 102(3) . . ?
O37 W10 O40 100(2) . . ?
O37 W10 O59 168(3) . . ?
O37 W10 O45 95(3) . . ?
O37 W10 O46 99(3) . . ?
O45 W10 O41 162(2) . . ?
O45 W10 O40 86(2) . . ?
O45 W10 O59 75(2) . . ?
O45 W10 O46 95(2) . . ?
O46 W10 O59 76(2) . . ?
O62 Co3 O60 112(2) . . ?
O62 Co3 O61 112(2) . . ?
O62 Co3 O59 114(2) . . ?
O61 Co3 O60 107(2) . . ?
O61 Co3 O59 103(2) . . ?
O59 Co3 O60 107(2) . . ?
O29 Co2 O65 93(2) . . ?
O29 Co2 O30 86(2) . . ?
O29 Co2 O64 175.9(19) . . ?
O34 Co2 O29 92(2) . . ?
O34 Co2 O65 82(2) . . ?
O34 Co2 O30 91(2) . . ?
O34 Co2 O64 84(2) . . ?
O30 Co2 O65 173.2(18) . . ?
O35 Co2 O29 93(2) . . ?
O35 Co2 O65 100(2) . . ?
O35 Co2 O34 175(2) . . ?
O35 Co2 O30 86(2) . . ?
O35 Co2 O64 92(2) . . ?
O64 Co2 O65 86(2) . . ?
O64 Co2 O30 94(2) . . ?
O34 Co1 O26 114(2) . . ?
O34 Co1 O27 112(2) . . ?
O25 Co1 O34 110(2) . . ?
O25 Co1 O26 108(2) . . ?
O25 Co1 O27 104(2) . . ?
O27 Co1 O26 107(2) . . ?
O31 Fe1 O32 89.6(17) . . ?
O31 Fe1 O64 94.6(19) . . ?
O62 Fe1 O31 170(2) . . ?
O62 Fe1 O32 82.3(17) . . ?
O62 Fe1 O34 81(2) . . ?
O62 Fe1 O63 94(2) . . ?
O62 Fe1 O64 93(2) . . ?
O34 Fe1 O31 93(2) . . ?
O34 Fe1 O32 90.5(19) . . ?
O34 Fe1 O63 172(2) . . ?
O34 Fe1 O64 83(2) . . ?
O63 Fe1 O31 93(2) . . ?
O63 Fe1 O32 94.7(17) . . ?
O63 Fe1 O64 91(2) . . ?
O64 Fe1 O32 173(2) . . ?
O62 Co4 O33 82.6(19) . . ?
O62 Co4 O32 82.2(18) . . ?
O62 Co4 O02B 174(2) . . ?
O32 Co4 O33 82.7(18) . . ?
O69 Co4 O33 176.6(18) . . ?
O69 Co4 O62 94.6(19) . . ?
O69 Co4 O32 94.8(18) . . ?
O69 Co4 O68 88.8(19) . . ?
O69 Co4 O02B 91(2) . . ?
O68 Co4 O33 93(2) . . ?
O68 Co4 O62 92.0(19) . . ?
O68 Co4 O32 173.4(18) . . ?
O68 Co4 O02B 86(2) . . ?
O02B Co4 O33 91(2) . . ?
O02B Co4 O32 99(2) . . ?
O62 Fe2 O33 83.8(19) . . ?
O62 Fe2 O28 167(2) . . ?
O62 Fe2 O65 94.7(19) . . ?
O62 Fe2 O34 81(2) . . ?
O28 Fe2 O33 88(2) . . ?
O28 Fe2 O65 93(2) . . ?
O65 Fe2 O33 177(2) . . ?
O34 Fe2 O33 92(2) . . ?
O34 Fe2 O28 89(2) . . ?
O34 Fe2 O65 85.1(19) . . ?
O66 Fe2 O33 94(2) . . ?
O66 Fe2 O62 93(2) . . ?
O66 Fe2 O28 98(2) . . ?
O66 Fe2 O65 89(2) . . ?
O66 Fe2 O34 171(2) . . ?
W14 Na7 Na01 66.4(8) . 3_655 ?
W13 Na7 W14 65.3(4) . . ?
W13 Na7 W11 93.2(5) . . ?
W13 Na7 Na01 131.7(10) . 3_655 ?
W11 Na7 W14 57.5(4) . . ?
W11 Na7 Na01 61.1(8) . 3_655 ?
W10 Na7 W14 93.5(5) . . ?
W10 Na7 W13 57.9(4) . . ?
W10 Na7 W11 66.6(4) . . ?
W10 Na7 Na01 126.9(9) . 3_655 ?
O58 Na7 W14 31.2(11) . . ?
O58 Na7 W13 34.4(11) . . ?
O58 Na7 W11 75.2(11) . . ?
O58 Na7 W10 77.5(12) . . ?
O58 Na7 O41 78.1(17) . . ?
O58 Na7 O47 64.0(19) . . ?
O58 Na7 Na01 97.3(15) . 3_655 ?
O58 Na7 O02G 108.8(19) . 3_656 ?
O58 Na7 O46 68.2(18) . . ?
O58 Na7 O49 97.7(19) . 3_655 ?
O41 Na7 W14 77.3(13) . . ?
O41 Na7 W13 77.1(13) . . ?
O41 Na7 W11 33.8(12) . . ?
O41 Na7 W10 33.3(12) . . ?
O41 Na7 O47 65.9(19) . . ?
O41 Na7 Na01 93.6(15) . 3_655 ?
O41 Na7 O46 67.0(18) . . ?
O47 Na7 W14 34.7(15) . . ?
O47 Na7 W13 95.3(16) . . ?
O47 Na7 W11 33.8(15) . . ?
O47 Na7 W10 95.8(15) . . ?
O47 Na7 Na01 40.3(16) . 3_655 ?
Na5 Na7 W14 129.1(16) 3_655 . ?
Na5 Na7 W13 151.4(17) 3_655 . ?
Na5 Na7 W11 80.3(14) 3_655 . ?
Na5 Na7 W10 94.4(16) 3_655 . ?
Na5 Na7 O58 155.5(19) 3_655 . ?
Na5 Na7 O41 82.5(19) 3_655 . ?
Na5 Na7 O47 94(2) 3_655 . ?
Na5 Na7 Na01 68.9(16) 3_655 3_655 ?
Na5 Na7 O02G 95(2) 3_655 3_656 ?
Na5 Na7 O46 117(2) 3_655 . ?
Na5 Na7 O49 90(2) 3_655 3_655 ?
O02G Na7 W14 133.1(17) 3_656 . ?
O02G Na7 W13 83.1(15) 3_656 . ?
O02G Na7 W11 163.4(18) 3_656 . ?
O02G Na7 W10 98.0(16) 3_656 . ?
O02G Na7 O41 130(2) 3_656 . ?
O02G Na7 O47 162(2) 3_656 . ?
O02G Na7 Na01 132.2(17) 3_656 3_655 ?
O02G Na7 O46 70.3(19) 3_656 . ?
O02G Na7 O49 83.7(19) 3_656 3_655 ?
O46 Na7 W14 96.7(14) . . ?
O46 Na7 W13 35.5(14) . . ?
O46 Na7 W11 97.4(14) . . ?
O46 Na7 W10 35.2(14) . . ?
O46 Na7 O47 118(2) . . ?
O46 Na7 Na01 157.3(16) . 3_655 ?
O49 Na7 W14 82.0(14) 3_655 . ?
O49 Na7 W13 118.0(16) 3_655 . ?
O49 Na7 W11 112.1(15) 3_655 . ?
O49 Na7 W10 175.1(16) 3_655 . ?
O49 Na7 O41 146(2) 3_655 . ?
O49 Na7 O47 81.6(19) 3_655 . ?
O49 Na7 Na01 52.9(15) 3_655 3_655 ?
O49 Na7 O46 143(2) 3_655 . ?
W7 Na1 W4 132.4(9) . 3_646 ?
W8 Na1 W7 64.4(5) . . ?
W8 Na1 W4 102.4(8) . 3_646 ?
W8 Na1 W2 92.2(6) . . ?
W2 Na1 W7 56.9(5) . . ?
W2 Na1 W4 165.2(10) . 3_646 ?
W3 Na1 W7 92.0(6) . . ?
W3 Na1 W8 57.6(4) . . ?
W3 Na1 W4 120.4(9) . 3_646 ?
W3 Na1 W2 65.6(5) . . ?
O8 Na1 W7 33.9(11) . . ?
O8 Na1 W8 93.1(13) . . ?
O8 Na1 W4 146.3(14) . 3_646 ?
O8 Na1 W2 32.8(11) . . ?
O8 Na1 W3 93.2(12) . . ?
O01E Na1 W7 77.2(14) . . ?
O01E Na1 W8 130.0(16) . . ?
O01E Na1 W4 80.2(14) . 3_646 ?
O01E Na1 W2 92.5(15) . . ?
O01E Na1 W3 157.9(17) . . ?
O01E Na1 O8 67.0(17) . . ?
O01E Na1 O7 164(2) . . ?
O19 Na1 W7 31.5(12) . . ?
O19 Na1 W8 33.2(12) . . ?
O19 Na1 W4 119.4(16) . 3_646 ?
O19 Na1 W2 74.6(13) . . ?
O19 Na1 W3 75.9(13) . . ?
O19 Na1 O8 63.1(17) . . ?
O19 Na1 O01E 102(2) . . ?
O19 Na1 O7 66.1(17) . . ?
O19 Na1 O6 75.1(17) . . ?
O17 Na1 W7 112.7(18) 3_646 . ?
O17 Na1 W8 84.0(16) 3_646 . ?
O17 Na1 W4 22.3(15) 3_646 3_646 ?
O17 Na1 W2 169.4(19) 3_646 . ?
O17 Na1 W3 119.6(18) 3_646 . ?
O17 Na1 O8 137(2) 3_646 . ?
O17 Na1 O01E 82(2) 3_646 . ?
O17 Na1 O19 97(2) 3_646 . ?
O17 Na1 O7 89(2) 3_646 . ?
O17 Na1 O9AA 96(3) 3_646 . ?
O17 Na1 O6 152(2) 3_646 . ?
O7 Na1 W7 94.4(13) . . ?
O7 Na1 W8 35.3(12) . . ?
O7 Na1 W4 96.4(14) . 3_646 ?
O7 Na1 W2 94.0(13) . . ?
O7 Na1 W3 33.1(12) . . ?
O7 Na1 O8 112.9(17) . . ?
O9AA Na1 W7 150(2) . . ?
O9AA Na1 W8 130(2) . . ?
O9AA Na1 W4 75(2) . 3_646 ?
O9AA Na1 W2 94(2) . . ?
O9AA Na1 W3 80.2(19) . . ?
O9AA Na1 O8 117(3) . . ?
O9AA Na1 O01E 100(2) . . ?
O9AA Na1 O19 156(2) . . ?
O9AA Na1 O7 95(2) . . ?
O9AA Na1 O6 84(2) . . ?
O6 Na1 W7 74.4(13) . . ?
O6 Na1 W8 75.1(13) . . ?
O6 Na1 W4 149.9(16) . 3_646 ?
O6 Na1 W2 32.7(12) . . ?
O6 Na1 W3 33.1(12) . . ?
O6 Na1 O8 63.0(17) . . ?
O6 Na1 O01E 125(2) . . ?
O6 Na1 O7 63.9(17) . . ?
O48 Na4 O01M 87(2) . . ?
Na3 Na4 O48 87(2) 4 . ?
Na3 Na4 O01M 87(2) 4 . ?
Na3 Na4 O030 89(2) 4 . ?
Na3 Na4 O032 83(2) 4 3_645 ?
O030 Na4 O48 172(2) . . ?
O030 Na4 O01M 86(2) . . ?
O030 Na4 O032 88(2) . 3_645 ?
O032 Na4 O48 98(2) 3_645 . ?
O032 Na4 O01M 168(3) 3_645 . ?
O038 Na4 O48 95(3) . . ?
O038 Na4 O01M 101(3) . . ?
O038 Na4 Na3 172(3) . 4 ?
O038 Na4 O030 90(3) . . ?
O038 Na4 O032 90(3) . 3_645 ?
W14 O58 W13 147(2) . . ?
W14 O58 Na7 108(2) . . ?
W13 O58 Na7 103.1(19) . . ?
W2 O4 W1 156(3) . . ?
W11 O41 Na7 103(2) . . ?
W10 O41 W11 151(2) . . ?
W10 O41 Na7 103(2) . . ?
W7 O33 Co4 129(3) . . ?
W7 O33 Fe2 136(3) . . ?
Fe2 O33 Co4 92.2(19) . . ?
W7 O8 Na1 101.0(19) . . ?
W2 O8 W7 116(2) . . ?
W2 O8 Na1 102(2) . . ?
W2 O9 W6 116(2) . . ?
W9 O31 Fe1 141(3) . . ?
Co3 O62 Fe1 117(2) . . ?
Co3 O62 Co4 118(2) . . ?
Co3 O62 Fe2 118(3) . . ?
Fe1 O62 Co4 100(2) . . ?
Fe2 O62 Fe1 100(2) . . ?
Fe2 O62 Co4 100(2) . . ?
W14 O60 W11 99.6(17) . . ?
W15 O60 W14 98.9(19) . . ?
W15 O60 W11 99.9(19) . . ?
Co3 O60 W14 117(2) . . ?
Co3 O60 W15 115(2) . . ?
Co3 O60 W11 122(2) . . ?
W16 O67 Na01 99.7(19) . . ?
W17 O67 W16 113.6(19) . . ?
W17 O67 Na01 120(2) . . ?
W13 O52 Na5A 132(3) . 3_656 ?
W12 O39 W11 156(3) . . ?
W16 O61 W12 97.2(19) . . ?
W17 O61 W16 97.1(17) . . ?
W17 O61 W12 98.1(19) . . ?
Co3 O61 W16 117(2) . . ?
Co3 O61 W12 123(2) . . ?
Co3 O61 W17 119(2) . . ?
W15 O42 Na3B 121(3) . . ?
W11 O42 W15 116(2) . . ?
W11 O42 Na3B 121(3) . . ?
W6 O28 Fe2 144(3) . . ?
W5 O29 Co2 142(3) . . ?
W13 O57 W18 111(2) . . ?
W13 O57 Na03 116(3) . . ?
W13 O57 Na0A 105(3) . . ?
W18 O57 Na03 123(3) . . ?
W18 O57 Na0A 111(3) . . ?
Na03 O57 Na0A 86(3) . . ?
W4 O11 Na10 101(3) . . ?
W1 O11 W4 111(3) . . ?
W1 O11 Na10 106(3) . . ?
W15 O55 W16 146(3) . . ?
W14 O65 Co2 124(2) . . ?
W14 O65 Fe2 137(3) . . ?
Fe2 O65 Co2 92.8(19) . . ?
W8 O24 W9 112(3) . . ?
W8 O24 Na8 121(3) . . ?
W9 O24 Na8 94(2) . . ?
W7 O20 W6 114(2) . . ?
W8 O32 Fe1 136(2) . . ?
W8 O32 Co4 128(2) . . ?
Co4 O32 Fe1 93.7(17) . . ?
W15 O48 Na4 121(3) . . ?
W5 O10 Na9 97(3) . . ?
W1 O10 W5 114(2) . . ?
W1 O10 Na9 122(3) . . ?
W14 O47 Na7 97(3) . . ?
W14 O47 Na01 125(3) . 3_655 ?
W11 O47 W14 116(3) . . ?
W11 O47 Na7 97(3) . . ?
W11 O47 Na01 112(3) . 3_655 ?
Na7 O47 Na01 102(2) . 3_655 ?
W10 O40 W12 156(3) . . ?
W18 O56 W17 152(3) . . ?
W18 O56 Na3 105(2) . . ?
W17 O56 Na3 103(2) . . ?
Co1 O34 Co2 118(3) . . ?
Co1 O34 Fe1 119(3) . . ?
Co1 O34 Fe2 119(3) . . ?
Fe1 O34 Co2 98(2) . . ?
Fe1 O34 Fe2 99(2) . . ?
Fe2 O34 Co2 100(2) . . ?
W4 O26 W5 96.2(17) . . ?
W4 O26 W1 100(2) . . ?
W1 O26 W5 100(2) . . ?
Co1 O26 W4 116(2) . . ?
Co1 O26 W5 116(2) . . ?
Co1 O26 W1 124(2) . . ?
W17 O69 Co4 139(3) . . ?
W17 O69 Na73 107(3) . . ?
Co4 O69 Na73 113(3) . . ?
W18 O63 Fe1 140(3) . . ?
W18 O63 Na8 111(3) . . ?
Fe1 O63 Na8 106(2) . . ?
W18 O59 W13 97(2) . . ?
W18 O59 W10 101(2) . . ?
W10 O59 W13 96.9(19) . . ?
Co3 O59 W13 114(3) . . ?
Co3 O59 W18 118(2) . . ?
Co3 O59 W10 125(3) . . ?
W4 O23 W9 148(3) . . ?
W4 O23 Na10 106(3) . . ?
W9 O23 Na10 105(3) . . ?
W14 O54 W15 109(2) . . ?
O67 Na01 Na7 83.8(15) . 3_645 ?
O67 Na01 Na5 88.0(17) . . ?
O67 Na01 Na3B 165(3) . 3_645 ?
O67 Na01 Na7B 69(3) . 2_655 ?
O47 Na01 Na7 37.8(15) 3_645 3_645 ?
O47 Na01 O67 112(2) 3_645 . ?
O47 Na01 Na5 62.2(18) 3_645 . ?
O47 Na01 Na3B 79(3) 3_645 3_645 ?
O47 Na01 Na7B 121(3) 3_645 2_655 ?
O02B Na01 Na7 96(2) . 3_645 ?
O02B Na01 O67 90(2) . . ?
O02B Na01 O47 119(3) . 3_645 ?
O02B Na01 Na5 62.6(19) . . ?
O02B Na01 Na3B 94(3) . 3_645 ?
O02B Na01 Na7B 120(3) . 2_655 ?
Na5 Na01 Na7 33.2(10) . 3_645 ?
Na3B Na01 Na7 110(2) 3_645 3_645 ?
Na3B Na01 Na5 107(2) 3_645 . ?
Na7B Na01 Na7 134(3) 2_655 3_645 ?
Na7B Na01 Na5 156(3) 2_655 . ?
Na7B Na01 Na3B 97(3) 2_655 3_645 ?
W17 O50 Na7B 147(4) . . ?
W17 O50 Na7B 125(4) . 2_655 ?
Na7B O50 Na7B 27(5) . 2_655 ?
W4 O30 Co2 138(3) . . ?
W18 O51 Na02 141(3) . . ?
W12 O44 W17 117(3) . . ?
W12 O44 Na3 111(2) . . ?
W12 O44 Na11 129(3) . . ?
W17 O44 Na3 99(2) . . ?
W17 O44 Na11 107(3) . . ?
Na11 O44 Na3 85(2) . . ?
W16 O68 Co4 140(3) . . ?
W16 O68 Na5 108(2) . . ?
Co4 O68 Na5 112(2) . . ?
W6 O15 Na12 105(3) . . ?
W6 O21 Na9 107(3) . . ?
W5 O21 W6 155(3) . . ?
W5 O21 Na9 97(3) . . ?
W5 O16 Na12 107(3) . . ?
W5 O16 Na6A 137(3) . . ?
Na6A O16 Na12 111(3) . . ?
W12 O43 W16 117(3) . . ?
W7 O25 W6 95.7(19) . . ?
W7 O25 W2 95.5(17) . . ?
W6 O25 W2 94.4(18) . . ?
Co1 O25 W7 124(3) . . ?
Co1 O25 W6 117(2) . . ?
Co1 O25 W2 123(2) . . ?
W3 O12 W9 113(2) . . ?
W3 O12 Na10 103(3) . . ?
W9 O12 Na10 101(2) . . ?
W4 O22 Na2 102(3) . . ?
W5 O22 W4 109(3) . . ?
W5 O22 Na2 119(3) . . ?
W7 O19 W8 149(3) . . ?
W7 O19 Na1 106(2) . . ?
W8 O19 Na1 103(2) . . ?
W4 O17 Na1 129(3) . 3_656 ?
Co4 O02B Na01 113(3) . . ?
Co2 O35 Na2 113(3) . . ?
O51 Na02 O3 79(3) . 4_456 ?
O51 Na02 Na8 63(2) . . ?
O51 Na02 Na9 115(3) . 4_456 ?
O51 Na02 Na03 81(3) . . ?
O51 Na02 Na5A 111(3) . 4_456 ?
O3 Na02 Na8 83(2) 4_456 . ?
O3 Na02 Na9 84(3) 4_456 4_456 ?
O3 Na02 Na03 158(3) 4_456 . ?
O3 Na02 Na5A 75(2) 4_456 4_456 ?
Na8 Na02 Na9 53(2) . 4_456 ?
Na8 Na02 Na5A 158(3) . 4_456 ?
Na9 Na02 Na5A 123(3) 4_456 4_456 ?
Na03 Na02 Na8 79(3) . . ?
Na03 Na02 Na9 95(3) . 4_456 ?
Na03 Na02 Na5A 122(3) . 4_456 ?
O1AA Na02 O51 99(4) 4_456 . ?
O1AA Na02 O3 119(3) 4_456 4_456 ?
O1AA Na02 Na8 46(2) 4_456 . ?
O1AA Na02 Na9 41(3) 4_456 4_456 ?
O1AA Na02 Na03 55(3) 4_456 . ?
O1AA Na02 Na5A 149(4) 4_456 4_456 ?
O73 Na02 O51 123(4) . . ?
O73 Na02 O3 154(4) . 4_456 ?
O73 Na02 Na8 118(4) . . ?
O73 Na02 Na9 96(4) . 4_456 ?
O73 Na02 Na03 49(3) . . ?
O73 Na02 O1AA 74(4) . 4_456 ?
O73 Na02 Na5A 83(3) . 4_456 ?
W13 O64 Co2 131(3) . . ?
W13 O64 Fe1 133(3) . . ?
Co2 O64 Fe1 94(2) . . ?
Na7 Na5 Na01 78.0(18) 3_645 . ?
Na7 Na5 O68 98(2) 3_645 . ?
Na7 Na5 O038 118(3) 3_645 . ?
Na7 Na5 Na1B 109(2) 3_645 2_755 ?
Na01 Na5 Na1B 141.8(19) . 2_755 ?
O68 Na5 Na01 56.4(15) . . ?
O68 Na5 Na1B 150(2) . 2_755 ?
O038 Na5 Na01 158(3) . . ?
O038 Na5 O68 105(3) . . ?
O038 Na5 Na1B 51(2) . 2_755 ?
W3 O1 Na5A 102(3) . . ?
W10 O37 Na1B 143(4) . 4_455 ?
W3 O5 W1 154(3) . . ?
W3 O5 Na10 101(3) . . ?
W1 O5 Na10 102(2) . . ?
W8 O7 Na1 99(2) . . ?
W8 O7 Na2 120(2) . 3_646 ?
W3 O7 W8 115(2) . . ?
W3 O7 Na1 101(2) . . ?
W3 O7 Na2 116(3) . 3_646 ?
Na1 O7 Na2 102(2) . 3_646 ?
O22 Na2 Na1 83(2) . 3_656 ?
O22 Na2 O35 92(2) . . ?
O22 Na2 Na6A 83(2) . 2_765 ?
O35 Na2 Na1 92(2) . 3_656 ?
O35 Na2 Na6A 142(3) . 2_765 ?
O7 Na2 Na1 37.0(13) 3_656 3_656 ?
O7 Na2 O22 112(3) 3_656 . ?
O7 Na2 O35 112(3) 3_656 . ?
O7 Na2 Na6A 104(2) 3_656 2_765 ?
Na6B Na2 Na1 143(3) 2_765 3_656 ?
Na6B Na2 O22 134(3) 2_765 . ?
Na6B Na2 O35 92(3) 2_765 . ?
Na6B Na2 O7 109(3) 2_765 3_656 ?
Na6B Na2 Na6A 66(2) 2_765 2_765 ?
Na6A Na2 Na1 125(2) 2_765 3_656 ?
W18 O45 Na3 102(2) . . ?
W10 O45 W18 113(3) . . ?
W10 O45 Na3 115(3) . . ?
W15 O66 Fe2 144(3) . . ?
Na4 Na3 O56 163(3) 4_455 . ?
Na4 Na3 O44 125(2) 4_455 . ?
Na4 Na3 O45 108(2) 4_455 . ?
Na4 Na3 Na11 102(2) 4_455 . ?
Na4 Na3 O0BA 96(2) 4_455 4_455 ?
O56 Na3 O44 56.2(19) . . ?
O56 Na3 Na11 89.2(19) . . ?
O44 Na3 Na11 44.3(17) . . ?
O45 Na3 O56 55.3(17) . . ?
O45 Na3 O44 91(2) . . ?
O45 Na3 Na11 135(2) . . ?
O0BA Na3 O56 96(2) 4_455 . ?
O0BA Na3 O44 122(2) 4_455 . ?
O0BA Na3 O45 114(2) 4_455 . ?
O0BA Na3 Na11 94(2) 4_455 . ?
W8 O27 W3 97.4(19) . . ?
W9 O27 W8 96(2) . . ?
W9 O27 W3 97(2) . . ?
Co1 O27 W8 120(3) . . ?
Co1 O27 W3 124(3) . . ?
Co1 O27 W9 116(2) . . ?
W1 O3 Na02 107(3) . 4_556 ?
O02Z Na6 Na3B 60(5) 4_556 4 ?
O02Z Na6 O5BA 72(6) 4_556 . ?
O033 Na6 O02Z 136(9) 4_556 4_556 ?
O033 Na6 Na3B 82(7) 4_556 4 ?
O033 Na6 O5BA 151(10) 4_556 . ?
Na10 Na6 O02Z 82(8) 4_556 4_556 ?
Na10 Na6 O033 91(9) 4_556 4_556 ?
Na10 Na6 Na3B 51(6) 4_556 4 ?
Na10 Na6 O5BA 103(9) 4_556 . ?
O5BA Na6 Na3B 127(7) . 4 ?
W2 O2 Na5A 98(3) . . ?
W9 Na8 Na03 76.4(16) . . ?
W9 Na8 Na73 111(2) . . ?
O24 Na8 W9 34.2(14) . . ?
O24 Na8 Na02 149(3) . . ?
O24 Na8 Na9 93(3) . 4_456 ?
O24 Na8 Na03 110(2) . . ?
O24 Na8 Na73 81(2) . . ?
O63 Na8 W9 86(2) . . ?
O63 Na8 O24 95(3) . . ?
O63 Na8 Na02 93(2) . . ?
O63 Na8 Na9 152(3) . 4_456 ?
O63 Na8 Na03 66.3(18) . . ?
O63 Na8 Na73 77(2) . . ?
Na02 Na8 W9 117(2) . . ?
Na02 Na8 Na03 47.3(19) . . ?
Na02 Na8 Na73 130(3) . . ?
Na9 Na8 W9 85(3) 4_456 . ?
Na9 Na8 Na02 67(3) 4_456 . ?
Na9 Na8 Na03 86(3) 4_456 . ?
Na9 Na8 Na73 131(3) 4_456 . ?
O1AA Na8 W9 73(2) 4_456 . ?
O1AA Na8 O24 103(3) 4_456 . ?
O1AA Na8 O63 103(3) 4_456 . ?
O1AA Na8 Na02 46(2) 4_456 . ?
O1AA Na8 Na9 49(3) 4_456 4_456 ?
O1AA Na8 Na03 37(2) 4_456 . ?
O1AA Na8 O70 122(4) 4_456 4_456 ?
O1AA Na8 Na73 176(4) 4_456 . ?
O70 Na8 W9 129(4) 4_456 . ?
O70 Na8 O24 99(4) 4_456 . ?
O70 Na8 O63 128(4) 4_456 . ?
O70 Na8 Na02 100(4) 4_456 . ?
O70 Na8 Na9 77(4) 4_456 4_456 ?
O70 Na8 Na03 147(4) 4_456 . ?
O70 Na8 Na73 56(3) 4_456 . ?
Na73 Na8 Na03 142(3) . . ?
W13 O46 Na7 97(2) . . ?
W10 O46 W13 112(3) . . ?
W10 O46 Na7 97(2) . . ?
Na6 O02Z Na10 35(5) 4_456 . ?
Na4 O030 Na1B 128(3) . . ?
Na6 O033 Na10 40(6) 4_456 . ?
W8 O13 Na73 115(3) . . ?
W5 Na9 Na02 109(3) . 4_556 ?
W5 Na9 Na6A 59.6(18) . . ?
O10 Na9 W5 33.5(17) . . ?
O10 Na9 O21 55(3) . . ?
O10 Na9 Na02 80(3) . 4_556 ?
O10 Na9 Na8 88(3) . 4_556 ?
O10 Na9 Na12 98(4) . . ?
O10 Na9 Na6A 61(2) . . ?
O21 Na9 W5 30.4(14) . . ?
O21 Na9 Na02 107(4) . 4_556 ?
O21 Na9 Na8 142(4) . 4_556 ?
O21 Na9 Na12 61(3) . . ?
O21 Na9 Na6A 88(3) . . ?
Na02 Na9 Na6A 118(3) 4_556 . ?
Na8 Na9 W5 116(3) 4_556 . ?
Na8 Na9 Na02 59(3) 4_556 4_556 ?
Na8 Na9 Na12 135(4) 4_556 . ?
Na8 Na9 Na6A 72(3) 4_556 . ?
Na12 Na9 W5 66(2) . . ?
Na12 Na9 Na02 165(4) . 4_556 ?
Na12 Na9 Na6A 72(3) . . ?
O1AA Na9 W5 150(4) . . ?
O1AA Na9 O10 117(5) . . ?
O1AA Na9 O21 143(5) . . ?
O1AA Na9 Na02 42(3) . 4_556 ?
O1AA Na9 Na8 50(3) . 4_556 ?
O1AA Na9 Na12 144(5) . . ?
O1AA Na9 Na6A 121(4) . . ?
O11 Na10 W3 85(2) . . ?
O11 Na10 O23 59(2) . . ?
O11 Na10 O12 103(3) . . ?
O11 Na10 O5 58(2) . . ?
O11 Na10 O02Z 139(3) . . ?
O11 Na10 Na3B 80(3) . 1_556 ?
O23 Na10 W3 67.2(18) . . ?
O23 Na10 O12 59(2) . . ?
O23 Na10 O5 66(2) . . ?
O23 Na10 O02Z 150(3) . . ?
O23 Na10 Na3B 138(4) . 1_556 ?
O12 Na10 W3 30.3(13) . . ?
O12 Na10 O5 58(2) . . ?
O12 Na10 O02Z 90(3) . . ?
O12 Na10 Na3B 145(4) . 1_556 ?
O5 Na10 W3 30.1(13) . . ?
O5 Na10 O02Z 101(3) . . ?
O5 Na10 Na3B 98(4) . 1_556 ?
Na6 Na10 W3 117(7) 4_456 . ?
Na6 Na10 O11 152(8) 4_456 . ?
Na6 Na10 O23 112(7) 4_456 . ?
Na6 Na10 O12 92(7) 4_456 . ?
Na6 Na10 O5 147(8) 4_456 . ?
Na6 Na10 O02Z 63(7) 4_456 . ?
Na6 Na10 O033 49(7) 4_456 . ?
Na6 Na10 Na3B 102(8) 4_456 1_556 ?
O02Z Na10 W3 88(2) . . ?
O02Z Na10 Na3B 68(3) . 1_556 ?
O033 Na10 W3 153(3) . . ?
O033 Na10 O11 103(3) . . ?
O033 Na10 O23 95(3) . . ?
O033 Na10 O12 123(3) . . ?
O033 Na10 O5 158(3) . . ?
O033 Na10 O02Z 101(3) . . ?
O033 Na10 Na3B 89(4) . 1_556 ?
Na3B Na10 W3 118(3) 1_556 . ?
Na4 O038 Na5 137(5) . . ?
O57 Na03 Na02 91(3) . . ?
O57 Na03 Na8 79(2) . . ?
O57 Na03 O9AA 97(3) . 3_656 ?
O57 Na03 O1AA 112(3) . 4_456 ?
O57 Na03 Na0A 52(2) . . ?
O57 Na03 Na5A 91(3) . 3_656 ?
Na02 Na03 Na8 54(2) . . ?
Na02 Na03 Na0A 82(3) . . ?
O9AA Na03 Na02 166(4) 3_656 . ?
O9AA Na03 Na8 116(3) 3_656 . ?
O9AA Na03 Na0A 112(3) 3_656 . ?
O1AA Na03 Na02 50(2) 4_456 . ?
O1AA Na03 Na8 34(2) 4_456 . ?
O1AA Na03 O9AA 116(3) 4_456 3_656 ?
O1AA Na03 Na0A 131(3) 4_456 . ?
O1AA Na03 Na5A 157(4) 4_456 3_656 ?
Na0A Na03 Na8 114(2) . . ?
Na5A Na03 Na02 139(3) 3_656 . ?
Na5A Na03 Na8 164(3) 3_656 . ?
Na5A Na03 O9AA 53(3) 3_656 3_656 ?
Na5A Na03 Na0A 67(3) 3_656 . ?
O73 Na03 O57 127(4) . . ?
O73 Na03 Na02 51(3) . . ?
O73 Na03 Na8 97(3) . . ?
O73 Na03 O9AA 129(4) . 3_656 ?
O73 Na03 O1AA 72(3) . 4_456 ?
O73 Na03 Na0A 84(3) . . ?
O73 Na03 Na5A 98(4) . 3_656 ?
O44 Na11 Na3 50.8(19) . . ?
O44 Na11 O02Y 102(3) . . ?
O44 Na11 O2BA 82(3) . . ?
O44 Na11 Na7B 106(4) . . ?
O44 Na11 Na7B 96(3) . 2_655 ?
O02Y Na11 Na3 59(2) . . ?
O02Y Na11 Na7B 62(3) . . ?
O02Y Na11 Na7B 81(3) . 2_655 ?
O2BA Na11 Na3 131(3) . . ?
O2BA Na11 O02Y 133(3) . . ?
O2BA Na11 Na7B 72(3) . . ?
O2BA Na11 Na7B 52(3) . 2_655 ?
Na7B Na11 Na3 104(3) . . ?
Na7B Na11 Na3 113(3) 2_655 . ?
Na7B Na11 Na7B 21(4) . 2_655 ?
O8BA Na11 O44 95(4) . . ?
O8BA Na11 Na3 94(3) . . ?
O8BA Na11 O02Y 121(4) . . ?
O8BA Na11 O2BA 105(4) . . ?
O8BA Na11 Na7B 158(5) . . ?
O8BA Na11 Na7B 152(4) . 2_655 ?
O15 Na12 Na9 78(3) . . ?
O15 Na12 Na6B 159(3) . . ?
O16 Na12 O15 111(3) . . ?
O16 Na12 Na9 65(3) . . ?
O16 Na12 Na6B 84(3) . . ?
Na6B Na12 Na9 98(3) . . ?
O8BA Na12 O15 91(3) 4 . ?
O8BA Na12 O16 108(4) 4 . ?
O8BA Na12 Na9 162(4) 4 . ?
O8BA Na12 Na6B 98(3) 4 . ?
Na6A O03C Na6A 92(5) . 2_765 ?
Na3 O0BA Na3B 171(4) 4 . ?
W16 O49 Na7 131(3) . 3_645 ?
O37 Na1B Na5 66(2) 4 2_755 ?
O37 Na1B O030 72(3) 4 . ?
O37 Na1B Na1B 109(2) 4 2_755 ?
O030 Na1B Na5 123(3) . 2_755 ?
O030 Na1B Na1B 94(4) . 2_755 ?
Na1B Na1B Na5 135(4) 2_755 2_755 ?
Na1 O9AA Na03 117(4) . 3_646 ?
Na1 O9AA Na5A 107(4) . . ?
Na5A O9AA Na03 62(3) . 3_646 ?
O42 Na3B Na01 74(3) . 3_655 ?
O42 Na3B Na6 74(4) . 4_455 ?
O42 Na3B Na10 100(5) . 1_554 ?
O42 Na3B O0BA 89(4) . . ?
Na6 Na3B Na01 101(4) 4_455 3_655 ?
Na10 Na3B Na01 116(4) 1_554 3_655 ?
Na10 Na3B Na6 27(4) 1_554 4_455 ?
O0BA Na3B Na01 98(4) . 3_655 ?
O0BA Na3B Na6 150(6) . 4_455 ?
O0BA Na3B Na10 146(5) . 1_554 ?
O4BA Na3B O42 145(6) 1_554 . ?
O4BA Na3B Na01 73(4) 1_554 3_655 ?
O4BA Na3B Na6 104(6) 1_554 4_455 ?
O4BA Na3B Na10 88(5) 1_554 1_554 ?
O4BA Na3B O0BA 104(5) 1_554 . ?
Na6B O5BA Na6 173(8) . . ?
Na02 O1AA Na8 88(3) 4_556 4_556 ?
Na02 O1AA Na03 76(3) 4_556 4_556 ?
Na8 O1AA Na03 110(4) 4_556 4_556 ?
Na9 O1AA Na02 97(4) . 4_556 ?
Na9 O1AA Na8 81(4) . 4_556 ?
Na9 O1AA Na03 167(4) . 4_556 ?
O57 Na0A Na03 41.8(18) . . ?
O57 Na0A Na5A 66(2) . 3_656 ?
Na0A Na0A O57 120(6) 2_665 . ?
Na0A Na0A Na03 109(3) 2_665 . ?
Na0A Na0A Na5A 134(2) 2_665 3_656 ?
Na5A Na0A Na03 40.7(18) 3_656 . ?
Na2 Na6B Na12 152(4) 2_765 . ?
Na2 Na6B Na6A 74(3) 2_765 . ?
Na12 Na6B Na6A 79(2) . . ?
O5BA Na6B Na2 112(5) . 2_765 ?
O5BA Na6B Na12 74(5) . . ?
O5BA Na6B Na6A 120(5) . . ?
O5BA Na6B O71 86(6) . . ?
O71 Na6B Na2 78(4) . 2_765 ?
O71 Na6B Na12 76(4) . . ?
O71 Na6B Na6A 35(3) . . ?
O82 Na6B Na2 82(4) . 2_765 ?
O82 Na6B Na12 97(4) . . ?
O82 Na6B O5BA 165(7) . . ?
O82 Na6B Na6A 68(4) . . ?
O82 Na6B O71 103(5) . . ?
O16 Na6A Na2 120(3) . 2_765 ?
O16 Na6A Na9 52(2) . . ?
O16 Na6A Na6B 81(3) . . ?
O16 Na6A Na6A 106(3) . 2_765 ?
O16 Na6A O70 91(4) . . ?
Na2 Na6A Na9 104(2) 2_765 . ?
O03C Na6A O16 127(4) . . ?
O03C Na6A Na2 107(3) . 2_765 ?
O03C Na6A Na9 138(3) . . ?
O03C Na6A Na6B 144(3) . . ?
O03C Na6A Na6A 44(3) . 2_765 ?
O03C Na6A O71 145(5) . . ?
O03C Na6A O70 79(4) . . ?
Na6B Na6A Na2 39.9(17) . 2_765 ?
Na6B Na6A Na9 76(2) . . ?
Na6A Na6A Na2 95(3) 2_765 2_765 ?
Na6A Na6A Na9 156(4) 2_765 . ?
Na6A Na6A Na6B 112(2) 2_765 . ?
O71 Na6A O16 86(4) . . ?
O71 Na6A Na2 54(4) . 2_765 ?
O71 Na6A Na9 50(4) . . ?
O71 Na6A Na6B 40(4) . . ?
O71 Na6A Na6A 148(5) . 2_765 ?
O71 Na6A O70 89(5) . . ?
O70 Na6A Na2 126(4) . 2_765 ?
O70 Na6A Na9 59(3) . . ?
O70 Na6A Na6B 128(4) . . ?
O70 Na6A Na6A 120(4) . 2_765 ?
Na01 Na7B Na11 108(4) 2_655 2_655 ?
O50 Na7B Na01 83(4) 2_655 2_655 ?
O50 Na7B Na01 120(5) . 2_655 ?
O50 Na7B O50 139(5) . 2_655 ?
O50 Na7B Na11 57(3) 2_655 2_655 ?
O50 Na7B Na11 130(5) . 2_655 ?
O50 Na7B Na11 65(3) . . ?
O50 Na7B Na11 148(5) 2_655 . ?
Na11 Na7B Na01 103(4) . 2_655 ?
Na11 Na7B Na11 92(4) . 2_655 ?
Na7B Na7B Na01 154(10) 2_655 2_655 ?
Na7B Na7B O50 81(10) 2_655 . ?
Na7B Na7B O50 71(10) 2_655 2_655 ?
Na7B Na7B Na11 59(8) 2_655 2_655 ?
Na7B Na7B Na11 100(9) 2_655 . ?
Na11 O8BA Na12 162(5) . 4_455 ?
W2 Na5A Na1 56.2(12) . . ?
W2 Na5A Na02 61.5(17) . 4_556 ?
W2 Na5A Na0A 125(3) . 3_646 ?
W3 Na5A W2 64.2(13) . . ?
W3 Na5A Na1 56.5(12) . . ?
W3 Na5A Na02 103(2) . 4_556 ?
W3 Na5A Na0A 150(3) . 3_646 ?
Na1 Na5A Na02 117(2) . 4_556 ?
O52 Na5A W2 163(3) 3_646 . ?
O52 Na5A W3 104(3) 3_646 . ?
O52 Na5A Na1 107(3) 3_646 . ?
O52 Na5A Na02 136(3) 3_646 4_556 ?
O52 Na5A O1 75(2) 3_646 . ?
O52 Na5A O2 158(3) 3_646 . ?
O52 Na5A Na03 87(3) 3_646 3_646 ?
O52 Na5A Na0A 72(3) 3_646 3_646 ?
O52 Na5A O6 132(3) 3_646 . ?
O1 Na5A W2 94(2) . . ?
O1 Na5A W3 29.9(13) . . ?
O1 Na5A Na1 71(2) . . ?
O1 Na5A Na02 122(3) . 4_556 ?
O1 Na5A O2 123(3) . . ?
O1 Na5A Na03 140(4) . 3_646 ?
O1 Na5A Na0A 131(3) . 3_646 ?
O1 Na5A O6 63(2) . . ?
O2 Na5A W2 28.8(13) . . ?
O2 Na5A W3 93(2) . . ?
O2 Na5A Na1 70(2) . . ?
O2 Na5A Na02 50.8(19) . 4_556 ?
O2 Na5A Na0A 100(3) . 3_646 ?
Na03 Na5A W2 94(3) 3_646 . ?
Na03 Na5A W3 138(3) 3_646 . ?
Na03 Na5A Na1 81(2) 3_646 . ?
Na03 Na5A Na02 96(3) 3_646 4_556 ?
Na03 Na5A O2 71(2) 3_646 . ?
Na03 Na5A Na0A 72(3) 3_646 3_646 ?
Na03 Na5A O6 112(3) 3_646 . ?
O9AA Na5A W2 90(3) . . ?
O9AA Na5A W3 80(3) . . ?
O9AA Na5A Na1 36(2) . . ?
O9AA Na5A O52 74(3) . 3_646 ?
O9AA Na5A Na02 146(4) . 4_556 ?
O9AA Na5A O1 76(3) . . ?
O9AA Na5A O2 95(3) . . ?
O9AA Na5A Na03 64(3) . 3_646 ?
O9AA Na5A Na0A 125(4) . 3_646 ?
O9AA Na5A O6 76(3) . . ?
Na0A Na5A Na1 154(3) 3_646 . ?
Na0A Na5A Na02 67(2) 3_646 4_556 ?
O6 Na5A W2 32.3(13) . . ?
O6 Na5A W3 33.8(13) . . ?
O6 Na5A Na1 40.8(14) . . ?
O6 Na5A Na02 87(2) . 4_556 ?
O6 Na5A O2 60(2) . . ?
O6 Na5A Na0A 154(3) . 3_646 ?
O72 Na5A W2 104(4) . . ?
O72 Na5A W3 81(4) . . ?
O72 Na5A Na1 138(4) . . ?
O72 Na5A O52 86(4) . 3_646 ?
O72 Na5A Na02 64(4) . 4_556 ?
O72 Na5A O1 74(4) . . ?
O72 Na5A O2 111(4) . . ?
O72 Na5A Na03 141(5) . 3_646 ?
O72 Na5A O9AA 148(5) . . ?
O72 Na5A Na0A 69(4) . 3_646 ?
O72 Na5A O6 101(4) . . ?
W2 O6 Na1 104(2) . . ?
W2 O6 Na5A 97(2) . . ?
W3 O6 W2 153(2) . . ?
W3 O6 Na1 102(2) . . ?
W3 O6 Na5A 91(2) . . ?
Na1 O6 Na5A 91(2) . . ?
Na6A O71 Na6B 105(5) . . ?
Na8 O70 Na6A 113(5) 4_556 . ?
Na03 O73 Na02 81(4) . . ?
W17 Na73 Na8 97(2) . . ?
O69 Na73 W17 29.1(14) . . ?
O69 Na73 Na8 90(3) . . ?
O69 Na73 O13 97(3) . . ?
O13 Na73 W17 126(3) . . ?
O13 Na73 Na8 79(2) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O58 W14 O65 Co2 -37(3) . . . . ?
O58 W14 O65 Fe2 108(4) . . . . ?
O58 W13 O52 Na5A -174(4) . . . 3_656 ?
O58 W13 O64 Co2 42(4) . . . . ?
O58 W13 O64 Fe1 -116(4) . . . . ?
O4 W2 O2 Na5A 72(3) . . . . ?
O4 W1 O3 Na02 19(3) . . . 4_556 ?
O41 W11 O42 W15 -15(7) . . . . ?
O41 W11 O42 Na3B -177(6) . . . . ?
O41 W10 O37 Na1B 44(6) . . . 4_455 ?
O41 W10 O45 W18 33(9) . . . . ?
O41 W10 O45 Na3 -83(8) . . . . ?
O33 W7 O20 W6 76(2) . . . . ?
O8 W7 O33 Co4 -112(6) . . . . ?
O8 W7 O33 Fe2 43(9) . . . . ?
O8 W7 O20 W6 -86(2) . . . . ?
O8 W2 O4 W1 30(10) . . . . ?
O8 W2 O2 Na5A -102(2) . . . . ?
O9 W6 O28 Fe2 -27(10) . . . . ?
O9 W6 O15 Na12 -104(3) . . . . ?
O9 W2 O4 W1 128(6) . . . . ?
O9 W2 O2 Na5A 163(2) . . . . ?
O60 W14 O58 W13 70(4) . . . . ?
O60 W14 O58 Na7 -91(2) . . . . ?
O60 W14 O65 Co2 -124(3) . . . . ?
O60 W14 O65 Fe2 21(4) . . . . ?
O60 W15 O55 W16 -71(4) . . . . ?
O60 W15 O48 Na4 113(6) . . . . ?
O60 W15 O66 Fe2 -22(5) . . . . ?
O60 W11 O42 W15 2(2) . . . . ?
O60 W11 O42 Na3B -160(4) . . . . ?
O60 Co3 O62 Fe1 119(3) . . . . ?
O60 Co3 O62 Co4 -121(3) . . . . ?
O60 Co3 O62 Fe2 0(3) . . . . ?
O67 W16 O68 Co4 -48(4) . . . . ?
O67 W16 O68 Na5 122(2) . . . . ?
O67 W16 O49 Na7 -134(3) . . . 3_645 ?
O67 W17 O69 Co4 52(3) . . . . ?
O67 W17 O69 Na73 -112(3) . . . . ?
O67 W17 O50 Na7B 6(4) . . . 2_655 ?
O67 W17 O50 Na7B -18(7) . . . . ?
O52 W13 O64 Co2 -59(4) . . . . ?
O52 W13 O64 Fe1 143(4) . . . . ?
O39 W11 O42 W15 -85(2) . . . . ?
O39 W11 O42 Na3B 113(4) . . . . ?
O39 W12 O44 W17 -18(8) . . . . ?
O39 W12 O44 Na3 95(6) . . . . ?
O39 W12 O44 Na11 -164(4) . . . . ?
O39 W12 O43 W16 86(3) . . . . ?
O61 W16 O68 Co4 25(4) . . . . ?
O61 W16 O68 Na5 -165(2) . . . . ?
O61 W16 O49 Na7 -171(5) . . . 3_645 ?
O61 W12 O44 W17 0(2) . . . . ?
O61 W12 O44 Na3 112(3) . . . . ?
O61 W12 O44 Na11 -147(4) . . . . ?
O61 W12 O43 W16 0(2) . . . . ?
O61 W17 O69 Co4 -22(3) . . . . ?
O61 W17 O69 Na73 175(3) . . . . ?
O61 W17 O50 Na7B 41(12) . . . . ?
O61 W17 O50 Na7B 66(9) . . . 2_655 ?
O61 Co3 O62 Fe1 -120(3) . . . . ?
O61 Co3 O62 Co4 0(4) . . . . ?
O61 Co3 O62 Fe2 121(3) . . . . ?
O42 W15 O55 W16 -142(5) . . . . ?
O42 W15 O48 Na4 157(2) . . . . ?
O42 W15 O66 Fe2 -19(10) . . . . ?
O28 W6 O15 Na12 79(3) . . . . ?
O29 W5 O21 W6 -14(8) . . . . ?
O29 W5 O21 Na9 156(3) . . . . ?
O29 W5 O16 Na12 -74(3) . . . . ?
O29 W5 O16 Na6A 136(4) . . . . ?
O53 W14 O58 W13 -124(5) . . . . ?
O53 W14 O58 Na7 75(2) . . . . ?
O53 W14 O65 Co2 67(3) . . . . ?
O53 W14 O65 Fe2 -149(4) . . . . ?
O57 W13 O52 Na5A 13(4) . . . 3_656 ?
O57 W13 O64 Co2 -157(4) . . . . ?
O57 W13 O64 Fe1 46(4) . . . . ?
O57 W18 O56 W17 73(10) . . . . ?
O57 W18 O56 Na3 -96(7) . . . . ?
O57 W18 O63 Fe1 -56(4) . . . . ?
O57 W18 O63 Na8 97(3) . . . . ?
O57 W18 O51 Na02 -27(5) . . . . ?
O11 W4 O23 W9 -145(6) . . . . ?
O11 W4 O23 Na10 25(3) . . . . ?
O11 W4 O30 Co2 -32(12) . . . . ?
O11 W4 O17 Na1 -155(4) . . . 3_656 ?
O11 W1 O3 Na02 -168(3) . . . 4_556 ?
O55 W16 O68 Co4 112(4) . . . . ?
O55 W16 O68 Na5 -77(2) . . . . ?
O55 W16 O49 Na7 55(4) . . . 3_645 ?
O55 W15 O48 Na4 -119(3) . . . . ?
O55 W15 O66 Fe2 -110(5) . . . . ?
O65 W14 O58 W13 -21(5) . . . . ?
O65 W14 O58 Na7 178(2) . . . . ?
O24 W8 O32 Fe1 44(4) . . . . ?
O24 W8 O32 Co4 -154(3) . . . . ?
O24 W8 O13 Na73 77(3) . . . . ?
O24 W9 O31 Fe1 -51(5) . . . . ?
O20 W7 O33 Co4 160(3) . . . . ?
O20 W7 O33 Fe2 -45(4) . . . . ?
O20 W6 O28 Fe2 45(5) . . . . ?
O20 W6 O15 Na12 174(2) . . . . ?
O32 W8 O24 W9 -75(3) . . . . ?
O32 W8 O24 Na8 35(3) . . . . ?
O32 W8 O13 Na73 -20(3) . . . . ?
O48 W15 O55 W16 123(4) . . . . ?
O48 W15 O66 Fe2 145(5) . . . . ?
O10 W5 O29 Co2 30(10) . . . . ?
O10 W5 O21 W6 150(8) . . . . ?
O10 W5 O21 Na9 -41(3) . . . . ?
O10 W5 O16 Na12 106(3) . . . . ?
O10 W5 O16 Na6A -44(5) . . . . ?
O10 W1 O3 Na02 -71(3) . . . 4_556 ?
O47 W14 O58 W13 142(5) . . . . ?
O47 W14 O58 Na7 -19(2) . . . . ?
O47 W14 O65 Co2 -132(7) . . . . ?
O47 W14 O65 Fe2 13(11) . . . . ?
O47 W11 O42 W15 74(3) . . . . ?
O47 W11 O42 Na3B -88(4) . . . . ?
O40 W12 O44 W17 -86(3) . . . . ?
O40 W12 O44 Na3 26(3) . . . . ?
O40 W12 O44 Na11 127(4) . . . . ?
O40 W12 O43 W16 25(8) . . . . ?
O40 W10 O37 Na1B -43(6) . . . 4_455 ?
O40 W10 O45 W18 90(3) . . . . ?
O40 W10 O45 Na3 -26(3) . . . . ?
O56 W18 O63 Fe1 107(4) . . . . ?
O56 W18 O63 Na8 -100(3) . . . . ?
O56 W18 O51 Na02 158(5) . . . . ?
O56 W17 O69 Co4 -107(4) . . . . ?
O56 W17 O69 Na73 89(3) . . . . ?
O56 W17 O50 Na7B 178(4) . . . 2_655 ?
O56 W17 O50 Na7B 154(7) . . . . ?
O34 Co1 O25 W7 -57(3) . . . . ?
O34 Co1 O25 W6 62(3) . . . . ?
O34 Co1 O25 W2 178(2) . . . . ?
O34 Co1 O27 W8 56(3) . . . . ?
O34 Co1 O27 W3 -179(2) . . . . ?
O34 Co1 O27 W9 -59(3) . . . . ?
O26 W4 O23 W9 -72(6) . . . . ?
O26 W4 O23 Na10 98(3) . . . . ?
O26 W4 O30 Co2 -26(4) . . . . ?
O26 W4 O17 Na1 179(5) . . . 3_656 ?
O26 W5 O29 Co2 24(4) . . . . ?
O26 W5 O21 W6 77(8) . . . . ?
O26 W5 O21 Na9 -114(3) . . . . ?
O26 W5 O16 Na12 120(6) . . . . ?
O26 W5 O16 Na6A -30(9) . . . . ?
O26 Co1 O34 Co2 -1(4) . . . . ?
O26 Co1 O34 Fe1 -119(3) . . . . ?
O26 Co1 O34 Fe2 120(3) . . . . ?
O26 Co1 O25 W7 177(3) . . . . ?
O26 Co1 O25 W6 -64(3) . . . . ?
O26 Co1 O25 W2 52(3) . . . . ?
O26 Co1 O27 W8 -178(2) . . . . ?
O26 Co1 O27 W3 -53(3) . . . . ?
O26 Co1 O27 W9 67(3) . . . . ?
O69 W17 O50 Na7B -87(4) . . . 2_655 ?
O69 W17 O50 Na7B -111(7) . . . . ?
O63 W18 O56 W17 -24(7) . . . . ?
O63 W18 O56 Na3 167(2) . . . . ?
O63 W18 O51 Na02 62(5) . . . . ?
O59 W13 O52 Na5A 68(8) . . . 3_656 ?
O59 W13 O64 Co2 129(4) . . . . ?
O59 W13 O64 Fe1 -29(4) . . . . ?
O59 W18 O56 W17 67(6) . . . . ?
O59 W18 O56 Na3 -102(2) . . . . ?
O59 W18 O63 Fe1 20(4) . . . . ?
O59 W18 O63 Na8 174(2) . . . . ?
O59 W18 O51 Na02 -74(11) . . . . ?
O59 W10 O37 Na1B -159(9) . . . 4_455 ?
O59 W10 O45 W18 4(2) . . . . ?
O59 W10 O45 Na3 -112(3) . . . . ?
O59 Co3 O62 Fe1 -3(3) . . . . ?
O59 Co3 O62 Co4 117(3) . . . . ?
O59 Co3 O62 Fe2 -122(3) . . . . ?
O23 W4 O30 Co2 -113(4) . . . . ?
O23 W4 O17 Na1 -69(4) . . . 3_656 ?
O23 W9 O31 Fe1 109(4) . . . . ?
O54 W14 O58 W13 85(7) . . . . ?
O54 W14 O58 Na7 -76(6) . . . . ?
O54 W14 O65 Co2 161(3) . . . . ?
O54 W14 O65 Fe2 -54(4) . . . . ?
O54 W15 O55 W16 -96(7) . . . . ?
O54 W15 O48 Na4 72(3) . . . . ?
O54 W15 O66 Fe2 53(5) . . . . ?
O50 W17 O69 Co4 152(3) . . . . ?
O50 W17 O69 Na73 -12(3) . . . . ?
O30 W4 O23 W9 21(6) . . . . ?
O30 W4 O23 Na10 -170(3) . . . . ?
O30 W4 O17 Na1 26(4) . . . 3_656 ?
O51 W18 O56 W17 -125(6) . . . . ?
O51 W18 O56 Na3 66(3) . . . . ?
O51 W18 O63 Fe1 -149(4) . . . . ?
O51 W18 O63 Na8 4(3) . . . . ?
O44 W12 O43 W16 -72(3) . . . . ?
O44 W17 O69 Co4 -20(8) . . . . ?
O44 W17 O69 Na73 177(5) . . . . ?
O44 W17 O50 Na7B 66(7) . . . . ?
O44 W17 O50 Na7B 90(4) . . . 2_655 ?
O68 W16 O49 Na7 -42(4) . . . 3_645 ?
O15 W6 O28 Fe2 143(5) . . . . ?
O21 W6 O28 Fe2 -113(5) . . . . ?
O21 W6 O15 Na12 -14(3) . . . . ?
O21 W5 O29 Co2 107(4) . . . . ?
O21 W5 O16 Na12 21(3) . . . . ?
O21 W5 O16 Na6A -129(5) . . . . ?
O16 W5 O29 Co2 -152(4) . . . . ?
O16 W5 O21 W6 -123(8) . . . . ?
O16 W5 O21 Na9 46(3) . . . . ?
O38 W11 O42 W15 175(3) . . . . ?
O38 W11 O42 Na3B 12(5) . . . . ?
O43 W16 O68 Co4 27(9) . . . . ?
O43 W16 O68 Na5 -163(5) . . . . ?
O43 W16 O49 Na7 141(3) . . . 3_645 ?
O43 W12 O44 W17 73(3) . . . . ?
O43 W12 O44 Na3 -175(3) . . . . ?
O43 W12 O44 Na11 -74(4) . . . . ?
O25 W7 O33 Co4 -125(3) . . . . ?
O25 W7 O33 Fe2 30(4) . . . . ?
O25 W7 O20 W6 -11(2) . . . . ?
O25 W6 O28 Fe2 -28(5) . . . . ?
O25 W6 O15 Na12 -139(9) . . . . ?
O25 W2 O4 W1 54(6) . . . . ?
O25 Co1 O34 Co2 -123(3) . . . . ?
O25 Co1 O34 Fe1 118(3) . . . . ?
O25 Co1 O34 Fe2 -2(4) . . . . ?
O25 Co1 O27 W8 -63(3) . . . . ?
O25 Co1 O27 W3 61(3) . . . . ?
O25 Co1 O27 W9 -179(3) . . . . ?
O12 W3 O1 Na5A -163(2) . . . . ?
O12 W9 O31 Fe1 17(11) . . . . ?
O22 W4 O23 W9 -90(10) . . . . ?
O22 W4 O23 Na10 80(8) . . . . ?
O22 W4 O30 Co2 50(4) . . . . ?
O22 W4 O17 Na1 121(4) . . . 3_656 ?
O22 W5 O29 Co2 -52(5) . . . . ?
O22 W5 O21 W6 86(10) . . . . ?
O22 W5 O21 Na9 -105(7) . . . . ?
O22 W5 O16 Na12 -169(3) . . . . ?
O22 W5 O16 Na6A 41(5) . . . . ?
O19 W7 O33 Co4 -40(3) . . . . ?
O19 W7 O33 Fe2 115(4) . . . . ?
O19 W7 O20 W6 -27(7) . . . . ?
O19 W8 O24 W9 28(9) . . . . ?
O19 W8 O24 Na8 138(6) . . . . ?
O19 W8 O32 Fe1 -118(4) . . . . ?
O19 W8 O32 Co4 44(3) . . . . ?
O19 W8 O13 Na73 -112(3) . . . . ?
O17 W4 O23 W9 124(6) . . . . ?
O17 W4 O23 Na10 -66(3) . . . . ?
O17 W4 O30 Co2 146(4) . . . . ?
O64 W13 O52 Na5A -82(4) . . . 3_656 ?
O37 W10 O45 W18 -170(3) . . . . ?
O37 W10 O45 Na3 74(3) . . . . ?
O5 W3 O1 Na5A -70(3) . . . . ?
O5 W1 O3 Na02 102(3) . . . 4_556 ?
O7 W8 O24 W9 86(3) . . . . ?
O7 W8 O24 Na8 -164(3) . . . . ?
O7 W8 O32 Fe1 -42(8) . . . . ?
O7 W8 O32 Co4 120(5) . . . . ?
O7 W8 O13 Na73 161(3) . . . . ?
O7 W3 O1 Na5A 104(3) . . . . ?
O14 W7 O33 Co4 60(4) . . . . ?
O14 W7 O33 Fe2 -145(4) . . . . ?
O14 W7 O20 W6 -178(2) . . . . ?
O45 W18 O56 W17 138(7) . . . . ?
O45 W18 O56 Na3 -30(2) . . . . ?
O45 W18 O63 Fe1 23(9) . . . . ?
O45 W18 O63 Na8 176(6) . . . . ?
O45 W18 O51 Na02 -116(5) . . . . ?
O45 W10 O37 Na1B -129(6) . . . 4_455 ?
O66 W15 O55 W16 17(5) . . . . ?
O66 W15 O48 Na4 -18(3) . . . . ?
O27 W8 O24 W9 13(3) . . . . ?
O27 W8 O24 Na8 122(3) . . . . ?
O27 W8 O32 Fe1 -32(4) . . . . ?
O27 W8 O32 Co4 130(3) . . . . ?
O27 W8 O13 Na73 126(7) . . . . ?
O27 W3 O1 Na5A 141(10) . . . . ?
O27 W9 O31 Fe1 22(4) . . . . ?
O27 Co1 O34 Co2 121(3) . . . . ?
O27 Co1 O34 Fe1 2(4) . . . . ?
O27 Co1 O34 Fe2 -118(3) . . . . ?
O27 Co1 O25 W7 64(3) . . . . ?
O27 Co1 O25 W6 -177(3) . . . . ?
O27 Co1 O25 W2 -61(3) . . . . ?
O2 W2 O4 W1 -132(6) . . . . ?
O46 W13 O52 Na5A 99(4) . . . 3_656 ?
O46 W13 O64 Co2 118(9) . . . . ?
O46 W13 O64 Fe1 -39(12) . . . . ?
O46 W10 O37 Na1B 135(6) . . . 4_455 ?
O46 W10 O45 W18 -71(3) . . . . ?
O46 W10 O45 Na3 173(3) . . . . ?
O18 W9 O31 Fe1 -149(5) . . . . ?
O13 W8 O24 W9 -179(3) . . . . ?
O13 W8 O24 Na8 -70(3) . . . . ?
O13 W8 O32 Fe1 140(3) . . . . ?
O13 W8 O32 Co4 -58(3) . . . . ?
O36 W12 O44 W17 175(3) . . . . ?
O36 W12 O44 Na3 -73(3) . . . . ?
O36 W12 O44 Na11 28(4) . . . . ?
O36 W12 O43 W16 -167(3) . . . . ?
O49 W16 O68 Co4 -142(4) . . . . ?
O49 W16 O68 Na5 28(3) . . . . ?
O6 W2 O4 W1 -30(6) . . . . ?
O6 W2 O2 Na5A -14(3) . . . . ?
O6 W3 O1 Na5A 16(3) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.55(5)
2 0.45(5)

